Multiscale Fatigue Crack Initiation and Propagation of Engineering Materials: Structural Integrity and Microstructural Worthiness
SOLID MECHANICS AND ITS APPLICATIONS Volume 152 Series Editor:
G.M.L. GLADWELL Department of Civil Engineering University of Waterloo Waterloo, Ontario, Canada N2L 3GI
Aims and Scope of the Series The fundamental questions arising in mechanics are: Why?, How?, and How much? The aim of this series is to provide lucid accounts written by authoritative researchers giving vision and insight in answering these questions on the subject of mechanics as it relates to solids. The scope of the series covers the entire spectrum of solid mechanics. Thus it includes the foundation of mechanics; variational formulations; computational mechanics; statics, kinematics and dynamics of rigid and elastic bodies: vibrations of solids and structures; dynamical systems and chaos; the theories of elasticity, plasticity and viscoelasticity; composite materials; rods, beams, shells and membranes; structural control and stability; soils, rocks and geomechanics; fracture; tribology; experimental mechanics; biomechanics and machine design. The median level of presentation is the first year graduate student. Some texts are monographs defining the current state of the field; others are accessible to final year undergraduates; but essentially the emphasis is on readability and clarity.
For a list of related mechanics titles, see final pages.
G.C. Sih Editor
Multiscale Fatigue Crack Initiation and Propagation of Engineering Materials: Structural Integrity and Microstructural Worthiness Fatigue Crack Growth Behaviour of Small and Large Bodies
G.C. Sih East China University of Science Shanghai, China and Institute of Fracture and Solid Mechanics Lehigh University Bethlehem, Pennsylvania, USA
ISBN13: 9781402085192
eISBN13: 9781402085208
Library of Congress Control Number: 2008xxxxx © 2008 Springer Science+Business Media, B.V. No part of this work may be reproduced, stored in a retrieval system, or transmitted in any form or by any means, electronic, mechanical, photocopying, microﬁlming, recording or otherwise, without written permission from the Publisher, with the exception of any material supplied speciﬁcally for the purpose of being entered and executed on a computer system, for exclusive use by the purchaser of the work. Printed on acidfree paper 987654321 springer.com
Table of Contents
Foreword
vii
Contributors
xi
Application of Virtual Testing for Obtaining Fracture Allowable of Aerospace and Aircracft Materials B. Farahmand
1
An Equivalent Block Approach to Crack Growth R. Jones, S. Pitt and D. Peng
23
Prediction of Fatigue Crack Growth Rates in Ti6Al4V Alloy A. M. Korsunsky, D. Dini and M. J. Walsh
47
Some Practical Implications of Exponential Crack Growth L. Molent, S. Barter and R. Jones
65
Fatigue Behaviour of FS, LB and MIG Welds of AA6061T6 and AA6082T6 P. M. G. P. Moreira, V. RichterTrummer and P. M. S. T. de Castro
85
Fatigue Damage from Surface to Bulk C. A. Rodopoulos
113
Microcracking in High Temperature Low Cycle Fatigue S. L. Mannan and M. Valsan
133
Invariant Form of Micro/MacroCracking in Fatigue G. C. Sih
181
Fatigue Crack Growth Rate of CableStayed Portion of Runyang Bridge: Part I – Cable Crack Growth Due to Disproportionate Cable Tightening/ Loosening and Trafﬁc Loading G. C. Sih and X. S. Tang
v
209
vi
Table of Contents
Fatigue Crack Growth Rate of CableStayed Portion of Runyang Bridge: Part II – Steel Wire Crack Growth Due to Disproportionate Cable Tightening/ Loosening and Trafﬁc Loading 249 G. C. Sih and X. S. Tang Fatigue of SmallScale Metal Materials: From Micro to NanoScale G. P. Zhang and Z. G. Wang Assessment of Fatigue Damage in Heterogeneous Materials by Application of a Novel Compliance Technique H. Mughrabi and H. W. Höppel
275
327
Fatigue Crack Growth of Aircraft Aluminum Alloys Sp. G. Pantelakis and Al. Th. Kermanidis
345
Author Index
367
Subject Index
369
Foreword
What can be added to the fracture mechanics of metal fatigue that has not already been said since the 1900s? From the view point of the material and structure engineer, there are many aspects of failure by fatigue that are in need of attention, particularly when the size and time of the working components are changed by orders of magnitude from those considered by traditional means. The 21st century marks an era of technology transition where structures are made larger and devices are made smaller, rendering the method of destructive testing unpractical. While health monitoring entered the field of science and engineering, the practitioners are discovering that the correlation between the signal and the location of interest depends on a priori knowledge of where failure may initiate. This information is not easy to find because the integrity of the physical system will change with time. Required is software that can selfadjust in time according to the monitored data. In this connection, effective application of health monitoring can use a predictive model of fatigue crack growth. Earlier fatigue crack growth models assumed functional dependence on the maximum stress and the size of the preexisting crack or defect. Various possibilities were examined in the hope that the data could be grouped such that linear interpolation would apply. The idea of associating fatigue test data with design was made when the data led to a straight line relationship with the range of mode I stress intensity factor on a loglog plot. The yintercept and slope of this line were found by curve fitting and considered to be material specific even though they also depended on specimen size. Wide acceptance of this approach was soon adopted due to the simplicity of integrating the twoparameter relation for determining the critical crack length for different specimen configuration. Moreover, the stage of slow and stable crack growth was able to be delineated from the onset of unstable and rapid crack propagation. Even at this date efforts are being made to better understood the physical meaning of the crack growth rate data outside the range of the twoparameter straight line zone referred to as region II. Region I and III are associated, respectively, with fatigue crack initiation and fast crack propagation, not to mention the two transitional zones where region II connects to regions I and III. Despite the exhaustive undertakings vii
viii
Foreword
to examine microphotographs the phenomenon of multiscale fatigue crack growth remains elusive. One of the main objectives of this book is to examine sizescale dependent microstructure evolution of fatigue damage affiliated with small specimens ranging from micrometer to nanometer. These details enhance the understanding of small scale fatigue damage mechanisms. The scale of investigation is also expanded by several orders of magnitude to include slip mismatch due to differences in grain size, orientation, microtexture, etc which arise because of the irregular propagation of short cracks. The fatigue damage map method (FDMM) was used to quantify the results which are compared with multiscale test data. In addition the effects of strain rate, temperature and hold time on the high temperature on the low cycle fatigue of austenitic and ferritic steels and Nimonic PE16 superalloy are also examined to study their microstructural changes and crack initiation and propagation behavior. Modeling crack growth rate data under simple and complex load spectra differing from the conventional approaches invoking crack closure or constraint effects are attempted. Micro to macro range of crack sizes in a variety of metals are used to correlate data on a straight line referred to a linear scale covering the regions I, II and III with two empirical parameters. A large number of problems are considered. They include the 1969 Lockheed F111 wing fatigue test; the F/A18 final test program; the round robin helicopter test program; cracking in composite patched panels; USAF C141 repair; and NASA centre notch panel tests. Analytical dual scale model is presented to describe the transitory behavior of micro/macrocracking for the fatigue of 7075T6 and 2024T3 aluminum precracked panels. Accounted for are small cracks that can close in compression and open in tension as in the case of alternating fatigue loading. Interactive effects of load, geometry and material are considered by using three independent micro/macro parameters to render the fatigue growth rate data form invariant in a loglog plot. The straight line correlation enables the connection of data referred to micro and macrocracking in fatigue. The same approach was applied to analyze the fatigue life of cables and steel wires of the Rungyang cablestayed bridge based on the design data with and without traffic. The wide variations of predicted life for the 52 cables can be problematic for the future maintenance of the bridge as some cables may need early replacement while others can still be used. Improved fatigue damage tolerance behavior of aerospace high purity 2024 aluminum alloy is discussed in connection with load sequence and spectrum effects. Of equal concern for aerospace application is thermomechanical fatigue in the presence of oxidation and creep strain
Foreword
ix
accumulation. Virtual testing methodology is explored for fatigue crack growth associated with the safelife assessment of aerospace structural components. Fatigue data of butt welded joints of aluminium alloys for 6061T6 and 6082T6 coupon specimens are found and needed to quantify the influence of three different welding techniques. They are the metal inert gas welding, laser beam welding and friction stir welding. It should be said the consideration of length alone is not enough for distinguishing micro from macrodefect since the change of defect morphology may take place during scale transition. Creation of macrofracture free surface is caused predominantly by mechanical load giving rise to symmetric or skewsymmetric geometric pattern whereas asymmetry typifies the creation of microfracture that are obstructed by the highly irregular material microstructure. Microcracks tend to wonder by curving and branching because of the inherent different constraint of the adjoining crack surface. Microphotos of fatigue striations suggest that the very tip of a microcrack always remains open on account of geometric asymmetry. This additional tip distance suggests a microstress singularity that can differ from the macrostress singularity. It so happen that a micro/macrocrack can possess a double singularity: one weak and one strong. The dual singularity gave allowance to scale transition where a microcrack can turn to a macrocrack or vice versa. This is precisely what occurs in tension/compression alternating fatigue loading. Micro and macrocracking correspond, respectively, to crack opening (tension) and closing (compression). Reference can be made to macromechanical and microstructural to accentuate the influence of scale with cause. Nanochemical would refer to imperfection size resulting from chemical reaction. The cause of fatigue can be traced to the loss of electrons from metal atoms in chemical reaction. Such a process in the presence of repeated mechanical loading even for small amplitude can greatly reduce the life of metals. The destruction can involve oxidation that increases the susceptibility of the local region to nanocrack initiation. The grain boundary is a likely location where the atoms are more loosely packed. A simple approach would be to use a mean characteristic length to describe a nano defect with the corresponding energy density weighed by a scale factor related to inhomogeneity of the atoms or the atomic lattices. The same can be done at the micro and macro scale level. When needed scale divisions can be further refined by introducing meso regions to fill the gaps from one scale range to another. Causeandeffect studies of material damage in fatigue require a sufficiently long stretch of scaling such that nano data can be brought up to the macroscopic scale. Use can be made of the overwhelming amount of micrograph data presented in this volume. They
x
Foreword
demonstrate the different fatigue crack growth details due to strain rate, temperature, loading type, material, processing technique and other factors. In this way the practitioner can benefit. Although the foregoing task is still far from being accomplished, it is essential to start focusing attention in that direction. No work on fatigue crack growth can possibly claim to be complete. The interpretation of the same data can vary as the physical models will differ. The field of fatigue damage being as important as it is to material and structure application, the entailing course of future development is inextricably linked to the social, political, economic and ideological predilection of the establishment. The limited attempt made here can only represent the views of the contributors to whom gratitude is due. Special thanks go to Ren Huifang who design the book cover and to Shen Shufang who help to format the manuscripts. Shanghai, China, 2007 G. C. Sih
Contributors
Barter S Air Vehicles Division, Defence Science and Technology Organisation, 506 Lorimer Street, Fishermans Bend 3207, Australia
[email protected] de Castro PMST Faculdade de Engenharia da Universidade do Porto Rua Dr. Roberto Frias, 200465 Porto Portugal
[email protected] Dini D Department of Mechanical Enginineering, Imperial College London South, Kensington Campus, London SW7 2AZ, UK
[email protected] Farahmand B The Boeing Company, IDS, 5301 Bolsa Ave, Huntington Beach, CA 92647, USA
[email protected] Höppel HW Department of Materials Science and Engineering, Universität ErlangenNuernberg, Martensstrasse 5, D91058 Erlangen, Germany
[email protected] Jones R Cooperative Research Centre for Integrated Engineering Asset Management (CIEAM), Department of Mechanical Engineering, Monash University, P.O. Box 31, Monash University, Victoria, 3800, Australia
[email protected] Kermanidis AlTh Department of Mechanical and Industrial Engineering, University of Thessaly, 38334 Volos, Greece
[email protected] xi
xii
Contributors
Korsunsky AK Department of Engineering Science, University of Oxford, Parks Road, Oxford OX13PJ, UK
[email protected] Mannan SL National Engineering College, Kovilpatti, TN, India
[email protected] Molent L Air Vehicles Division, Defence Science and Technology Organisation, 506 Lorimer Street, Fishermans Bend 3207, Australia
[email protected] Moreira PMGP Faculdade de Engenharia da Universidade do Porto Rua Dr. Roberto Frias, 4200465 Porto, Portugal
[email protected] Mughrabi H Department of Materials Science and Engineering, Universität ErlangenNuernberg, Martensstrasse 5, D91058 Erlangen, Germany
[email protected] Pantelakis SpG Laboratory of Technology and Strength of Materials, Department of Mechanical Engineering and Aeronautics, University of Patras, Greece
[email protected] Peng D DSTO Centre of Expertise for Structural Mechanics, Department of Mechanical Engineering, Monash University, P.O. Box 31, Monash University, Victoria, 3800, Australia
[email protected] Pitt S Air Vehicles Division, Defence Science and Technology Organisation, 506 Lorimer Street, Fishermans Bend, Victoria 3207, Australia
[email protected] RichterTrummer V Combustion Systems Engineering, RollsRoyce plc, P.O. Box 31, Derby DE24 8BJ, UK
[email protected] Contributors
xiii
Rodopoulos CA Laboratory of Technology and Strength of Materials, Department of Mechanical Engineering and Aeronautics, University of Patras, Panepistimioupolis, Patras 26500, Greece
[email protected],gr Sih GC International Center for Sustainability, Accountability and EcoAffordability of Large Structures (ICSAELS) Advanced Technology for Large Structural Systems (ATLSS), Lehigh University, Bethlehem, PA 18015, USA; and Department of Mechanical Engineering and Mechanics, Lehigh University, Bethlehem, PA 18015, USA
[email protected] Tang XS School of Bridge and Structural Engineering, Changsha University of Science and Technology, Changsha, Hunan 410076, China
[email protected] Valsan M Indira Gandhi Centre for Atomic Research, Kalpakkam, TN, India Walsh MJ Combustion Systems Engineering, RollsRoyce plc, P.O. Box 31, Derby DE24 8BJ, UK
[email protected] Wang ZG Shenyang National Laboratory for Materials Science, Institute of Metal Research, Chinese Academy of Sciences, 72 Wenhua Road, Shenyang 110016, China
[email protected] Zhang GP Shenyang National Laboratory for Materials Science, Institute of Metal Research, Chinese Academy of Sciences, 72 Wenhua Road, Shenyang 110016, China
[email protected] Application of Virtual Testing for Obtaining Fracture Allowable of Aerospace and Aircraft Materials B. Farahmand The Boeing Company, IDS 5301 Bolsa Ave, Huntington Beach, CA 92647, USA Email:
[email protected] Abstract Fracture toughness and fatigue crack growth rate data are two key parameters which are necessary for conducting safe life analysis of fracture critical parts used in space and aircraft structures. Currently, these allowables are obtained through the ASTM testing standards which are costly and time consuming. In many occasions, due to budget limitations and deadlines set forth by the customer, it is not possible to conduct fracture related tests in time. A proposed numerical approach has been developed [13] that is based on the extended Griffith theory and can predict fracture allowables for a variety of alloys. The simplicity of the concept is based on the use of basic, and in most cases available, uniaxial full stressstrain data to derive material fracture toughness values. Because the fracture toughness is thickness dependent, its value for several thicknesses can be calculated and used in the residual strength capability analysis. More importantly, its value is used to predict the region III of the fatigue crack growth rate curve. Regions I & II of the da/dN versus 'K curve can be estimated separately and will be connected to region III to establish the total fatigue crack growth rate data. As the result of this work two computer codes, fracture toughness determination (FTD) and fatigue crack growth (FCG), were generated under the NASA contract. Results of fracture toughness and fatigue crack growth rate data calculated by this approach were compared with numerous test data in the NASGRO database [4]. Excellent agreements between analyses and test data were found, which will validate the FTD and FCG methodology. This novel approach is referred to as the virtual testing technique. It enables engineers to generate fracture allowable analytically by eliminating unnecessary tests. Yet, there is another innovative approach in the virtual testing arena that relies on the multiscale modeling and simulation technique. This technique is becoming popular in the field of computational materials, where failure mechanism is defined from the bottom up approach. The methodology is based on the abinitio concept where it is assumed that the failure of material will initiate from the atomistic level, where nanocracks under the applied load will grow (as the G.C. Sih (ed.), Multiscale Fatigue Crack Initiation and Propagation of Engineering Materials: Structural Integrity and Microstructural Worthiness, 1–22. © Springer Science+Business Media B.V. 2008
2
B. Farahmand
result of poor bonding) and advance toward the micro, meso, and macro level, which thereafter will cause total structural failure. It should be noted that in most cases microscopic cracks already preexisted in the part during the machining operation, assembling parts, or rough handling. Section 6 will briefly review the application of multiscale modeling and simulation technique and its application on aerospace and aircraft parts. 1. Introduction & Background The requirements of all fracture control plans for space and aircraft structures dictate that fracture critical components must have adequate life during their service operation. The safelife assessment of these components requires information on material allowables such as: the plane stress (Kc), plane strain (KIc), partthrough fracture toughness (KIe), and the fatigue crack growth rate properties. Fracture tests under the ASTM testing standard procedures require detailed specimen preparation, prefatiguing the notch, fatigue crack growth rate measurements and interpretation of raw data, which are all costly and time consuming. Furthermore, in order for valid material property data to be produced for each casespecific material batch, a substantial number of tests will typically need to be performed. Therefore, any method that can improve and optimize this process, and reduce the number of experimental tests, will help reduce costs without compromising any safety issues. The proposed analytical technique uses fundamental fracturemechanicsbased reasoning to establish a link between plastic damage development in uniaxial stressstrain data and the material’s fracture mechanics allowables. Even though the methodology is working for a variety of aerospace alloys, further validation for a wider range of materials may be required. In this work, the concept uses steel, aluminum and titanium based alloys from a pedigree database. Furthermore, it quantifies material property sensitivity to the predictions for KIc and Kc and the subsequent estimation of 'Kth threshold and the Paris constants, C and n values. The prediction of KIc and Kc is based on the energy balance approach. It has been shown previously that material residual strength capability curve (a plot of fracture stress versus half a crack length) can be generated through the Griffith theory for an elastic media. This has been extended to account for the presence of plastic deformation at the crack tip [1, 3]. The energy absorption rate at the crack tip process zone could be assumed to have a similar mode of deformation of uniaxial specimens. Hence the material stressstrain curve of a uniaxial specimen can reflect the local energy dissipation profile within the process zone and can describe the fracture behavior of a cracked specimen as long as the stress and strain distribution and the subsequent energy balance is satisfied. Similar ideas of
Virtual Testing for Fracture of Aerospace and Aircraft Materials
3
a process zone have been previously considered at high temperatures [5] whereby creep cracking within a process zone can be described by the failure behavior of uniaxial creep test. In this proposed model, the failure range in the process zone is due to the elastic/plastic loading in a uniaxial tensile test specimen, whereas in the creep case the criteria for the damage process is a time dependant elastic/plastic/creep phenomenon. However, it has been shown that creep and plasticity can be treated in a selfsimilar manner using nonlinear fracture mechanics concepts. In a tensile case, the total energy per unit thickness absorbed in plastic straining around the crack tip, UP, can be written as the sum of two energy terms (UP = UF + UU) where UF and UU are the energy absorbed per unit thickness in plastic straining of the material beyond the ultimate at the crack tip and below the ultimate stress near the crack tip, respectively. The rate of energy absorbed at the crack tip in terms of available and consumed energy terms, UE, US, UF and UU, can be rewritten by w [UE  US  UF  UU]/wc = 0. Determining the rate at which energy is absorbed in crack tip plastic deformation (wUF/wc and wUU/wc), the residual strength capability equation for ductile material can be established. The quantity wUS/wc is the energy rate for creating two new crack surfaces. Having fracture stress and half critical crack length on hand, the critical value of the stress intensity factor (fracture toughness, Kc) can be calculated. More importantly, the variation of material fracture toughness, Kc, as a function of part thickness, can be established, which is extremely useful when conducting a safelife assessment of fracture critical components of aircraft and space hardware where parts thickness can vary significantly. Section 2 will include the detail description of the extended Griffith theory. Fracture toughness values calculated for a variety of aerospace alloys were in excellent agreement with test data which will be discussed in section 3. Moreover, this technique was further extended to predict the fatigue properties of aerospace metallic material under a cyclic loading environment. Fatigue crack growth rate tests under the ASTM E645 testing standard procedures are costly and time consuming. In the proposed technique, each region of the da/dN curve will be established separately and then connected to obtain the total fatigue crack growth rate data. It uses the predicted Kc and KIc values to derive the Paris constants, C & n. Section 4 includes a detailed explanation related to this topic. 2. Detail Description of the Extended Griffith Theory This theory assumes the fracture characteristics of a metal, local to the crack tip, are directly related to its ability to deform. Crack tip straining is assumed to be of two kinds: local strainability at the crack tip (the region of
4
B. Farahmand
highly plastic deformation) and uniform strainability near the crack tip. Thus, fracture behavior can be characterized by two energy released terms representing the absorbed energy at and near the crack tip. Both terms can be shown to be determinable from the full uniaxial stressstrain curve. The two deformation regions are illustrated in Fig. 1. The total energy per unit thickness absorbed in plastic straining of the material around the crack tip, UP, can be written as: U P = U F + UU
(1)
where UF and UU are the energy absorbed per unit thickness in plastic straining of the material beyond the ultimate at the crack tip and below the ultimate stress near the crack tip, respectively. Eq. (1) can be rewritten as: ∂[UE − UF − UU ]/∂c = 0
(2)
where wUF/wc and wUU/wc are the rates at which energy is absorbed in plastic straining beyond the ultimate stress at the crack tip and below the ultimate stress near the crack tip, respectively. To obtain a relationship between the applied stress and critical crack length, the energy absorption rates, wUF/wc and wUU/wc, for the two plastic regions formed around the crack tip must be determined. Sections 2.1 and 2.2 will discuss the derivation of wUF/wc and wUU/wc terms, respectively. Applied stress and crack length relationship will be discussed in section 2.3.
Fig. 1 The crack tip plastic zone and different region of the stressstrain curve.
Virtual Testing for Fracture of Aerospace and Aircraft Materials
5
2.1 Determination of wUF/wc term To obtain the energy absorption rate for the highly strained region at the crack tip, the extended Griffith equation in terms of its components can be rewritten as: ∂UF ∂UU πσ 2 c = 2T + + E ∂c ∂c
(3)
where 2T=wUS/wc =E̓ED is the surface tension of the material, that is, the work done in breaking the atomic bonds, D is the atomic spacing in angstroms, E is the material modulus of elasticity, and E ҏis the correction factor (3.94x1010 inch/angstrom). The quantity wUF/wc in Eq. (3), is set equal to WFhF, where WF is equal to the unrecoverable energy density (energy per unit volume) represented by the area under the plastic uniaxial engineering stressstrain curve (from the stress at which necking begins to the stress at the fracture point) for an uncracked tensile specimen. For a given alloy, the area under the stressstrain curve from the stress at which necking begins to the stress at the fracture point is a constant for a wide range of thicknesses, and therefore, the value of WF is a constant. It is assumed that essentially all of the energy represented by WF is absorbed at the crack tip in a single dominant coarse slip band. The quantity hF is the size of the highly strained portion of the small region at the crack tip as a result of WF. Its minimum value is considered to be equal to the effective o height of a coarse slip band oriented to make an angle of 45 with the plane of the crack under monotonic load. At room temperature the quantity hF = 0.00056 in. (approximately 10 micrometers). An empirical relationship based on test data [1,3] has been developed for tough metals with large necking strains that gives a higher hF value and better correlation with the test data than the value hF = 0.00056 in. It is assumed that the quantity hF is directly related to the energy per unit volume, WF, for the material in consideration, and was formulated as: hF = γ (E 2 /σU3 )WF
(4)
where J =Ҟ (8/S)Dhmin, VU is the material ultimate allowable stress, hmin=0.00056 in. and D ҏis material atomic spacing. The atomic spacing, D, for Aluminum, Titanium alloys, and Iron and Nickel are 2.86 and 2.48 Angstrom, respectively. The quantity WF in Eq. (4) is the area under the
6
B. Farahmand
stress strain curve from necking up to fracture (see Fig. 1) and is approximately equal to: WF = σ¯ U F εP N
(5)
where V UF is the neck stress and its value is taken at the centroid of the plastic energy bounded on the top by the stressstrain curve from the beginning of necking to fracture and on the bottom by a straight line from the beginning of necking to fracture. For material with a negligible amount of necking the neck stress VUF = (VUlt + VF)/2. The plastic straining, HPN, (Eq. 5) at the onset of necking is fully discussed in reference [1]. Eq. (3) in terms of hF, VUF , and HPN can be expressed as: ∂UU πσ c = 2T + hF σ¯ U F εP N + E ∂c
(6)
Fig. 2 The quantity hF is the effective height of the highly strained portion of the small region at the crack tip as a result of WF.
2.2 Determination of wUU/wc term The quantity w UU can be expressed as WUhU, where WU is the wc
unrecoverable energy density represented by the area under the plastic uniaxial stressstrain curve from the elastic limit stress, VL, to the ultimate allowable stress, VU, for an uncracked specimen. Eq. (6) becomes:
Virtual Testing for Fracture of Aerospace and Aircraft Materials πσ 2 c = 2T + hF σ¯ U F εP N + WU hU E
7
(7)
The effective height of the volume in which WU is absorbed in the uniform plastic region at the crack tip is hU. Steps taken to derive the energy rate term, w UU , for the plane stress condition are as follows: wc
x
x x
Obtain the true crack tip stresses (VTr,̓ VTT, and VTrT) in terms of applied stress and crack length in polar coordinates by using the linear elastic fracture mechanics. These stresses are responsible for material deformation at the crack tip region. Use the octahedral shear stress theory [1, 3] to correlate the biaxial tension stress with the true uniaxial tension stress, VT. Apply the crack tip uniaxial tension strain, VT, in the energy absorption rate equation, to obtain the w UU term (or WUhU). wc
The term w UU in its final form is given by: wc ∂UU n+1 εF T εT L εT U =h WU ∗ ∂c n−1 εT U εT εT U
−
−1 β
(8)
where h=0.00056 inch. The unrecoverable energy density WU is: n σT L n+1 εT P U σT U 1 − WU = n+1 σT U
(9)
2.3 Applied stress and crack length relationship Eq. (3) describing the extended Griffith theory in terms of crack length, c: c=
E [2T + WF hF + WU hU ] πσ 2
(10)
For a thin plate the value of E=1.3 describing the thickness correction for the plane stress conditions. Expressing half a crack length, c, in terms of its components, WUhU and WFhF, for wide plate becomes:
8
B. Farahmand
E σT n+1 n 2T + σ¯ U F εP N hF k + h ∗ σT U εT U 1 − c= πσ 2 µ n−1 σT U (11) εT U n−1/n εT F ε T L ∗ −1 β ∗ εT U εT εT L
where n is the strain hardening coefficient. For a finite width condition the width correction factor Y is included:
σT n+1 σT U εT U E n 2T + σ¯ U F εP N hF k + h ∗ 1− c= n−1 σT U πσ 2 µY 2 Y6 (12) εT U n−1/n εT F εT L ∗ −1 β ∗ εT U εT εT L
where Y = cos
πc −1 . Other terms in Eq. (12) are related to true stress W
and strain and are defined as:
c n
Half crack length Strain hardening coeficient
V Applied stress V T True stress V TU True stress at ultimate V UF Stress between ultimate & fracture H T True strain H PN Plastic strain at necking H TU , H TL , H TL True strain at ultimate, limit & fracture k , P , E Thickness corrections Parameters P, k and E are factors that are used to account for the thickness correction and they are applied to both sides of the components of Eq. (12) where energy is available and consumed for plastic deformation. Fig. 3 describes the shear lip formation in the planestress fracture, whereas a planestrain fracture is characterized by a flat fracture surface. It is assumed that the energies released and absorbed in planestress and
Virtual Testing for Fracture of Aerospace and Aircraft Materials
9
planestrain are in proportion to these thicknesses. Let t0 be the maximum thickness for planestress fracture. The thickness corrections k & P are applied to two strained regions at the crack tip. These quantities, thickness parameters are expressed in terms of maximum thickness for plane stress fracture, t0 (the amount of shear lip), total thickness, t, (Fig. 3) and Poisson’s ratio Q. t − t0 t0 t0 t − t0 t0 t − t0 2 + 2 ,µ= + (1 − ν ) , β = 0.13 + 0.12 k= t t t t t t
Fig. 3 The shear lip formation in the planestress fracture. The planestrain fracture is characterized by a flat fracture surface.
3. Fracture Toughness Calculation To obtain the fracture toughness value of aerospace alloys through the virtual testing approach (by applying the proposed technique), the equation of the stress intensity factor of a center crack specimen can be used, K=YVSc, where half crack length, c, can be calculated via Eq. (12). It should be noted that a full stressstrain curve for the material under investigation must be available as shown in Fig. 1. To validate the result of this technique, test data from the NASGRO material database [4] were selected and the variations of Kc versus part thickness were plotted for two aluminum alloys using the FTD software [6], Fig. 4. The effect of plate width and crack length on fracture toughness (narrow and wide plates) was compared with the data from the NASGRO database [4]. It should be noted that the NASGRO curve for a given material is not based on numerous tests at different thicknesses through which a smooth curve passes. Rather, it is based on a relationship between Kc and thickness
10
B. Farahmand
observed from multiple materials (Fig 5). This relationship is available via an empirical equation proposed by [7] as a function of KIc and material yield value, which represent the lower bound of Kc values for a given part thickness. Fig. 5 contains numerous test data which umbrellas the whole range of plate width and crack lengths, a. The estimated empirical NASGRO curve fit represents the lower bound and in some cases the typical values of Kc. The upper bound value of data shown in Fig. 5 must be associated with larger cracks and wider plates. For this reason the FTD has the option of plotting the fracture toughness versus thickness variations for plates of different width. The narrow plate represents the fracture toughness associated with small cracks where the residual strength can be as high as 75% of the material yield value. Good agreement between the physical testing and analysis can be seen when analytical data were compared with typical values of test data.
(a) 2219T87 (b) 2014T6 Fig. 4 Example of Fracture toughness versus plate thickness for two aluminum alloys compared to NASGRO data [4]).
Fig. 5 Measured Fracture Toughness versus thickness for several crack lengths of 2219T87 aluminum [1]).
Virtual Testing for Fracture of Aerospace and Aircraft Materials
11
4. Generating Fatigue Crack Growth Rate Curve without Testing 4.1 Establishing region I (fracture toughness) The testing procedure in the ASTM E647 is currently used to obtain fatigue crack growth rate data through physical testing. The proposed technique identifies the relevant parameters affecting the micromechanical behavior within a plastic process zone and relates it to plastic damage in uniaxial tensile tests. It then uses the data from the uniaxial stress/strain test to derive the materials’ fracture toughness values via the extended Griffith theory. The fracture toughness value is used to establish region III of the da/dN versus 'K curve (the accelerated region). The total curve will then be plotted by estimating the other two regions of the curve (Fig. 6). Using data derived from the analysis of a wide range of tensile data it has been established [8] that a relationship exists between Kth ('Kth for R=0) and the plane strain fracture toughness for aluminum, KIc, giving D = KIc/'Kth. 4.2 Establishing region II (Paris region) To estimate the Paris region, the two quantities Kc & Kth must be available. These two quantities will be helpful to establish two points in the Paris region. The two points in Fig. 6 (the lower and upper points of the Paris region corresponding to points 1 and 2) have unique properties which are common among many aluminum alloys. The lower point in the steady crack growth rate region, just before getting into the threshold zone of the fatigue curves (point 1 of Fig. 6), has a material independent property. That is, the ratio of the stress intensity factor, K, at the mean lower bound point and the threshold value, Kth, ('K/'Kth for R=0) is ~1.125 for the crack growth rate per cycle, da/dN ~2.54E6 mm/cycle (~1.0E7 in./cycle). In the upper region of the da/dN curve (at the end of the steady crack growth Paris region, point 2 of Fig. 6), the ratio of the upper bound stress intensity factor, K, and its critical value, Kc, ('K/Kc for R=0) is found to be ~0.9 for the da/dN ~0.127 mm/cycle (~0.005 in./cycle) from the data. These two unique points in the Paris region were found when plotting numerous fatigue crack growth rate data for aluminum as shown in Fig. 7. Therefore, by having the two quantities Kc and Kth available, the two points in the Paris region can be
12
B. Farahmand
Fig. 6 Three regions of the da/dN curve (threshold, Paris and accelerated regions).
Fig. 7 Fatigue crack growth rate curve for several aluminum alloys where the two points in the Paris region are unique.
Virtual Testing for Fracture of Aerospace and Aircraft Materials
n K n 1 − Kth p C(1 − f ) K da =
q dN K (1 − R)n 1 − (1−R)Kc
13
(13)
generated. Hence, the C and n of fatigue crack growth rate constants shown in Eq. (13) (region II) can be determined [4]. The above assumptions used for establishing the Paris region are also applicable to Titanium and Steel alloys. 4.3 Establishing region III (threshold stress intensity factor, Kth) The methodology used to estimate the threshold stress intensity factor analytically is based on studying the threshold values of more than one hundred tests from different metallic alloys and relating it to several key static and fracture allowables. The variation of Kth values for R=0 for each alloy were compared with the variation of other parameters such as material yield, Fty, final elongation, Hf, and the plane strain fracture toughness, KIc. The quantity Kth was found to be related to the material plane strain fracture toughness for aluminum alloys, where KIc.= DKth. In the latter portion of this section we will also assess the relationship between the Kth and final elongation, Hf, for aluminum, titanium and steel alloys separately. Fig. 8 shows the NASGRO value of Kth for several aluminum, titanium and steel alloys. Fig. 9 shows the plot of D=KIc/Kth for the data points shown in Fig. 8. From Figs 8 and 9 it can be seen that the NASGRO value of Kth is material dependent and has varying ranges for aluminum, titanium and steel alloys. From the experimental Kth values in Fig. 8, mean values of 'Kth=2.5 MPa¥m for Aluminum alloys, 'Kth=4 MPa¥m for the Titanium alloys and 'Kth=5 MPa¥m for steels are found. The scatter for the steels are seen to be highest because of different types of steel with wide range of tensile properties and the scatter for Aluminum is seen to be the lowest. Looking at the stressstrain curves for several aluminums, the final elongation for most aluminums fall between 8 and 12% with KIc values range from 20 to 27 MPam. This is one reason for aluminums alloys having the minimum amount of scatter as indicated in Fig. 8 when compared with the steel. The range of D for aluminums and titanium falls approximately between 714 and 916, respectively (see Fig. 9). The range of D for variety of steels is also shown in Fig. 9 and their lower and upper values are 5 and 25, respectively.
14
B. Farahmand
Fig. 8 Threshold stress intensity factor values for more than one hundred alloys.
Fig. 9 The plot of D=KIc/Kth for the data points shown in Fig. 8.
To understand the physical relationship that may exist between tensile and fracture behavior, correlations between them has been established for the different alloys. Fig. 10 shows the relationship between tensile final elongation, Hf, and Kth for the data of different alloys. Fig. 10 suggests that the tensile elongation could be an important factor in understanding the fracture properties in these alloys and improving the predictions for fatigue and fracture. Using the best fit equations shown in the Fig. 10, it would possible to get the Kth using available tensile ductility for use in the FCG code [6] to calculate da/dN data. The best fit equations for Kth give: Kt h = −0.6337 + 0.3148εf
(14)
Virtual Testing for Fracture of Aerospace and Aircraft Materials
15
Fig. 10 Best fit curve for the variation of Kth versus elongation, Hf .
Eq. (14) gives a very good indication of a linear relationship between Kth and Hf. This will allow FCG to use the estimated Kth from Eq. (14) to generate the total da/dN curve. The total predicted fatigue crack growth data, covering all the regions of the da/dN curve, can then be plotted using Eq. (13), where the fracture parameters and constants are taken from the estimated Kc, Kth, and the Paris constants C and n values. For any other range of Rratios the Newman closure equation, f, [4] can be used to establish the full fatigue crack growth rate curve when Rz0. In all cases the constants p and q of equation 13 were taken as 0.5 and 1, respectively. 5. Comparison of Predicted Bounds with Experimental Fatigue Crack Growth Data Established and then compared with fatigue crack growth test data in NASGRO database. The computer program, [6] which can run the simulations of the model, and the World Wide Web were made available in order to verify a number of test cases. The input of data can be treated as deterministic data or as probabilistic bounds of the data. Based on the abovementioned assumptions (construction of accelerated, Paris, and threshold regions), the fatigue crack growth curves for three alloys are e. The use of the statistical method gives further confidence to the methodology and is therefore crucial to any sensitivity analysis that would be needed in design and life estimation methods. In obtaining material properties data through physical or virtual testing, it is always expected some level of scatter on fracture toughness and fatigue crack growth values. The scatter is due to material variations through heat lots when the material
16
B. Farahmand
is processed. A lesser amount of variation can also be observed in test coupons that have been machined from a given plate of a given manufacturer by a specified heat lot. For comparison with test data, the upper and lower bounds for alpha, D, for each of the alloy sets were taken from Fig. 9 and compared with test data available in NASGRO. Figs. 1113 show the predicted bounds of fatigue crack growth curves for the Al, Ti and the steel family of alloys. In all cases the experimental data fall between the two limits of Hf ҏvalue. Numerous data comparisons between analyses and test data are available and are reported in [8].
Fig. 11 FCG and NASGRO da/dN curves for 6061T62 aluminum.
For life assessment analysis of structural components it will be appropriate to use the lower bound da/dN data corresponding to the upper bound D values. The upper bound values of D (lower Kth value) can provide a conservative life assessment. It may be possible to avoid unnecessary conservatism by tuning the threshold value to the material ductility, using the correlations shown by Eq. (10), in order to obtain a better agreement with the test data.
6. Fracture Mechanics & Multiscale Modeling & Simulation The virtual testing methodology discussed in the previous sections of this chapter was based on the continuum mechanics approach, where the linear
Virtual Testing for Fracture of Aerospace and Aircraft Materials
17
Fig. 12 FCG and NASGRO da/dN curves for Ti2.5 Cu Titanium.
Fig. 13 FCG and NASGRO da/dN curves for Inconel 706 Steel.
elastic fracture mechanics were used to describe the crack tip behavior. Furthermore, fracture mechanics allowables were obtained analytically through the extended Griffith theory, which can enable engineers to generate fracture related data without conducting ASTM testing. Both the fracture toughness and fatigue crack growth rate data can be generated via the FTD & FCG computer codes and can be used in life assessments of
18
B. Farahmand
fracture critical parts. It should be noted that all the assumptions used in the derivation of Kc and the da/dN data were based on large crack behavior. However, in reality the initial cracks embedded in material prior to their service usage are much smaller in length and the laws of continuum mechanics may not apply in order to assess their behavior. The largest flaw size that escapes inspection after machining parts, prior to their service usage, depends on the capability of NDI technique. If the NDI inspection shows the surface of the part is free from cracks, the analyst will use the standard NDI flaw size as the initial flaw in their damage tolerant analysis [4]. The standard NDI initial flaw size is different for different NDI method and it is related to the capability of the inspection technique. The life assessment analysis results based on this approach are too conservative and in some cases lead to redesigning the part and adding unnecessary weight into the structure. Experimental and analytical work showed that the typical flaw size found on the surface of the part after machining operation and prior to service operation is much smaller than the standard NDI flaw size, typically of the order of a few microns in dimensions. Clearly, the safelife analysis for this crack will result in a much larger number of cycletofailure when fatigue crack growth analysis is performed. To assess microscopic crack growth when subjected to a load varying environment is challenging, and the conventional linear elastic fracture mechanics based on large crack methodology is not applicable for predicting fracture allowables. The virtual testing methodology for crack growth behavior must be assessed by the multiscale modeling and simulation approach. Recently, industries are transitioning from conventional metallic alloys to super light high strength material such as the next generation of highperformance structural and multifunctional composites reinforced with nanoparticles. Weight has been and always will be the driver for aircraft and aerospace structure designs. Depending on the application, the cost savings associated with the weight reduction of structural parts is estimated to range from $100/lb to $10,000/lb. Aerospace and other industries have made significant investments in nanomaterials in an attempt to modify proven material systems to have superior mechanical/thermal/electrical properties. Successes with nanocomposite materials have been seen in limited applications across the composites sporting goods industry or with lowergrade polymers. Incorporating nanoparticles into existing material systems is proving to be more difficult that one would anticipate. Carbon nanotubes have many remarkable standalone physical characteristics such as novel electronic properties, exceptionally high axial strengths, and outstanding axial Young’s moduli (~an order of magnitude above metallic alloys). However, once incorporated into a
Virtual Testing for Fracture of Aerospace and Aircraft Materials
19
compositematerials system, these benefits, in some cases, are negated if bonding between the resin and nanotubes are weak. Proper dispersion and functionalization (establishing strong bonds between Carbon nanotubes and polymer) of nanotubes in the polymer matrix can enhance the mechanical and fracture toughness of nanocomposites. In most cases the failure initiation in nanocomposites is at the interface area, where a lack of bonds between the polymer matrix and nanotubes are weak. Fig. 14 shows the nanocrack initiation at the interface that will contribute to the material degradation and premature failure of the part when subjected to a service load.
Fig. 14 Weak interface bonds between nanotubes and polymer can be the source of damage initiation.
The multiscale modeling of resin and carbon nanotubes can be conducted through the coarsegraining technique to assess the localized regions of Fig. 14. A beadsandsprings concept will be used to represent the polymer and the nanotubes within the matrix, which can reduce the computational time and scaling considerably vs. the use of explicitly atomistic models [921]. As shown in Fig. 15, the ~200+ atoms will be replaced by a few beadsandsprings, where each bead represents several atoms of polymer and nanotubes, including the interface interactions. Nanocracks are incorporated into the modeling by allowing them to have various sizes, where their length can be as small as a few nanometers and as large as a few microns (mimicking the width and length of nanotubes). 6.1 Brief description of the coarse grain technique Multiscale modeling simulation technique will be implemented to assess the global properties of the nanocomposites through the coarse grain technique [919]. The Materials Studio of Accelrys software [19] is a powerful tool that can be used to bridge the length scale describing the interface bonds
20
B. Farahmand
Fig. 15 The coarse grain technique approach linking atomistic model to the airframe parts.
behavior between nanotubes and the resin to micro, meso and the airframe parts. The scale linking is possible via implementation of several powerful modules in the Accelrys as well as the Materials Visualizer tool for modeling the polymer of choice. A few examples of Material Studio modules are Amorphous Cell Construction, Blends, DMole, Dissipative Particle Dynamics (DPD), Discover, and Synthia. For example, the Synthia calculates polymer properties using advanced Quantitative StructureProperty Relationships (QSPRs). It allows researchers to rapidly screen candidate polymers for a wide range of properties, and allows the property prediction of copolymer blends. Or, the DPD module will help analyst to obtain the global properties of nanocomposite through the coarse grain technique by establishing super cells containing several molecules of a given polymer. 7. Conclusion The proposed analytical approach (also referred to as the virtual testing) can provide a useful tool for engineers to derive fracture toughness and fatigue crack growth data for classical metal alloys used in the aerospace industry when only a few or no test data are available. The methodology is based on continuum mechanics and basic material properties. It was shown that fracture properties can be predicted by the energy under the uniaxial tensile test via the extended Griffith theory. Two computer codes (FTD & FCG) have been developed that can estimate material fracture toughness and fatigue crack growth rate data. Excellent agreements between analytical results and test data were found for variety of alloys used in aerospace. In addition to the deterministic calculations in the program a probabilistic module has been developed to allow the user to reach a better understanding
Virtual Testing for Fracture of Aerospace and Aircraft Materials
21
of the effect of scatter on material reliability, and life prediction. It has been found that material plane strain and stress fracture toughness are sensitive to material variations observed in the full stressstrain curve. Moreover, material fatigue crack growth curve is sensitive to parameters that contribute to the threshold, Paris, and accelerated regions. The proposed method takes into account both these effects in the predictions for fracture toughness and fatigue crack growth rates. A multiscale computational modeling approach that will dramatically reduce computational time was also discussed. This approach outlines a methodology to overcome one of the primary challenges associated with hierarchical modeling of materials: namely, the accurate prediction of physical/chemical properties and behavior from the nanoscale to the macroscale without a loss of intrinsic structural information. Due to large computationalpower requirement, the computational modeling of large atomistic systems is not possible and the coarsegrain modeling technique for computational material study can be used. This technique will dramatically reduce computational complexity where computation times can be reduced by several orders of magnitude. The proposed computational method will use the coarsegrain simulation technique to bridge these length scales and to address the mechanical behavior of NanoComposite materials based fully or in part on the fundamental laws of physics (classic and quantum). This will enable the material scientist to alter key variables, via modeling, by varying parameters such as bond capability, NanoTube length, nanotube strength, and singlewalled NanoTube versus multiwalled tubes, etc. before attempting to conduct laboratory tests, which can be costly and time consuming. The impact of each the above elements on global properties can be addressed through a reliable software tool that can be applied to fully assess all the regions of the time and length scale. To remain competitive in the world market, it is imperative that the U.S. aerospace community invest in fundamental technologies and novel applications. The increased reliance on validated simulation methods linked to rapid, interdisciplinary design is a clear indicator that a Computational Materials program is required in order to take advantage of the multifunctional benefits of nanostructured materials in aerospace structures. References [1] Farahmand B. The fracture mechanics of ductile metals theory. In: Fatigue & fracture mechanics of high risk parts. Chapman & Hall, New York, (1997) 289322.
22
B. Farahmand
[2] Farahmand B. The fracture mechanics of ductile metals theory. In: Fracture mechanics of metals, composites, welds, and bolted joints. Kluwer Academic Publisher, Boston, (2000)237277. [3] Farahmand B. Predicting Fracture and fatigue crack growth properties using tensile properties. J Eng Frac Mech, 2007, Accepted for publication. [4] JSC, SRI, ESA, FAA. Fatigue crack growth computer program. NASGRO 4.0, 2000. [5] Nikbin KM, Smith DJ and Webster GA. Prediction of creep crack growth from uniaxial data. Proceedings of the Royal Society of London, 1984. [6] NASA/LaRC Contract # NAS01067. Virtual Testing. NASA Langley Research Center, Alpha STAR Corporation and Boeing Aerospace Company, 2000. [7] Vroman GA. Material thickness effect on critical stress intensity factor. Monograph #16, TRW Space and Technology Group, 1983. [8] Farahmand B, Xie D and Abdi F. Estimation of fatigue and fracture allowables for metallic materials under cyclic loading. AIAA Conference, 2007. [9] Baschnagel J, Binder K and Doruker P. Bridging the gap between atomistic and coarsegrained models of polymers. Adv. Polym. Sci., (2000) 41156. [10] Carmesin I and Kremer K. Monte Carlo and molecular dynamics simulations of polymers. Macromolecules, 21 (1988) 2819. [11] Paul W, Binder K, Kremer K, Heermann D. Dynamics of polymer solutions and melts. Reptation predictions and scaling of relaxation times. J of Chemical Phys, (1991) 77267740. [12] Baschnagel J, Binder K, Paul W, Laso, Suter UW and Batoulis I. On the construction of coarsegrained models for linear flexible polymer chains. J. Chem. Phys, (1991) 60146025. [13] Doruker P and Mattice W. A second generation of mapping/reverse mapping of coarsegrained and fully atomistic models of polymer melts Macromolecules. Institute of Polymer Science, 1997. [14] Groot, R and Warren P. Dissipative particle dynamics: Bridging the gap between atomistic and mesoscopic simulation. J. Chem. Phys., (1997) 44434435. [15] Tartakovsky A M and Meakin P. A smoothed particle hydrodynamics model for miscible flow in threedimensional fractures and the twodimensional RayleighTaylor instability. J. Comput. Phys., (2005) 610624. [16] Groot RD andRabone KL. Mesoscopic simulation of cell membrane damage, morphology change and rupture by nonionic surfactants. J. of Biophys., (2001) 725736. [17] Reith D, Meyer H and Muller F. Deriving effective mesoscale potentials from atomistic simulations. MaxPlanckInstitut fur Polymerforschung, Ackermannweg,( 2003) 16251636 . [18] Gates TS, Odegard GM, Frankland JV and Clancy TC. Multiscale modeling and simulation of nanostructured materials. Composites Science and Technology, (2005) 24162434. [19] Accelrys . Materials studio release notes, Release 4.1, Accelrys Software, Inc., San Diego, 2006.
An Equivalent Block Approach to Crack Growth R. Jones1,2*, S. Pitt3 and D. Peng2 Cooperative Research Centre for Integrated Engineering Asset Management (CIEAM), Department of Mechanical Engineering, Monash University, P.O. Box 31, Monash University, Victoria, 3800, Australia 2 DSTO Centre of Expertise for Structural Mechanics, Department of Mechanical Engineering, Monash University, P.O. Box 31, Monash University, Victoria, 3800, Australia. 3 Department of Mechanical Engineering, Monash University, P.O. Box 31, Monash University, Victoria, 3800, Australia *Email:
[email protected] 1
Abstract This work is concerned with the recent developments in the formulation and application of the generalised FrostDugdale crack growth law and illustrates how it can be used to predict crack growth, from near micron size initial flaws, under variable amplitude load spectra. 1. Introduction The problems of global warming, which led to the Koyoto agreement, and the potential depletion of oil reserves have focused attention on the need for even greater fuel efficiency. This has led Boeing to design their latest civil aircraft the B787 Dreamliner to achieve a 20% reduction in fuel. In contrast in 2006 the USAF used ~$6 billion worth of jet fuel, and as a result is now actively seeking ways to reduce its carbon footprint. In military and civil aircraft the majority of the heavy primary structural members are dominantly metallic. Thus a means for lightening these life limiting metallic parts is essential. However, all new aircraft design and structural changes made to inservice aircraft require a damage tolerance analysis, as outlined in the US Joint Services Structural Guidelines JSSG2006. The purpose of this requirement is to ensure that any cracks present in the structure will not cause loss of the structure for some predetermined period of inservice operation. Thus the challenge is to reduce weight without compromising structural integrity. This requires tools that can accurately estimate the entire fatigue crack growth history under complex variable amplitude load spectra. To meet this challenge it is necessary to have the capability to:
G.C. Sih (ed.), Multiscale Fatigue Crack Initiation and Propagation of Engineering Materials: Structural Integrity and Microstructural Worthiness, 23–45. © Springer Science+Business Media B.V. 2008
24
R. Jones et al.
(1) Rapidly and accurately assess the durability, and therefore the safety, of existing and new designs and structural modifications under both current and future operational environments; and (2) To allow a reduction in weight without compromising safety or durability. One possible approach is to use an equivalent block method whereby crack growth data either generated from the measured load spectra, or one mandated by the certifying authority, is used to develop an expression for the average crack growth per load block. The development of one such equivalent block method, which is based on the generalised FrostDugdale law [1,6], for predicting fatigue crack growth under variable amplitude loading is a focal point of this Chapter. The ability of this law to model cracks growing under constant amplitude loading was studied in [16], and its applicability to predict crack growth in both specimens and in F111 and F/A18 aircraft fullscale fatigue tests was illustrated in [1, 6]. A background to the prognosis tools discussed in this Chapter is presentedprior to assessing crack growth under variable amplitude loading. At this stage it should be mentioned that most current approaches are based on the concept of similitude. This Chapter reveals that this hypothesis is invalid in Region I. 2. Crack Growth The recent papers [16] have shown that the generalized FrostDugdale law can be applied to a wide class of engineering problems and that there is often a near linear relationship between the log of the crack size and the life, i.e. the number of cycles, or blocks. These observations are reinforced by the work presented in [7] which studied the growth of physically small cracks, which ranged in size from 20 microns to several mm’s in length, in an austeniticferritic 2205 duplex stainless steel and a range of other materials and concluded that over these length scales da/dN was proportional to the crack length and that the crack growth history could be written as per Frost & Dugdale, in the form: a = ai eYN
(1)
where Y is a load and geometry dependent parameter, and ai is the initial flaw size. A near linear relationship between ln(a) and N has also been reported, for physically small cracks, by a large number of researchers [814]. This conclusion, i.e. a near linear relationship between ln(a) and N, was also one of the primary findings reported in an early USAF/General Dy
An Equivalent Block Approach to Crack Growth
25
namics [15] study into small crack growth undertaken as part of the F16 research and development program. The observation that da/dN was often proportional to the crack length led to the conjecture [16] that in the low to mid range 'K region, i.e. in Region I and part way into Region II, the increment in the crack length per cycle (da/dN) could be described by the generalised FrostDugdale law, viz: da/dN = C c ( a/a*)(1J/2) ('N)J (da/dN)0 = C* a(1J/2) ('N)J  (da/dN)0
(2)
where 'N, is the crack driving force, C c , a*, and J are constants, C* = C c /a*(1J/2) and (da/dN)0 reflects both the fatigue threshold and the nature of the notch (defect/discontinuity) from which cracking initiates. Note that this law has da/dN dependent on both the crack driving force and the crack length. For the special case of a small crack in a large centre cracked panel under remote constant amplitude loading with R ~ 0.0 equation (2) implies that da/dN is proportional to the quantity a'VJ. This relationship agrees with that derived by Tomkins [13] who assumed that crack growth was proportional to the accumulated plastic strain, which was averaged over a characteristic length ahead of the crack length. Equation (2), which is a generalized form of the FrostDugdale law in that J is not assumed to be 3 as in [6], also resembles the fractal based crack growth law proposed in [1618], and has da/dN proportional to both 'VJ and the crack length a as per [7]. A similar equation was developed in [19] which also found that the increment in the crack length per cycle (da/dN) was a function of both the stress intensity factor K and the crack length. A similar crack growth law was also proposed in [20]. Here they considered a crack to have a series of dislocations ahead of the crack tip, which they termed a super dislocation, and that crack growth occurred as a result of the formation of microcracks ahead of the crack tip. These assumptions led to a crack growth equation of the form: da/dN = F 'V(1/O1) ('K 'Kth)2/(K2Ic'K2)
(3)
where F, and O are material constants and KIc is the plane strain Mode I fracture toughness. It should be noted that for small cracks 'K is proportional to 'V Sa so that when 'K 5
Crack length x 100 (Pm)
(a) At r0.6%
50
Modified 9Cr1Mo steel (forged bar) 3 1 Strain rate: 3x10 s Strain amplitude: +1.0%
Number of cracks
40
30
20
773 K 873 K
10
0
00.5 0.51 11.5 1.52 22.5 2.53 33.5 3.54
44.5 4.55 55.5
Crack length x 100 (Pm)
(b) At r1.0% Fig. 24 Frequency distribution of secondary cracks in Modified 9Cr1Mo steel (forged bar) .
3.3 Creepfatigueenvironment interaction  Hold time effects Hold times are introduced in a strain cycle either in tension, compression or tension plus compression peaks. This leads to creepfatigue interaction. However, in air testing oxidation effects also play a role in degrading the
Microcracking in High Temperature Low Cycle Fatigue
163
fatigue life of the material at high temperatures. Tension hold is found to be more damaging than compression hold in stainless steels namely SS 304[45], 304L[46], 316[47], 316L[48], 316L(N)[49] and Alloy D9 [50] whereas, the converse holds good for 2.25 Cr–1Mo[51, 52], IMI 829 [53], nickel base alloys [54,55] and Modified 9Cr1Mo [18, 5658]. In the following section studies conducted by the present authors to understand the hold time effects on 316L(N) SS and its welds are discussed first followed by the influence of hold time on Mod.9Cr1Mo steel. 3.3.1 316L(N) Stainless steel base metal and weld metal
The introduction of strain hold at the peak strain in tension/compression in total strain controlled testing causes stress relaxation leading to creepfatigue interaction. The creepfatigue lives of the 316L(N) base metal and 316 weld metal as a function of the length of the hold time are shown in Fig. 25. It could be seen that, at 873 K, in both continuous cycling and hold time tests, 316 weld metal showed a higher fatigue endurance compared to the base metal. It was also evident that the hold time effect on fatigue life was dependent on the position as well as the duration of hold. Compared to continuous cycling conditions, imposition of hold at peak strain was found to decrease the fatigue life. Tensile hold was observed to be more damaging than the compression hold. Further, a significant reduction in fatigue life was observed by increasing the duration of tensile hold. The greater creep fatigue life of the weld metal compared to the base metal at 873 K can be correlated to the crack propagation differences between the base metal (Fig.26(a)) and weld metal, Fig. 26(b). In base metal under 1 min. tension hold the crack initiation occurs in intergranular mode and crack propagation by mixed mode, Fig. 26(a). However in weld metal microstructural changes influences the microcrack growth (crack growth slowed down by crack deflection), Fig. 26(b). The fine duplex austeniteferrite microstructure in 316 weld metal with its many transformed phase boundaries at these testing conditions, offered a greater resistance to the extension of the fatigue cracks by causing deflection of the crack paths compared to the base metal. G ferrite got transformed to brittle V phase during testing. Crack deflection at the transformed G phase boundaries was found to increase the crack propagation resistance causing an enhanced fatigue life. At a given strain amplitude, the relaxed stress during hold time at half life for the 316L(N) base metal is provided in Table 4. In all the hold time tests, rapid stress relaxation occurred in the first few seconds of the strain hold, followed by a slower rate of stress relaxation during the rest of the hold period. During stress relaxation, conversion of elastic to plastic strain
164
S. L. Mannan and M. Valsan
took place and the strain rates were typically of the order of 104 s1 to 108 s1 during the slow relaxation period. The build up of tensile inelastic strain led to the accumulation of grain boundary creep damage in the form of cavities. With increase in the duration of the hold time a significant amount of stress relaxation took place, leading to enhanced build up of intergranular creep damage. This conforms with the magnitude of Vr developed during stress relaxation (Table 4) i.e. Vr increases with increase in the length of the hold time and is greater in tension hold compared with the compression hold. Tension hold +0.6%, base Comp. hold, +0.6%, base Tension hold, +1.0%, base Tension hold, +0.6% weld
Number of cycles to failure Nf
800
600
400
200
3
1
316L(N) SS, 873 K, 3 x 10 s 0 0
20
40
60
80
100
120
Hold time (min.) Fig. 25 Fatigue life as a function of hold time.
It must be pointed out that the absolute magnitude of the Vr alone could not be associated with the damage that determines the creepfatigue life. As a function of the strain amplitude, it was observed that Vr was relatively large at high strain amplitudes. However, the degree of reduction in life during hold time tests, defined as N/Nf (N, the fatigue life during holdtime tests and Nf the corresponding fatigue life in continuous cycling) was found to be larger at lower strain amplitudes, compared to higher strain amplitudes of testing (Table 4). The strain rates during relaxation at higher strain amplitudes were generally higher than those observed at low strain amplitudes of testing. In general, the relaxation strain rates of magnitude >
Microcracking in High Temperature Low Cycle Fatigue
165
104 s1 observed at high strain amplitudes are typically expected to cause matrix deformation, while those observed at low strain amplitudes namely, < 104 s1, corresponded to that of creep deformation. It has been suggested that relaxation strain rates < 104 s1 generally contribute to grain boundary damage and cause a greater reduction in life [59, 60].
(a) Mixed mode crack growth in 1 min. tension hold, 316L(N) base metal
(b) Crack growth in 316 weld metal, 1 min. T hold and +0.6% Fig. 26 Crack morphology at 873 K.
166
S. L. Mannan and M. Valsan Table 4 Effects of hold time on LCF properties at 873 K. Hold 'Ht/2 'V/2 V r N N/Nf (min) (%) (MPa) (MPa) (Cycles) 0 ±0.6 328 580(Nf) 1 1t
,,
307
51
475
0.819
1c
,,
323
45
510
0.879
10t
,,
291
57
409
0.705
30t
,,
288
74
330
0.635
90t
,,
274
94
235
0.405
0
±1.0 370

130(Nf) 1
10t
,,
342
68
140
1.08
30t
,,
322
96
110
0.846
where, t : Tensile hold ; c : Compression hold; 'Ht/2 : Total strain amplitude 'V/2 : HalfLife stress amplitude N : Number of cycles to failure (with hold) Nf : Number of cycles to failure (without hold) V r : Relaxed stress during hold
The grain boundary damage developed during relaxation changes the modes of crack initiation and propagation. In 1 min. compression hold, the crack initiation and propagation occurs by transgranular mode (Fig.27(a)) similar to continuous cycling conditions, Fig. 27(b). However, under tension hold conditions crack initiation becomes intergranular and propagation is mixed mode (trans + intergranular), Fig. 26(a). It is seen that the surfaceconnected slip bands are oxidized under 10 min. tension hold conditions, Fig. 28(a) and the fracture surface is marked periodically by fatigue striations and intergranular cracks , Fig. 28(b). Oxidation interaction is found to be more as the length of the hold time is increased to 90 minutes (Fig. 29(a)). Both crack initiation and propagation seem to be strongly assisted by oxidation and fracture surface is completely covered by a thick oxide layer, Fig. 29(b).
Microcracking in High Temperature Low Cycle Fatigue
(a) Within 1 min. compression hold for 316L(N) base metal
(b)Include crack initiation at 873 K:continuous cycling at strain amplitude r0.6% Fig. 27 Microstructure for transgranular crack propagation.
167
168
S. L. Mannan and M. Valsan
(a) Oxidation assisted crack initiation from slip bands
(b) Mixed mode crack propagation assisted by oxidation Fig. 28 Microsdtructure for 316L(N) SS with 10 minutes tension hold at 873 K.
(a) Oxide location A
Microcracking in High Temperature Low Cycle Fatigue
169
(b) Oxide location B Fig. 29 Oxidation induced Intergranular Cracking in 90 min. Tension Dwell Tests, 316L(N) Base Metal, strain amplitude r0.6%.
The influence of the predominant fracture mode on fatigue can be assessed from a quantitative measurement of crack density i.e. cumulative length of the trans and intergranular secondary cracks on the longitudinal section per unit area, as shown in Fig. 30(a) along with the frequency distribution of the crack length, Fig. 30(b). It was seen that intergranular crack density was the lowest in compression hold test, and crack propagation was mainly transgranular. This behaviour could be attributed to the following reasons. During stress relaxation in compression hold, the growth of internal grain boundary cavities was very unlikely, since this needed both shear and normal tensile stresses across the grain boundary. Thus for cycles containing compression hold periods, failure was dominated by transgranular crack initiation and growth mechanisms and fatigue lives were longer, compared with tensile hold periods. However, bulk creep damage was favoured under tension hold conditions. Crack density measurements on this steel, Fig.30(a) indicated that the transgranular crack density decreased with an increase in the length of the holdtime in tension and crack propagation was mainly intergranular. Moreover, it was noted that crack linkage becomes extensive as the length of the hold time increased and long intergranular cracks were observed in 10 and 90 minutes tensionhold tests, Fig. 30(b). Thus the reduced fatigue life for longer holdtimes could be ascribed to the occurrence of enhanced creep and oxidation damage at grain boundaries that facilitates accelerated intergranular crack initiation and propagation.
S. L. Mannan and M. Valsan
350
316L(N), 873 K, +0.6% 1 Min. compression 90 Min. tension 10 Min. tension 1 Min. tension
2
Crack density (Pm/mm )
300 250 200 150 100 50 0
Intergranular Transgranular (a) Crack Density 316L(N), 873 K, +0.6% 1 Min. compression 90 Min. tension 10 Min. tension 1 Min. tension
14 12
Number of cracks
170
10 8 6 4 2 0
8
Crack length x 100 (Pm) (b) Crack Length Fig. 30 Crack distribution as a function of hold time with 873 K at r0.6%.
Microcracking in High Temperature Low Cycle Fatigue
171
3.3.2 Modified 9Cr1Mo steel
The influence of tensile and compressive hold times on LCF behaviour of modified 9Cr1Mo steel was investigated at 873 K at a strain amplitude of r0.6%. The variation of fatigue life with the duration of tensile hold time up to 30min on Mod.9Cr1Mo steel (forged condition) at 873 K is shown in Fig. 31 and a comparison of the effect of tensile, compressive and tensile plus compressive hold time on fatigue life at 873 K of Modified 9Cr1Mo material (extruded tube) is shown in Fig. 32. It was seen that the fatigue life decreased with increase in the length of hold time up to 30 min. Dwell in compression was found to be more deleterious than dwell in tension and tensionpluscompression dwell was found to be the most detrimental. Enhanced dwell sensitivity in compression has also been reported in this alloy by other investigators [56,57]. Further, it has been reported that tension hold is more damaging than compression hold in vacuum testing whereas the converse to be true for air testing [58]. Large tensile dwell sensitivity is essentially observed in materials exhibiting creep cavitation [4550]. However, enhanced compressive dwell sensitivity, can be attributed to one of the following reasons, namely, development of tensile mean stress, shape and size of cavities and oxidation behaviour. The greater vulnerability of 2.25Cr1Mo steel to compression hold has been interpreted in terms of the behaviour of oxides [61]. It was shown that in compression after a tensile hold, the oxide spalls, thus revealing a 950
Modified 9Cr1Mo Steel Temperature 873 K 3 1 Strain Rate: 3 x 10 s Strain Amplitude: +0.6%
Number of cycles to failure Nf
900 850 800 750 700 650 600 550 500 450 0
5
10
15
20
25
30
35
Hold time (min.)
Fig. 31 Influence of hold time on fatigue life at 873 K.
172
S. L. Mannan and M. Valsan
Number of cycles to failure Nf
500
Modified 9Cr1Mo Steel Temperature 873 K 3 1 Strain Rate: 3 x 10 s Strain Amplitude: +0.6%
450
400
350
300
250
Tension Hold Compression Hold Tension + Compression Hold
200
150 0
5
10
Hold time (min.)
Fig. 32 Fatigue life as a function of hold time, Mod. 9Cr1Mo steel (extruded tube), 873 K.
(a)Through
(b) 1minute tension hold
(c) 10 minutes tension hold (d) 1 minute compression hold, 873 K, + 0.6%, Modified 9Cr1Mo steel (extruded tube) Fig. 33 Fractograph showing slip band cracking under continuous cycling.
Microcracking in High Temperature Low Cycle Fatigue
173
fresh surface, enabling the removal of surface damage. Conversely, in tension after a compression hold, the oxide film cracks facilitating early crack nucleation in the underlying material. This behaviour was related to the tensile strain in the oxide [62]. In Modified 9Cr1Mo steel no appreciable tensile mean stress in compression hold has been noticed. Further, creep cavitation was also not observed during hold time experiments. Fractographs of the fatigue tested samples under continuous cycling, 1 min tension, 10 min tension and 1 min compression shown in Fig. 33(a) through (d) respectively showed clearly transgranular crack initiation from surface connected slip bands and transgranular crack propagation marked by fatigue striations. This clearly negates the role of intergranular cavities in degrading the fatigue life of this material under hold time conditions. Detailed metallography conducted on longitudinal sections of the fatigue tested samples (under 1 min tension, 10 min tension and 1 min compression depicted in Figs. 34 (a) through (c ) respectively) showed multiple crack initiation sites and oxidation assisted crack initiation and propagation. Also the number density of secondary cracks was more in the case of compression hold compared to tension hold. This clearly indicated that the larger compression dwell sensitivity in Modified 9Cr1Mo ferritic steel essentially arises from the oxidation effects. However, unlike 2.25Cr1Mo steel no oxide spallation was noticed in this steel during tension hold. It is conceived that in modified 9Cr1Mo steel an oxide layer formed on the surface of the specimen cracks which on further oxidation during tension hold leads to crack tip blunting, while during compression hold they stay sharp [56]. Moreover, it has also been proposed that the wedge effect of the exfoliated oxide cause oxidationassisted cracking in Modified 9Cr1Mo steel. Further, the oxide layer formed on the surface of the specimen was a weak barrier that could be easily overcome by slip and several crack initiation sites were observed in airtested specimen compared to that in vacuum [63]. The reduced life in this steel, under creepfatigue interaction conditions has thus been attributed to oxidation assisted crack initiation and propagation. 4. Concluding Remarks Discussed are a few aspects of how microstructure, both initial and that developed subsequently during LCF deformation influence the formation and propagation of microcracks which eventually determine fatigue life, from examples of authors’ work on materials of interest to fast breeder reactor technology. In Nimonic PE16 shearing of J' precipitates leads to cyclic softening. Shearing of precipitates under heterogeneous distribution
174
S. L. Mannan and M. Valsan
(a) 1 minute tension hold
(b) 10 minutes tension hold
(c) 1 minute compression hold, modified 9Cr1Mo steel (extruded tube), 873 K, +0.6%. Fig. 34 Optical Metallograph of longitudinal section of fatigue tested samples depicting secondary cracks.
can lead to localization of strain resulting in enhanced transgranular and intergranular cracking and a reduced fatigue life. Intergranular fracture is
Microcracking in High Temperature Low Cycle Fatigue
175
accentuated by the presence of carbide precipitates on the grain boundaries. Dynamic strain ageing is found to influence fatigue deformation and fracture at high temperatures and low strain rates conducive to dislocation solute atom interaction. DSA leads to enhanced localization of slip leading to inhomogeneity of deformation and accelerated intergranular and transgranular cracking. This caused a reduction in life. In austenitic stainless steel base metal and weld metal fatigue life decreased with the introduction of hold. Tension hold was found to be more deleterious than compression hold. Further, fatigue life decreased with increase in the length of the hold time. Creep and oxidation contributed to reduction in fatigue life with hold time. In situations where crack deflection associated with the G ferrite transformation occurred, 316 weld metal showed a higher fatigue life compared to the base metal. In Modified 9Cr1Mo ferritic steel compression hold was found to be more deleterious than tension hold. It is suggested that the thin oxide layer formed on the surface is cracked by slip processes in this steel. Further, crack tip blunting by oxidation during tension hold reduces the crack propagation rate, whereas in compression hold the crack remains sharp leading to enhanced crack propagation rate. Understanding of mechanism of microcracking in different alloy systems under a variety of test conditions is important for the development of microstructures resistant to fatigue cracking under specific test conditions. Further considering the fact that many approaches are available for life prediction at elevated temperatures, understanding of the mechanisms of deformation and damage would lead to realistic life assessment and prediction techniques. References [1] Coffin LF. Effect of frequency and environment on fatigue crack growth of A286 at 1100 F. In: Carden AE, Mc Evily AJ, Wells CH (eds) Fatigue at elevated temperatures. STP 520, ASTM, Philadelphia, PA, (1973) 112122. [2] Gell M and Leverant GR. Mechanism of high temperature fatigue. In: Carden AE, Mc Evily AJ, Wells CH (eds) Fatigue at elevated temperatures. STP 520, ASTM, Philadelphia, PA, (1973,) 3767. [3] Antolovich SD, Liu S and Baur R. Low cycle fatigue behaviour of Rene 80 at elevated temperature. Metall Trans A, 12 (1981) 473481. [4] Valsan M, Parameswaran P, Bhanu Sankara Rao K, Vijayalakshmi M, Mannan SL and Sastry DH. Hightemperature low cycle fatigue behaviour of a Nimonic PE16 superalloy  correlation with deformation and fracture. Metall Trans A, 23 (1992) 17511761. [5] Mannan SL, Valsan M High temperature low cycle fatigue, creepfatigue and thermomechanical fatigue of steels and their welds. Int J Mechanical Sciences 48 (2006) 160175.
176
S. L. Mannan and M. Valsan
[6] Sidey D and Coffin LF Jr. Low cycle fatigue damage mechanisms at high temperature. In: Fong JT (ed) Symp. on fatigue mechanisms. ASTM STP, 675 (1979) 528570. [7] Wells CH, Sullivan CP and Gell M. Mechanism of fatigue in creep range, In: Manson SS (ed) Metal fatigue damage: mechanism, detection, avoidance and repair. ASTM STP, 495 (1971) 61122. [8] Bhanu Sankara Rao K. Time dependent low cycle fatigue behaviour of high temperature alloys. Trans Indian Inst Met, 42 (1989) 6182. [9] Mannan SL. Role of dynamic strain ageing in low cycle fatigue. Bull of Mater Sci, 16(6) (1993) 561582. [10] Valsan M, Sastry DH, Bhanu Sankara Rao K and Mannan SL. Effect of strain rate on hightemperature lowcycle fatigue properties of a Nimonic PE16 superalloy. Metall Trans A, 25 (1994) 159171. [11] Valsan M, Sundararaman D, Ray SK and Mannan SL. Low cycle fatigue deformation behaviour of a Nimonic PE16 superalloy in a doubleaged microstructural condition. Trans Indian Inst Met, 49(4) (1996) 471477. [12] Srinivasan VS, Sandhya R, Bhanu Sankara Rao K, Mannan SL and Raghavan KS. Effects of temperature on the low cycle fatigue behaviour of nitrogen alloyed type 316L stainless steel. Int J of Fatigue, 13(6) (1991) 471478. [13] Valsan M, Sundararaman D, Bhanu Sankara Rao K and Mannan SL. A comparative evaluation of low cycle fatigue behaviour of type 316L(N) base metal, 316 weld metal and 316L(N)/316 weld joint. Metall and Mater Transactions A, 26 (1995) 12071219. [14] Nagesha A, Valsan M, Bhanu Sankara Rao K and Mannan SL. Strain controlled fatigue of type 316L(N) base metal and 316 SS weld metal at elevated temperatures. In: XueRen Wu, Wang ZG (eds) Proceedings of the seventh International fatigue conference, FATIGUE ’99,2. Beijing, China, (1999) 13031308. [15] Srinivasan VS, Valsan M, Sandhya R, Bhanu Sankara Rao K, Mannan SL and Sastry DH. High temperature timedependent low cycle fatigue behaviour of a type 316L(N) stainless steel. Int J of Fatigue, 21 (1999) 1121. [16] Nagesha A, Valsan M, Kannan R, Bhanu Sankara Rao K and Mannan SL. Influence of temperature on the low cycle fatigue behaviour of a modified 9Cr1Mo ferritic steel. Int J of Fatigue, 24(12) (2002) 12851293. [17] Mannan SL, Bhanu Sankara Rao K, Valsan M and Nagesha A. Strain controlled low cycle fatigue and creepfatigue interaction behaviour of Modified 9Cr1Mo ferritic steel. Trans Indian Inst Met, 58(23) (2005) 159168. [18] Vani Shankar, Valsan M, Kannan R, Bhanu Sankara Rao K, Mannan SL and Pathak SD. Low cycle fatigue behavior and microstructural evolution of 9Cr1MoVNb ferritic steel. Mat Sci and Engg, 437(2) (2006) 413422. [19] Srinivasan VS, Valsan M, Bhanu Sankara Rao K, Mannan SL and Raj B. Low cycle fatigue and creepfatigue interaction behaviour of 316L(N) stainless steel and life prediction by artificial neural network approach. Int J of Fatigue, 25 (2003) 13271338. [20] Srinivasan VS, Sandhya R, Valsan M, Bhanu Sankara Rao K and Mannan SL. Comparative evaluation of strain controlled low cycle fatigue behaviour
Microcracking in High Temperature Low Cycle Fatigue
[21]
[22]
[23] [24]
[25]
[26]
[27]
[28] [29] [30]
[31]
[32]
[33]
[34] [35]
177
of solution annealed and prior cold worked 316L(N) stainless steel. Int J of Fatigue, 26 (2004) 12951302. Coffin LF Jr. Fatigue at high temperature. In: Carden AE, Mc Evily AJ, Wells CH (eds) Fatigue at elevated temperatures. ASTM STP, 520 (1973) 134. Brinkman CR, Gieseke BG and Maziasz PJ. The influence of long term thermal ageing on the microstructure and mechanical properties of modified 9Cr1Mo steel. In: Liaw PK, Viswanathan R, Murty KL, Simonen EP, Frear D (eds) Microstructure and mechanical properties of ageing material. The Minerals, Metals and Materials Society, (1993), 107115. White RJ and Fisher SB. The precipitation and growth kinetics of Jc in Nimonic PE16. Mat Sci and Engg, 33 (1978) 149157. Seetharaman V, Bhanu Sankara Rao K, Mannan SL and Rodriguez P. Microstructure and mechanical properties of a Nimonic PE16 superalloy subjected to double ageing treatment. Mat Sci and Engg, 63 (1984) 3550. Taillard R, Degallaix S and Foct J. Effect of nitrogen upon the low cycle fatigue behaviour of 316L stainless steels. In: Rie KT (ed) Low cycle fatigue and elastoplastic behaviour of materials. Elsevier, Munich, (1987) 8388. Sandstrom R, Engstrom J, Nilsson JO and Nordgren A. Elevated temperature low cycle fatigue of the austenitic stainless steel type 316 and 253 MA – influence of microstructure and damage mechanisms. High Temp Technol, 7 (1989) 29. Nilsson JO. The influence of nitrogen on high temperature low cycle fatigue behaviour of austenitic stainless steel. Fat Fract Engg Mater Struct 7, (1984) 5564. Vogt B, Degallaix S and Foct J. Low cycle fatigue life enhancement of 316L stainless steel by nitrogen alloying. Int J Fatigue, 6(4) (1984) 211215. Nilsson JO. The effect of slip behaviour on the low cycle fatigue behaviour of two austenitic stainless steels. Scripta Metall, 17 (1983) 593596. Taillard R and Foct J. Mechanisms of the action of nitrogen interstitials upon low cycle fatigue behaviour of 316 stainless steels. In: Foct J, Hendry A (eds) Proc Int conf on high nitrogen steels 88. The Institute of Metals and the Socitie francaise de Metallurgie , Lillie, France, (1988) 387391. Nilsson JO and Thorvaldsson T. The influence of nitrogen on microstructure and strength of a highalloy austenitic stainless steel. Scand J Metall, 15 (1985,) 8389. Stoltz RE and Pineau AG. Dislocationprecipitate interaction and cyclic stressstrain behaviour of a J' strengthened superalloy. Mater Sci Eng, 34 (1978) 275284. Calabrese C and Laird C. Cyclic stressstrain response of two phase alloys part I. Microstructure containing particles penetrable by dislocations. Mater Sci Engg, 13 (1974) 141157. Lerch A and Gerold V. Cyclic hardening mechanisms in Nimonic 80A. Metall Trans A, 18 (1987) 21352141. Kim WH and Laird C. Crack nucleation and stage I propagation in high strain fatigue – II mechanism. Acta Metall, 26 (1978) 789799.
178
S. L. Mannan and M. Valsan
[36] Hornbogen E and Zum Gahr KH. Microstructure and fatigue crack growth in a J FeNiAl alloy. Acta Metall, 24 (1976) 581592. [37] Arbuthnot CHD. The Micromechanisms of fatigue deformation in Nimonic PE16. In: Maurer KL, Matzer FE (eds) Proc 4th european conf on fracture and role of microstructure 2. Leoben, Austria, The Chameleon press Ltd., London, United Kingdom, (1982) 407413. [38] Mediratta SR, Ramaswamy V and Rama Rao P. Two stage cyclic work hardening and twoslope CoffinManson relationship in dual phase steels. Scripta Metall, 20 (1986) 555558. [39] Sanders TH Jr and Starke EA Jr. The relationship of microstructure to monotonic and cyclic straining of two age hardening aluminum alloys. Metall Trans, 7A (1976) 14071418. [40] Bhanu Sankara Rao K, Valsan M, Sandhya R, Mannan SL and Rodriguez P. Synergistic interactions during high temperature fatigue of type 304 stainless steelgrain size dependence. Trans Indian Institute of Metals, 44(3) (1991) 255270. [41] Bhanu Sankara Rao K, Valsan M, Sandhya R, Mannan SL and Rodriguez P. Grain size dependence of dynamic strain ageing during low cycle fatigue of type 304 stainless steel. In: Salama K, Ravi Chandar K, Taplin DMR, Rama Rao P (eds) ICF7, Advances in fracture research 2, Pergamon, Oxford, (1989) 13231330. [42] Kanazawa K, Yamaguchi K and Nishijima S. Mapping of low cycle fatigue mechanisms at elevated temperatures for an austenitic stainless steel. In: Solomon HD, Halford GR, Kaisand LR, Leis BN (eds) Low cycle fatigue. ASTM STP 942, Philadelphia, (1988) 519530. [43] AbdelRaouf H, Plumtree A and Topper TH. Effect of temperature and deformation rate on cyclic strength and fracture of low carbon steel. In: Coffin LF, Krempl E (eds) Cyclic stressstrain behaviour analysis, experimentation and failure prediction. ASTM STP, 519 (1971) 2857. [44] Bressers J. Fatigue and microstructure. In: Marriott JB, Merz M, Nihoul J, Ward J (eds) High temperature alloys, their exploitable potential. Elsevier Applied Science, Amsterdam, (1987) 385410. [45] Lee SB and Miller AK. A phenomenological model for intergranular fatigue by rtype and wedge type cavitation. J Engg Mater Tech, 117 (1995) 311321. [46] Halford GR, Johnson JR and Brown JA. In: Richmond RJ, Wu ST (eds) Advanced earth – to – orbit propulsion technology. NASA Conf publications, (1986) 24372450. [47] Yamaguchi K and Kanazawa K. Effect of strain wave shape on high temperature fatigue of type 316 steel and application of strain range partitioning method. Metall Trans, 11A (1980) 20192027. [48] Shi HJ and Pluvinage G. Cyclic stress strain response during isothermal and thermomechanical fatigue. Int J Fatigue, 16 (9) (1994) 549557. [49] Srinivasan VS, Nagesha A, Valsan M, Bhanu Sankara Rao K, Mannan SL and Sastry DH. Effect of hold time on low cycle fatigue behaviour of nitro
Microcracking in High Temperature Low Cycle Fatigue
[50]
[51]
[52]
[53] [54] [55] [56]
[57]
[58]
[59]
[60]
[61]
[62]
[63]
179
gen bearing 316L stainless steel. Int J of Pressure Vessels and Piping, 76 (1999)863870. Sandhya R, Bhanu Sankara Rao K and Mannan SL. Creep fatigue interaction behaviour of a 15Cr15Ni Ti Modified austenitic stainless steel as a function of Ti/C ratio and microstructure. Mat Sci and Engg A, 392 (2005) 326334. Brinkman CR, Strizak JP, Brooker MK and Jaske CEJ. Time dependant strain controlled fatigue behaviour of annealed 2.25Cr1Mo steel for use in nuclear steam generator design. J Nucl Mater, 62 (2/3) (1976) 181204. Goswami T. Creepfatigue: Paper 1. Compilation of data and trends in the creep fatigue behaviour of low alloy steels. High Temp Mater Proc, 14(1) (1995) 119. Plumbridge WJ and Stanley M. Low cycle fatigue of a Titanium 829 alloy. Int J Fatigue, 8 (1986) 209216. Plumbridge WJ and Ellison EG. Low cycle fatigue behaviour of superalloy blade materials at high temperatures. Mater Sci Tech, 3 (1987) 706715. Nazmy MY. High temperature low cycle fatigue of Inconel 783 and application of strain range partitioning. Metall Trans, 14A (1983) 449461. Aoto K, Komine R, Ueno F, Kawasaki H and Wada Y. Creepfatigue evaluation of normalized and tempered modified 9Cr1Mo. Nucl Engg Design, 153 (1994) 97110. Van Den Avyle JA and Jones WB. Substructure and strengthening mechanisms in 2.25Cr1Mo steel at elevated temperatures. Metall Trans, 11A (1980) 12751286. Kim S and Weertman JR. Investigations of microstructural changes in a ferritc steel caused by high temperature fatigue. Metall Trans A, 19 (1988) 9991007. Bhanu Sankara Rao K, Meurer HP and Schuster H. Creepfatigue interaction of Inconel 617 at 950 qC in simulated nuclear helium. Mat Sci and Engg, 104A (1988) 3751. Rie KT, Schmidt RM, Ilschner B and Sam SW. A model for predicting low cycle fatigue life under creepfatigue interaction. In: Solomon HD, Halford GR, Kaisand LR, Leis BN (eds) Low cycle fatigue. ASTM STP 942, Philadelphia, (1988) 313328. Teranishi H and McEvily AJ. On the fatigue crack initiation and propagation at elevated temperatures. In: Francois O (ed) ICF 5, Advances in Fracture Research, Pergamon Press, Paris, (1980) 24392445. Challenger KD. Elevated temperature fatigue of 2.25Cr1Mo steel. In: Valluri SR, Taplin DMR, Rama Rao P, Knott JF, Dubey R (eds) ICF6, New Delhi, India, (1984) 22392248. Ebe G and McEvily AJ. Effect of processing in high temperature low cycle fatigue properties of modified 9Cr1Mo steel. Fatigue and Fracture Engg Mat Struct, 17 (1984) 299314.
Invariant Form of Micro/MacroCracking in Fatigue G. C. Sih 1, 2 * International Center for Sustainability, Accountability and EcoAffordability of Large Structures (ICSAELS) Advanced Technology for Large Structural Systems (ATLSS) Lehigh University, Bethlehem, PA 18015, USA 2 School of Mechanical and Power Engineering, East China University if Science and Technology, Shanghai 200237, China *Email:
[email protected],
[email protected] 1
Abstract The size/time transitory character of fatigue cracking can be hidden in the data or revealed explicitly depending on the manner of presentation. The former can correspond to the crack length while the latter to the crack growth rate variations, both referred to the number of fatigue cycles. Conventionally speaking, the sigmoidal curve for the plot of log da/dN against log 'K consists of three regions known as I, II and III. They are referred to, respectively, as crack initiation, stable crack growth and fast fracture although the transition from one region to another involving scale shifting is seldom discussed. Even though damage by very small defects are recognized in fatigue but their representation may become dubious when the parameter “a” in the crack growth rate expression da/dN may have to adopt a different physical interpretation. Using the line crack configuration for describing crack growth in metals, reference will be made to three approximate crack size range of a 1080 mm (macromechanical) for regions II and III, a 103 to 101mm (micro structural) for region I and presumably a 104 mm or smaller (nano chemical) for the lower scale regions. The objective of developing a multiscale fatigue crack growth model is to determine the increment of a stress intensity or energy density parameter such that the data in regions I, II and III can be related. One way is to have the crack growth rate da/dN to lie on a straight line such that linear interpolation can be applied to relate the nano, micro and macro fatigue data. This behavior is referred to as forminvariant. The proposed scheme accounts for two succeeding scales such as micro/macro and nano/micro. In this way. the scaling shifting capability can be extended, say from nano to macro. The dual scale micro/macro line crack model will be presented. It consists of three physical parameters d* (micro/macro length), P* G.C. Sih (ed.), Multiscale Fatigue Crack Initiation and Propagation of Engineering Materials: Structural Integrity and Microstructural Worthiness, 181–208. © Springer Science+Business Media B.V. 2008
182
G. C. Sih
(micro/macro material constants) and V* (external/internal stresses). The model can also delve into the details of the material microstructure when needed. For structural applications many of the incidental material parameters can be absorbed by the macro empirical parameters which will be limited to two such that the present findings can be incorporated into the current fracture control methodology. Using the available fatigue crack growth data for the 7075T6 and 2024T3 aluminum panels, the sigmoidallycurved regions I, II and III will be shown to become a straight line whose slope and yintercept in a loglog plot will depend on the mean stress Vm and stress amplitude Va that are accounted for simultaneously by the dual scale energy density expression. The slopes of lines line referred to the energy density plots ranged from 2.890 to 3.019 when Vm varied from 9 to 12 kg/mm2 and Va from 2.5 to 6.5 kg/mm2. The slopes obtained a wider scatter of 3.532 to 4.224 when the energy density range was replaced by the stress intensity range. This was expected because the stress intensity approach leaves out the mean stress effect. The present work is offered as the first step to include scaling effects so that micro material behavior can enter into the macro fatigue crack growth process. 1. Introduction The macro mechanical properties are known to be affected by the material microstructure which can be changed by heat treatment and/or high pressure. Various processing techniques have been developed and applied to alter the strength of uniaxial specimens. The results presumably can be extended to the design of structural members under multiaxial stress states. As the test data scatter increased with increasing material strength, it was found necessary to account for the effect of preexisting defects. The classical notion of plane stress for thin bodies and plane strain for thick sections were realized to be inadequate as they entail only global scale dimensions. The size of failure initiation locality relative to global instability is fundamental. This has led to crack initiation and propagation as the two events considered in the facture mechanics discipline [13]. Scale segmentation was also necessary such that analyses can be divided into different ranges referred to as nanoscopic, microscopic and macroscopic. The interconnecting gap has been known as the mesoscopic [4,5] region. These distinctions were necessary to avoid considering the process of nonequilibrium [6,7] where the material properties changed not only from location to location but also in elapsed time. By tradition, the open thermodynamic system has been simplified to a closed system where
Invariant Form of Micro/MacroCracking in Fatigue
183
the conditions on the boundary are assumed to be known and hence specified. The fluctuations or movements at the interface are assumed to be localized for large bodies and ignored. As the body size is decreased, the average and bulk properties are no longer representative of the physical behavior. At the nano scale, the physical laws can differ [8,9] and the description of matter can adopt an uncertain character as advocated in quantum mechanics where the origin of failure may initiate from the nonuniform distribution of the electrons [10]. Advancement in micro/macro crack interaction in fatigue has been crawling at the a snail’s pace because not enough attention has been directed to understand the mechanism of crack opening followed by closing in the same cycle repeated many times. Most of the data are collected for metals undergoing low amplitude loads alternating at onehalf of the yield strength according to the ASTM standard. This corresponds to the situation where the elements ahead of a macroscopic crack would undergo permanent deformation such that the local hyteresis loops would be measurable. The cracked material at the microscale has sufficient restraint to close upon unloading, A restraining force or stress is said to prevail that changes with the crack length. This mechanism is believed to be fundamental in describing the transitory character of micro/macrocracking that correspond to regions I and II of the conventional sigmoidal fatigue crack growth rate curve. The dual scale crack model [11,12] provided the impetus for developing a fatigue crack model that can switch from a microcrack to a macrocrack and vice versa. Such a crack prevails in a nonhomogeneous medium where the top and bottom surface of the crack would subject to different constraint that can be modeled by the freefixed boundary condition. That is the crack path would in general wonder about without symmetry. This led to the discovery of a crack with double stress singularity [13]. The weak singularity of order 1/r0.25 can model the microcrack behavior and the strong singularity of order 1/r0.75 can model the macrocrack. The solution was validated by satisfying the equations of continuum mechanics with finite displacements at the singular crack tip. In addition, the microstructure effects of the material were also shown to affect the angular distribution of the double singularity local stress field. Hence, two additional parameters M1 and M2 would affect the angular variations of the stresses where the coordinate angle T is measured from the line extended from the original crack plane. The details can be found in [14]. They reveal the complexities of the analysis when the microstructural effects of the material are included. The influence of material microstructure on fatigue crack growth has received much interest in recent years [1520] although the approaches
184
G. C. Sih
varied from the empirical to the semianalytical models. The results when presented in terms of the crack growth rate da/dN can be irratic if the spatial and temporal scale is not carefully observed. Variance in data presentation cannot be avoided if no agreement can be found in defining nano, microand macrocrack size in relation to time. Consistency in data presentation appears to be needed before progress can be made to understand the underlying physical mechanisms that govern fatigue crack growth. 2. Statement of Fatigue Crack Growth Rate Models The advent of linear elastic fracture mechanics was followed by the development of the twoparameter fatigue crack growth relation [21]
da =A(ǻK) p dN
(1)
In Eq.(1), A and p were found empirically from a loglog plot of da/dN versus 'K which is known as the macrostress intensity factor such that it depends on the stress amplitude range and the square root of the half crack length a for a panel with a central crack of length 2a. To be more specific, reference can be to the plot in Fig.1 for aluminum alloys [22]. Region II refers to long cracks for a from 10 to 40mm. For short cracks with a in the range of 1 to 10mm, the curve acquires a different slope and has been referred to as the “threshold”. Under alternating tension and compression loading, the crack mouth opens and closes for each cycle. It can change from invisible (microscopic) to visible (macroscopic). The corresponding data switches from region I to region II. For lower da/dN, the crack size is even smaller with dimensions of 102 to 101mm. The recent concern is whether the classical 'K correlation should be replaced by other quantities to account for the change of small to large cracks. This would no doubt alter the shape of the da/dN curve, in addition to a possible reinterpretation of the physical mechanism(s) that is causing this change. Although countless empirical forms of 'K in Eq.(1) has been proposed to offer a better fit of the data, few of the models revealed any significant progress. The exception is the work in [23,24] that gave an exponent of p=2 using a selfsimilitude argument in contrast to p=4 [21] arrived from a plot of a multitude of fatigue data for aluminum alloys. By in large; the form of Eq.(1) has been retained while the exponent p may vary in application. In what follows, the classical form of 'K will be replace by ǻK macro micro such that
Invariant Form of Micro/MacroCracking in Fatigue
da dN
n C('K macro micro )
185
(2)
The superscript “macro” and subscript “micro” are introduced to show that ǻK macro micro can represent the intensity factor for the microcrack or the macrocrack depending on the tightness ratio V* of the contacting crack surfaces in addition to the micro/macro shear modulus ratio P* and a relative length parameter d* that defines the relative size of the local crack tip region as shown in Fig.2. The restraining stress Vo that controls the tightness of the crack surfaces is normalized to the applied stress Vf to define V*. In situations where the mean stress Vm plays an important role in addition to the stress amplitude Va, Eq.(2) will be further replaced by the range of the micro/macro energy density factor 'S macro micro offering another form of the fatigue crack growth relation:
da dN
m B('Smacro micro )
Fig. 1 Fatigue crack size increase with growth [22].
(3)
186
G. C. Sih
Fig. 2 Strong and weak stress singularity for the dual scale crack model.
3. Stress Intensification Approach The strength of stress singularity near a crack tip played a fundamental role in the development of the linear elastic fracture mechanics model as it can be related to the energy released by a unit extension of a selfsimilar crack. Such a simple interpretation ceases to prevail for a microcrack where antisymmetry becomes the rule rather than the exception. A brief description of the double singularity stress field will be made for the sake of continuity. 3.1 Double singularity stress field The double singularity solution can be found in [13]. Adopted in this discussion is a crack with freefixed surface condition. Two singularities of different order prevail at the same crack tip. There is the strong singularity with order 1/r0.75 and the weak singularity with order 1/r0.25 having the W macro respective intensities of (K S ) macro micro and ( K ) micro as shown by
(V ij ) macro micro
(K S ) macro micro 2Sr 0.75
f ij (M1 , T)
(K W ) macro micro 2Sr 0.25
g ij (M 2 , T)
The method of scale multiplier can be used [13] to give
(4)
Invariant Form of Micro/MacroCracking in Fatigue
(K S ) macro micro
d (K W ) macro micro
187
(5)
Eq. (1) can thus be rewritten only in terms of (K S ) macro micro as macro (ıij ) micro =
macro (K S ) micro
2ʌ r
0.75
[fij (ĳ1 ,ș)+
r g (ĳ 2 ,ș)]+ d ij
(6)
To be reminded is the notation ( ) macro micro that applies to the dual scale model to denote that the crack can be micro or macro depending on the ratio d/r (or d*) and the restraining stress Vo to applied stress ratio Vf ratio given * by V* that is contained in (K S ) macro micro . Large V would close the crack making it invisible and the opposite would result if the restraining stress is small. Refer to Fig.1. This effect is particularly important in fatigue where loading and unloading tend to open and close the crack continuously. As it can be seen from Eq. (6), the local crack tip stresses depend on the distance on the relative distance r/d. Such a character is also necessary for W macro addressing micro/macro effects. Since both (K S ) macro micro and ( K ) micro are related by Eq.(5), it suffices to consider (K S ) macro micro only and superscript s can be dropped to give
16 K macro micro =
ʌ (1Ȟ macro )µ micro ı f c 2 a 2 2ı a (1 o sin 1 ) 0.25 f(ĳ1 ,ĳ 2 )µ macro d ʌı f c
(7)
f(M1, M2)=5M1+7M2+12
(8)
provided that
The relation between c and a can be found in Fig.1. Eq. (4) can be found in [13] and will not be elaborated any further. 3.2 Crack growth relation based on stress intensity Assuming that the maximum and minimum values of applied and crack tip stresses occur at the same time without phase change, then the increment change of the local stress intensification K macro micro can be denoted by
188
G. C. Sih
'K macro micro
macro (K macro micro ) max ( K micro ) min
(9)
Making use of Eq.(7) and letting Vf equal to Vmax at maximum stress and to Vmin at minimum stress, it is found that
(K
macro micro max
)
16 S (1 Q macro )P micro c 2 a 2 2V o a (1 sin 1 )V max 0.25 c SV f f (M1 , M 2 )d P macro (10)
(K
macro micro min
)
16 S (1 Q macro )P micro c 2 a 2 2V a (1 o sin 1 )V min 0.25 c SV f f (M1 , M 2 )d P macro (11)
Inserting Eqs. (10) and (11) into Eq. (9), there results
'K macro micro
16 S (1 Q macro )P micro c 2 a 2 2V a (1 o sin 1 )(V max V min ) 0.25 c SV f f (M1 , M 2 )d P macro (12)
Recall that V*=Vo/Vf and P*=Pmicro/Pmacro. The length d=ca is defined in Fig.1 and the quantities M1 and M2 can be identified with different microcrack branching patterns [14]. They may also be related to fissures and striations that are observed by micrographs in the fatigue of aluminum alloys. Although these microscopic effects involving the Ms can be included in Eq. (12), it is more pertinent to focus attention on the invariant form of da/dN by first expressing Eq.(2) in the form
da dN
n C1 ('K macro micro )
(13)
At this stage, the incidental variables M1 and M2 or the function f(M1,M2) can be absorbed into the macroparameters. More specifically, the quantity 3f(M1,M2)/40 may be factored out of Eq.(13) after eliminating ǻK macro micro by
using Eq.(12). This renders a new ǻK macro micro without f(M1,M2) that will be understood to be
Invariant Form of Micro/MacroCracking in Fatigue
'K
189
6 S (1 Q macro )P micro c 2 a 2 2V a (1 o sin 1 )(V max V min ) 0.25 c SV f 5d P macro
macro micro
(14)
A new parameter C can now be defined as n
C
ª º 40 « » C1 ¬ 3f (M1 , M 2 ) ¼
(15)
Application of Eqs.(14) and(15) can convert, Eq.(13) to the form of Eq.(2) which will be used for the calculation of numerical data. There should be no confusion between the use of ǻK macro micro in Eq.(12) with f(M1,M2) and the use of ǻK macro micro in Eq.(14) without f(M1,M2). Both form of da/dN involves only two empirical parameters C1 and n or C and n. The foregoing exercise shows explicitly that microscopic effects can be hidden in the macroscopic empirical constants C, C1 and n. 4. Energy Density Intensification Approach The local energy density factor can be used to include the effect of mean stress. The form of dW/dV that can be applied to micro/macrocracking given by macro
§ dW · ¨ ¸ © dV ¹ micro
[S(r, T)]macro micro r
(16)
4.1 Strength of energy density singularity The 1/r singularity for dW/dV applies also for the double stress singularity field of Eq.(4) or (6). Knowing that K is related to S [3], it can be shown that [13]
S
macro micro
(1 Q macro ) 2 (c 2 a 2 ) P 2V a ( micro V f ) 2 (1 o sin 1 ) 2 F(T) 2 0.5 0.5 SV f c P macro 128f (M1 , M 2 )P micro d r (17)
Note that
190
G. C. Sih
F(T)
1 [f r (T) f T (T)]2 2[f rT (T)]2 2
(18)
in which fr(T), fT(T) and frT(T) are complicated functions of T and Mj with j=1, 2. They can be found in [13] and will not be repeated here since they can be absorbed into the empirical parameters to be shown later. The energy density intensification is nonuniform around the crack and S macro micro in Eq.(17) can depend on the radial distance r from the crack tip and the microstructural details via f(M1, M2). 4.2 Crack growth relation based on energy density intensification While nonlocal effects are included in 'K macro micro of Eq.(2), 'K of Eq.(1) applies locally only in the limit that the distance r approaches zero. Scaling for crack growth has also been excluded in the classical 'K. This limitation does not exist in the 'S macro micro which can be regarded as the energy released when the crack extends by the amount r='a. Now let (S macro micro ) max be associated with Vmax and (S macro micro ) min associated with Vmin such that
'S macro micro
macro (S macro micro ) max (S micro ) min
(19)
and using Eq. (17), it can be shown that 'Smacro micro
(1 Q macro ) 2 (c 2 a 2 ) P 2V a ( micro ) 2 (1 o sin 1 ) 2 F(T)(V 2max V 2min ) 128f 2 (M1 , M 2 )P micro d 0.5 r 0.5 P macro SV f c (20)
A two parameter fatigue crack growth rate relation can thus be obtained:
da dN
m B1 ('S macro micro )
(21)
This is reminiscence of the classical strain energy density approach to fatigue in [3] if 'S macro micro in Eq. (21) is replaced by 'S for macrocracking only. A simplified version of Eq. (20) or (21) may be used by leaving out
Invariant Form of Micro/MacroCracking in Fatigue
191
the details of the incidental parameters M1 and M2. This can be
accomplished by letting
B [
F(T) ]m B1 32f (M1 , M 2 )(1 2Q micro ) 2
(22)
and defining a new 'S macro micro without f(M1, M2). Again, there should be no confusion between Eq.(20) with f(M1, M2).and Eq.(23) without f(M1, M2). In what follows, Eqs.(22) and (23) will be used such that da/dN can be computed from Eq.(3). This completes the derivation of the dual scale line crack model based on the energy density intensification approach. Calculation of numerical results will follow. 'Smacro micro
(1 2Q micro )(1 Q macro ) 2 (c 2 a 2 ) P micro 2 2V a ( ) (1 o sin 1 ) 2 (V 2max V 2min ) 0.5 0.5 P macro SV f c 4P micro d r
(23) 5. Invariant Form of TwoParameter Fatigue Crack Growth Rate Relation The two parameter crack growth rate relation of Eq. (1) was first proposed in [21] and discussed in [23, 24] with reference to the value of the exponent p on 'K. Although much work has been done in the ways that A and p in Eq.(1) are affected by microscopic effects, it is rather recent that da/dN were made reference to small cracks [25,26]. While crack sizes can be addressed with reference the three regions I, II and III in Fig.3, it is not clear how the crack size/time effects can be identified with the 'K since the two parameter fit applies only to region II by the equation
log
da = plog(ǻK)+logA dN
(24)
With data fitted to a straight line, A can be determined from yintercept and p from the slope of the line in Fig. 3. The three regions I, II and III are also referred to the micro, macro and fast crack growth in Fig.4(a). Use of macro 'K macro micro or 'S micro can make the fatigue data to lie on a straight line as shpwn in Fig. 4(b). In this way, linear interpolation can be used to connect the results of regions I, II amd III and Eqs.(2) nd (3) are said to be form invariant for microcracking and macrocracking in fatigue.
192
G. C. Sih
Fig. 3 Fatigue data representation of Eq.(1) for through cracks in two dimensions.
(a) Crack growth data (b) Invariant form of 'K or 'S Fig. 4 Invariant form of crack growth rate in relation to region I, II and III: (a) Crack growth data; (b)Linear line plot of 'K or 'S.
5.1 Crack surface tightness stress ratio As mentioned earlier, accommodation for the opening and closing of the crack surfaces is a major consideration for modeling the fatigue crack growth behavior. This implies that the restraining stress Vo in relation to the applied stress Vf or the ratio Vo/Vf should vary with the crack half length a. Assuming that
Invariant Form of Micro/MacroCracking in Fatigue
Vo Vf
0.65, for a 3mm ° ®0.48421, for a 10mm °0.01049, for a 65mm ¯
193
(25)
the bilinear relationship between the stress ratio Vo/Vf and the crack half length a is adopted.
Vo Vf
0.023684a 0.72105, for 1 d a d 10mm ® ¯ 0.008613a 0.57034, for 10 d a d 65mm
(26)
The unit of length a is millimeter. The two stage bilinear relationship is displayed in Fig. 5. The corresponding numerical values of the curve in Fig. 5 are summarized in Table 1. 5.2 Microcrack tip open segment ratio As the micro/macro crack extends, the tip opening segment length d can also have an effect. That is local intensification will depend on the relative distance r/d which will increase with a as the microcrack becomes macroscopic. This ratio is not sensitive for very small cracks. The behavior
Fig. 5 Bilinear relationship for stress ratio Vo/Vf versus crack half length a.
194
G. C. Sih Table 1 Values of stress ratio Vo/Vf with the crack half length a.
Fig. 6 Length ratio r/d versus crack half length a.
a(mm) r/d
Table 2 Values of length ratio r/d with the crack half length a. 10 40 60 65 d8 0.73 1 5 7.7 8.3
is shown in Fig. 6 and the numerical results can be found in Table 2. The 'K macro micro model of Eq.(14) is independent of the radial distance r. A value of d=1mm will be used. The curve in Fig. 6 applies only to the 'S macro micro of Eq. (23). It suffices to know the trends of the curves in Figs. 5 and 6 for application of the dual scale model. Moreover, only Fig. 5 is needed to make the form
Invariant Form of Micro/MacroCracking in Fatigue
195
of the crack growth rate relation in Eq.(14) invariant. However, better correlation of fatigue data is obtained using Eq. (23) where Fig. 6 is also used. This because Eq.(23) corrects for the mean stress effects whereas Eq. (14) does not. 6. Linearization of Micro/MacroData for Fatigue Crack Growth Rate Referring to the data in [22] for the fatigue tests of 2024T3 and 7075T6 aluminum precracked panels, the dual scale models based on 'K macro micro in Eq. (14) and 'S macro micro in Eq. (23) will be used such that data in regions I, II and III as shown in Fig.3 would lie on a straight line without any bends. The shear modulus ratio Pmicro/Pmacro will be set at two because its value is not known to change with the crack length. The parameters V* and d* will account for the transition of microcracking to macrocracking and vice versa. Use will be made of the macroscopic properties of 2024T3 and 7075T6 given in Table 3. Data [22] for six different cases will be analyzed. They are referred to the means stress Vm= (Vmax+Vmin)/2 and the stress amplitude Va= VmaxVmin as shown in Table 4 with R being the mean stress ratio Vmin/Vmax. Table 3 Mechanical properties of 2024T3 and 7075T6 aluminum alloy. Material type
Yield strength Vyd (kg/mm2)
Ultimate strength Vult (kg/mm2)
Shear modulus Pmacro(kg/mm2)
Poisson’s ratio Qmacro
2024T3
37.1
48.3
2812
0.33
7075T6
47.3
53.0
2742
0.33
Table 4 Case classification of fatigue crack growth data. Case
Vm (kg/mm2)
Va (kg/mm2)
R
I
12
2.5
0.655
II
12
4.0
0.500
III
12
6.5
0.291
IV
9
2.5
0.565
196
G. C. Sih V
9
4.0
0.385
VI
9
6.0
0.161
6.1 Discussion of results using Eq.(2) Based on the numerical results provided earlier, the log of da/dN versus log of 'K macro micro may be plotted. The curves for 2024T3 and 7075T6 aluminum alloy are displayed in Fig. 7. Note that the data in all three regions I, II and III can now be adequately represented by straight lines. The slope for 2024T3 signified by n is 3.532 which is smaller than that of 7075T6 with n=4.179. This means that the crack growth rate of 2024T3 is slower than that of 7075T6 which is to be expected. Not to be misled is that the xcoordinate in Fig. 7 has been shifted and did not start from zero. The full scale is exhibited in Fig. 8 such that the yintercepts give log C=6.967 for 7075T6 and 6.710 for 2024T3. When the stress amplitude Va is raised from 2.5 to 4.0 kg/mm2 for the same mean stress Vm= 12 kg/mm2 although the stress ratio R is reduced from 0.655 to 0.500, a slight increase in the crack growth rate da/dN for both materials are seen. This is
Fig.7 Log crack growth rate da/dN v.s. log micro/macro stress intensity range
'K macro micro for Case I.
Invariant Form of Micro/MacroCracking in Fatigue
197
Fig.8 Coordinates redefined for log crack growth rate da/dN v.s. log micro/macro stress intensity range
'K macro micro for Case I.
Fig.9 Log crack growth rate da/dN v.s. log micro/macro stress intensity range
'K macro micro for Case II. the results of increase in the slopes of the straight lines for 2024T3 (n=3.632) and 7075T6 (n=4.297). The straight line fit in Fig. 9 is good because most of the data points pertained to half crack length in the range 10 to 40 mm corresponded to region II.
198
G. C. Sih
A further increase of the stress amplitude to Va = 6.5 kg/mm2 with Vm= 12 kg/mm2 leads to additional reduction in R to 0.297. This shows that the slopes of da/dN acquire further gain with n=4.224 for 2024T3 and n=4.742 for 7075T6 although the data gained more scatter as shown in Fig.10. The detrimental effect of increase stress amplitude on fatigue life is exemplified as in the use of the classical SN curve where no consideration to crack growth was made. Reduction of the maximum stress also has a noticeable effect on the crack growth rate. Consider Case IV in Table 4 where Va = 2.5 kg/mm2 with Vm= 9 kg/mm2 and R = 0.565 being similar to that in Case I. A complete set of data points for all three regions were obtained as exhibited in Fig. 11. Decrease in the slopes of the curves confirms a reduction of the crack growth rate when the stress amplitude is decreased. The effect of stress amplitude starts to take over in Case V when Va = 4.0 kg/mm2 with Vm= 9 kg/mm2 and R = 0.385. Fig. 12 shows that the slopes of the curves are increased to n=3.725 for 2024T3 and n=3.781 for 7075T6. Further aggravation of the crack growth rate is seen by the curves in Fig. 13 when the stress amplitude is raised to Va = 6.0 kg/mm2. Now the slopes attain even higher values of n=3.812 for 2024T3 and n=4.511 for 7075T6.
Fig.10 Log crack growth rate da/dN v.s. log micro/macro stress intensity range
'K macro micro for Case III.
Invariant Form of Micro/MacroCracking in Fatigue
199
Fig.11 Log crack growth rate da/dN v.s. log micro/macro stress intensity range
'K macro micro for Case IV.
Fig.12 Log crack growth rate da/dN v.s. log micro/macro stress intensity range
'K macro micro for Case V.
G. C. Sih
200
Fig.13 Log crack growth rate da/dN v.s.log micro/macro stress intensity range
'K macro micro for Case VI. The findings in Figs. 7 and 13 can be summarized in Table 5 for a comparison of the data for the 2024T3 and 7075T6 material, particularly with reference to the parameters C and n in Eq. (2) for the 'K macro micro model. The stress amplitude is seen to play a dominant role by the fatigue data in Table 5. Cases I to III show that the increase in stress amplitude tends to increase the crack growth rate by raising both the yintercept log C and the slope n. The reduction of maximum stress reflected by lowering the mean stress Vm for Cases IV to VI did lower the da/dN as shown by Case IV but the further increase in the stress amplitude again raised the absolute log C and n values as summarized in Table 5. Table 5 Stress amplitude and mean stress effects on C and n in Eq. (2). Case I II III IV V VI
Log C 6.961 7.336 8.907 6.455 6.748 8.530
7075T6 n 4.179 4.297 4.742 3.765 3.781 4.511
Log C 6.770 7.067 8.492 7.139 7.410 7.854
2024T3 n 3.532 3.632 4.224 3.707 3.725 3.812
Invariant Form of Micro/MacroCracking in Fatigue
201
6.2 Discussion of results using Eq.(3) macro The difference between 'K macro micro in Eq. (14) and 'S micro in Eq. (23) is not insignificant and will vary for different test conditions and materials. Based on the same crack growth data as those used for obtaining the curves in Figs. 7 to 13, Fig. 14 displays a plot of log(da/dN) versus log( 'S macro micro ). All data points fell on straight lines, one for 2024T3 and one for 7075T6 with the respective slopes of m=2.690 and 3.394. These values are smaller than those of n=3.532 and 4.179 in Table 5 for Case I of the 'K macro micro model. The difference in slopes for the two materials using the two models is about the same. Fig. 15 shows similar trends for Case II where the data are more scattered as the stress amplitude was increased from 2.5 to 4.0 kg/mm2. Much more scatter of the data resulted in Case III where Va is increased to 6.5 kg/mm2 with Vm kept at 12 kg/mm2. This is also accompanied by an increase in the crack growth rates as illustrated in Fig. 16. The values of the slope m in Figs. 14 to 16, however, are much closer together when the same data are represented by the 'K macro micro model shown by the curves in Figs. 7 to 10 inclusive. A good fit of the data is found in Fig. 17 for Case IV. The two straight lines for 2024T3 and 7075T6 are nearly parallel with slopes of m=3.036 and 3.055. The superiority of the fatigue crack growth resistance for 2024T3 does not show up for the applied mean stress and stress amplitude. The 7075T6 aluminum would have served equally well. This illustrates the location specificity when selecting the use of materials in nonuniform stress and/or energy density fields. The crack growth behavior of the two materials start to deviate from one another as the stress amplitude is raised to 4.0 kg/mm2 with a mean stress of 9 kg/mm2 as in Case V where the plot of 'S macro micro is given in Fig. 18. Case VI for
Va=6.0 kg/mm2 corresponds to the results in Fig. 19. Data for large stress amplitudes tend to have more scatter. It is worthwhile to note the slopes m in Table 6 and compare them to the values n in Table5. An important conclusion is that the variations of the m values are much less than those for n as the mean stresses are change. This is to be expected because the macro 'S macro micro model accounts for the mean stress effect whereas the 'K micro model does not. This concludes the presentation of the numerical results for the fatigue crack growth rate where the data were transformed onto a straight line relationship. To be noted is that the position of the xaxis in Figs. 14 to 19 has been shifted and did not start from the origin. The difference in reference can be seen from the curves in Figs. 7 and 8. The
202
G. C. Sih
locations of the yintercepts in Table 6 should now be clear. Moreover, the macro log 'S macro micro in Figs 14 to 19 are negative while 'S micro in Eq. (23) is positive definite.
Fig. 14 Log crack growth rate da/dN vs. log micro/macro energy density range
'S macro micro for Case I.
Fig. 15 Log crack growth rate da/dN vs. log micro/macro energy density range
'S macro micro for Case II.
Invariant Form of Micro/MacroCracking in Fatigue
203
Fig. 16 Log crack growth rate da/dN vs. log micro/macro energy density range
'S macro micro for Case III.
Fig. 17 Log crack growth rate da/dN vs. log micro/macro energy density range
'S macro micro for Case IV.
204
G. C. Sih
Fig. 18 Log crack growth rate da/dN vs. log micro/macro energy density range
'S macro micro for Case V.
Fig. 19 Log crack growth rate da/dN vs. log micro/macro energy density range
'S macro micro for Case VI.
Invariant Form of Micro/MacroCracking in Fatigue
205
Table 6 Stress amplitude and mean stress effects on B and m in Eq. (21). 7075T6 2024T3 Case Log B m Log B m I
8.314
3.394
6.286
2.890
II
8.098
3.394
6.224
2.888
III
7.268
3.153
7.052
3.303
IV V
7.711 7.035
3.055 2.947
6.885 6.741
3.036 3.015
VI
7.992
3.326
6.632
3.019
7. Concluding remarks Even though metal fatigue has been researched for more than a century, full confidence is still lacking when prediction of fatigue life of structural components is at stake.. By in large, the effort has been concerned with relating the onset of rapid fracture to the initiation of cracks under low stress but repeated many times. In more recent times, attention has been focused on explaining the size and time scaling effects associated with the fatigue crack growth rate da/dN models with reference to the commonly known regions I, II and III. In particular, the use of the macroscopic stress intensity factor range 'K for region I is questioned. The concerns are whether data for micron size and smaller cracks could still be adequately correlated by the two parameter relation. Hence, a fourth region for crack nucleation has been proposed [25.26]. This region is effectively concerned with nanometer size cracks with length a  104 mm or smaller. Crack nucleation may have to be identified with a fifth region. What this indicates is that the discovery of defect initiating at smaller and smaller time and size scales necessitates a more refined procedure for modeling the evolution of crack initiation to propagation. Several issues are in need of additional attention: (1) Is it possible to retain the two parameter da/dN relation using 'K macro micro or some other parameter and describe nanoscale cracks assuming that the line crack configuration can be retained? (2) If the answer to (1) is positive, then will it be possible to establish an macro invariant form of da/dN using 'K macro micro or 'S micro ?
206
G. C. Sih
What has been learned from experience is that through crack specimens are more conducive to the aircraft structure engineers who entail crack length a 1080 mm (macromechanical) that falls into region II. Material engineers are more concerned with surface cracks due material microstructure effects associated with region I where a 103 to101mm (microstructural). The fourth region would presumably fall into the scale range most sensitive to chemical reactions. This corresponds to a 104 mm or smaller (nanochemical) [27]. Defects in this size range appear very early and are deeply trapped to the interior of the material. The inherent coupling of size and time scale possesses a hierarchy in the damage process that can be referred to as macromechanical, microstructural and nanochemical. Subatomic effects will no doubt be of interest to the biologists that may be further classified with the prefix pico or femto. The point to be made is that the creation of different imperfections, defects or cracks are intimately related to the dissipated energy density of a particular physical process. They are inherently paired in size and time. It is clear that length alone is not adequate for distinguishing micro and macrocracks. In fatigue, the time variable is accounted for by dN/dt which is in fact the frequency of the fatigue cycles. Hence data can be represented in terms of da/dt just as well as da/dN. Tightness of the crack mouth, however, is regarded important because it can change microcracking to macrocracking or the other way around under alternating tension and compression loading. The clue that there prevails a very small segment of the microcrack tip that does not close because of microasymmetry prompted the discovery of double singularity stress field [13]. Two competing singularities prevail one being stronger with the order 1/r0.75 and the other weaker with the order 1/r0.25. The simultaneous consideration of the double singularity is responsible for explaining the transitory behavior of micro and macrocracking. In retrospect, any multiscale crack models should have the capability to alter the morphology of the defect during scale transition. At the same time, connection of the results at the different scales can be best achieved by linear interpolation if the da/dN data can be made to lie on a line. Such a possibility can also be realized in a transformed plane that is often used in space transformation. An immediate extension of the present approach would be the development of a triple scale model of macro/micro/nano cracks. References [1] [2]
Griffith A A. The phenomenon of rupture and flow in solids, Philosophical Transactions, Royal Society of London, Series A221 (1921) 163198. Irwin GR. Fracture Mechanics, In: Structural Mechanics, Pergamon Press,
Invariant Form of Micro/MacroCracking in Fatigue
[3] [4] [5] [6] [7] [8] [9] [10]
[11]
[12]
[13]
[14]
[15]
[16]
[17]
[18]
[19]
207
New York, (1960) 557592. Sih GC. Mechanics of fracture initiation and propagation. The Netherlands: Kluwer Academic Publishers, 1991. Sih G.C. Crack front behavior of mesofracture in nonequilibrium mechanics, Journal of Physical Mesomechanics, 1(1) (1998) 7787. Popov VL. and Kroner E. On the role of scaling in elastoplasticity, Journal of Physical Mesomechanics, 1(1) (1998) 103112. Sih GC. Thermomechanics of solids: nonequilibrium and irreversibility, J. of Theoretical and Applied Fracture Mechanics, 9(3) (1988) 175198. Sih GC. Some basic problems in nonequilibrium thermomechanics, eds. S. Sienietyez and P. Salamon, Taylor and Francis, New York, 1992, 218247. Schwab K. Henrikson E. A., Worlock J. M. and Roukes M. L. Measurement of the quantum of thermal conductance, Nature, 404 (2000) 974976. Roukes ML. Plenty of room indeed. In: The Edge of Physics, Scientific America (2001) 92100. Sih GC. Signatures of rapid movement of electrons in valence band region: interdependence of position, time and temperature, J. of Theoretical and AppliedFracture Mechanics, 45(1) (2006) 112. Sih GC. and Tang X. S. Dual scaling damage model associated with weak singularity for macroscopic crack possessing a micro/mesoscopic notch tip, J. of Theoretical and Applied Fracture Mechanics, 42(1) (2004) 124. Tang X.S. and Sih G. C. Weak and strong singularities reflecting multiscale damage: microboundary conditions for freefree, fixedfixed and freefixed constraints, J. of Theoretical and Applied Fracture Mechanics, 43(1) (2005) 562. Sih G.C. and Tang X. S. Simultaneous occurrence of double micro/macro stress singularities for multiscale crack model, J. of Theoretical and Applied Fracture Mechanics, 46(2) (2006) 87104. Tang XS. and Sih GC. Evaluation of microstructural parameters for micro/ macroline crack damage model, J. of Theoretical and Applied Fracture Mechanics,46(3) (2006) in press. Sih GC. and Tang XS. Simultaneous occurrence of double micro/macro stress singularities for multiscale crack model, J. of Theoretical and Applied Fracture Mechanics, 46(2) (2006) 87104. Vasudevan AK. Sadananda K. and Louat N. A review of crack closure, fatigue crack threshold and related phenomena, Material Science and Engineering, A188 (1994) 122. Newman Jr. JC. Brot A. and Matias C. Crackgrowth calculations in 7075T7351 aluminum alloy under various load spectra using an improved crackclosure model, Engineering Fracture Mechanics 71 (2004) 2347–2363. Noroozi AH. Glinka G. and Lambert S. A two parameter driving force for fatigue crack growth analysis, International Journal of Fatigue, 27 (2005) 12771296. Jones R. Barter S. Molent L. and Pitt S. Crack growth at low K's and the FrostDugdale law, Journal of the Chinese Institute of Engineers, Special Issue inHonour of Professor G. C. Sih, 27(6) (2004) 869875.
208
G. C. Sih
[20] Jones R. and Pitt S. On the Frostdugdale law and the two parameter driving force for fatigue crack growth analysis, Sixth Int. Conf on Fatigue Damage of Structural Materials: Fatigue Damage VI, Hyannis, Massachusetts, Sept. 1722, 2006. [21] Paris PC. The growth of cracks due to variations in load, Ph. D. Dissertation, Department of Mechanics, Lehigh University (1962). [22] Broek D. and Schijve J. The influence of the mean stress on the propagation of fatigue cracks in aluminum alloy sheets, National Aeronautics and Astronautics Research Institute NLRTN M. 21111, Amsterdam (1963) 157. [23] Liu HW. Fatigue crack propagation and applied stress range, ASME Trans., J. Basic Eng. 85D(1) (1963) 116122. [24] Liu HW. A review of fatigue crack growth analyses, J. of Theoretical and Applied Fracture Mechanics 16 (1991) 91108. [25] McDowell DL. Multiaxial small fatigue crack growth in metals, Int. J. Fracture, 19(1) (1997) S127S135. [26] Wang CH. Effect of stress ratio on short fatigue crack growth, ASME Journal of Engineering Materials and Technology, 118 (1996) 362366. [27] Sih GC. Crack tip system for environment assisted failure of nuclear reactor alloys: multiscaling from atomic to macro via mesos, J. of Pressure Equipment and Systems, 3(2005)125.
Fatigue Crack Growth Rate of CableStayed Portion of Runyang Bridge: Part I–Cable Crack Growth Due to Disproportionate Cable Tightening/Loosening and Traffic Loading G. C. Sih 1, 2 * and X. S. Tang 3 International Center for Sustainability, Accountability and EcoAffordability of Large Structures (ICSAELS) Advanced Technology for Large Structural Systems (ATLSS) Lehigh University, Bethlehem, PA 18015, USA 2 School of Mechanical and Power Engineering, East China University of Science and Technology, Shanghai 200237, China 3 School of Bridge and Structural Engineering, Changsha University of Science and Technology, Changsha, Hunan 410076, China * Email:
[email protected],
[email protected] 1
Abstract Relatively little is known about the fatigue crack growth behavior of bridge cables. Such information can become increasingly more important in time for the cablestayed bridges whose structural integrity can be greatly affected by the degradation of the individual cable material due to aging as well as defect growth. Moreover, crack initiation and propagation are intimately related such that they have to be treated as one of the same process. This requires a dual scale fatigue crack growth model involving both micro and macrocracking where the interaction of three micro/macro material, geometric and load parameters is considered. Based on the design data for the stresses in the 52 cables of the Runyang cablestayed bridge, three typical cables referred to as #28, #38 and #50 are selected for analyzing fatigue crack growth under traffic and no traffic conditions. The initial tension in the cable can vary by using D=1 as the reference such that deviation from the design condition may be regarded as tightening and loosening. Under traffic, initial tightening and loosening of the cable can enhance and impede fatigue crack growth, respectively. When traffic is removed, initial tightening and loosening of the cable can impede and enhance fatigue crack growth. Opposing effects of fatigue crack growth are observed for cables with and without traffic. These results are discussed in terms of crack growth rate and crack length as a function of the fatigue cycles assuming that the cable has a life of two million cycles. Substantial variance in fatigue crack growth is found. Crack G.C. Sih (ed.), Multiscale Fatigue Crack Initiation and Propagation of Engineering Materials: Structural Integrity and Microstructural Worthiness, 209–247. © Springer Science+Business Media B.V. 2008
210
G. C. Sih and X. S. Tang
length can vary from a few mm to 50 mm and more before reaching the onset of rapid fracture. The stiffness of the cable is also affects crack growth. Each cable is found to behave as a structure of its own. Replacement of cables appears to be eminent during the life span of cablestayed bridge because of the wide variance of fatigue lives of the cables. This means that some cables will fail while others may still have ample remaining life. 1. Introduction The critical components in a cablestayed bridge are no doubt the cables each of them behaves differently and acts as a structure in itself. The effects of the main load carried by the bundles of high strength steel wires are susceptible to change in time because aging and degrading of the material property will occur in addition to corrosion caused by the environment conditions. The current construction of the cables inhibits and prevents the successful use of nondestructive testing despite extensive efforts are being made in health monitoring. For bridges that have been in service after a decade or more the situation becomes even more uncertain because damage accumulates at the different scales, say micro and macro. This fact was recognized from the earlier research on dual scaling [1,2]. Empirical models may not be adequate because they are unable to know the presence of tightly closed cracks even though the material may have separated locally. In this case, there is no signal to transmit for detection. To reiterate, this is especially true for situations where the faults can closed and remain dormant but they can open to inflict serious damage under overload or unexpected accidents such as earthquakes or vehicle impact. The undetected flaws can alter a situation of failsafe to one that triggers disaster. On site health monitoring is only as effective as knowing the locations where gages should be placed. The critical sites are often hidden and inaccessible for inspection until damage becomes excessive. Not enough emphasizes can be placed on knowing the potential sites of damage for a given design and how damage would develop in service. An understanding of failsafe in the design of large structures [3] is vital for the mitigation or prevention of potential injury/life and property. The period for the inspection of bridges is every two years. This is a mandatory requirement of the US National Bridge Inspection Standard (NBIS). The recent disaster of the I35W bridge in Minnesota [4] is indicative of the ineffectiveness of implementing the standards. Although the current stateoftheart of bridge maintenance and inspection recognizes the importance of flaw detection caused by fatigue for steel structure bridges [5,6] but relatively little attention [79] has been devoted
Fatigue Crack Growth Rate of Runyang Bridge: Part I
211
to the long term fatigue of cables for suspension and cablestayed bridges. Most of the cable fatigue works address the initial design requirement [10,11] which can cast false confidence on the interpretation of field data, particularly when uncertainties prevail with the assumed boundary conditions in design. This problem is particularly acute for the cablestayed bridge that may possess more than one hundred cables and each of them can have widely different behavior. It means that some of them may be on verge of breaking while others may still have ample remaining life. The study in [9] has shown such effects to be prevalent by using the design data of the cablestayed portion of the Runyang bridge [12]. The diversification of cables’behavior is typical as they can experience loosening and tightening every hours of the day where the traffic may vary from full to no load, not counting for wind that also causes variation in cable tension. This becomes increasingly problematic for aging cablestayed bridges as the cables do not deteriorate at the same rate. Some may have ample remaining life while others are in need of replacement. The present monitored data are not capable of sorting out the degree of cable damage because no confidence can be placed on their association with the actual physical damage. This problem cannot be alleviated by embedding sensors into the cables during fabrication. There is not a direct correspondence between the sensor and the local damaged area. It is necessary to have a validated software that can address fatigue damage for interpreting the sensor data, preferably over an area that is large in comparison with the damage. Not enough emphasis can be placed on the latter, especially when microcracking and macrocracking are both mingled in the signal. It was demonstrated in [9] that the crack growth behavior in two of the Runyang bridge cables differed widely when fatigued under traffic and no traffic conditions. The discrepancy can be the difference of stable crack growth and the onset of rapid fracture. Additional work is carried out in this communication to offer a more complete discussion of the fatigue crack growth behavior of cables for the Runyang bridge. Considered in particular is the crack growth rates of some typical cables showing that the variance may be relevant for the future development of maintenance and inspection procedures. 2. Problem Statement The Runyang bridge consists of two portions as shown in Fig. 1(a) for the cabledstayed portion and Fig. 1(b) for the suspension portion. A close view of the cables for the cablestayed portion can be found in Fig. 2. Note that the cables are mounted onto the two towers and anchored at the girders of the bridge. The distance between the two compressed towers is
212
G. C. Sih and X. S. Tang
406m. The structure is sufficiently flexible such that it can sway. Because of the load variations, tightening and loosening of the cables is expected. Considered are conditions for the bridge under traffic and notraffic conditions. The large variations of fatigue lives for the cables are identified for several different scenarios of cable tightening and loosening that can be caused by climate changes, a particular concern in recent years. The results are needed for the development of inspection procedures for the health monitoring of the Runyang bridge. Similar analysis should be done for the suspension portion of the bridge.
(a) Cablestayed portion (b) Suspension portion Fig. 1 Close view of the cablestayed and suspension portions of Runyang bridge.
Fig. 2 The Runyang cablestayed portion of the bridge with 406m span.
2.1 Cable forces with and without traffic Assuming symmetry, only 52 of the total of 104 cables of the Runyang cablestayed bridge need to be shown. The tension in the cable with no traffic and with traffic is as shown, respectively, in Figs. 3 and 4. The position
Fatigue Crack Growth Rate of Runyang Bridge: Part I
213
of each cable is shown and numbered from left to right. The largest forces prevail in cables #3 and #50. They are located, respectively, third from the left and right end position. The small differences in the forces in cables #1~#26 and #27~#52 can be ignored. To be examined are the fatigue crack growth characteristics in cables #28, #38 and #50 where cable #38 corresponds to the minimum tension.
Fig. 3 Load in cables without traffic.
Fig. 4 Maximum and minimum load in cables with traffic.
2.2 Multiscale application of fracture mechanics Modern bridge design takes into account the influence of material properties such as high to very high strength, high temperature and corrosive resistance. This implies that the microstructural effect of the material comes
214
G. C. Sih and X. S. Tang
into play. From the fracture mechanics view point, it is necessary to consider the behavior of small cracks that might be dormant under one condition and grow to large cracks under another condition. Microcracks and its transition to macrocracks must be accounted for. The traditional sigmoidal curve as illustrated in Fig. 5 can no longer be represented by the twoparameter crack growth rate relation [13] because it remains straight only for the portion Region II for macrocrack growth (or long cracks). Microcracks grow in Region I referred to as the threshold. Region III pertains to fast crack propagation heading towards the onset of global instability. Nondestructive testing should therefore be designed to detect the stable macrocrack growth in Region II.
Fig. 5 Traditional twoparameter fatigue crack growth rate.
Fig. 6(a) shows the crack growth curves partitioned with reference to the crack size from nano to macro. In order to preserve the traditional framework of fracture control of using only two empirical parameters, a multiscale model of crack growth was advanced [14,15] by replacing the range or of stress intensity factor 'K [13] for macrocracks only with 'K macro micro that can account for the transition of microcracks to macrocracks 'S macro micro or vice versa. The extension to triple scale involving nano, micro and macro is straightforward. In general the use of 'S macro is preferred because micro or it accounts for the effect of mean stress. Examples of using 'K macro micro can be found in [14,15]. In a log da/dN versus log 'K macro or 'S macro micro micro log 'S macro domain, the three Regions I, II and III no longer appear as sigmicro moidal. Instead, a straight line is obtained. This is shown in Fig. 6(b). This enables the shifting of the results from nano to micro and from micro to macro or directly from nano to macro.
Fatigue Crack Growth Rate of Runyang Bridge: Part I
215
(a) Crack growth curve (b) Crack growth rate Fig. 6 Form invariant property of multiscale crack growth rate relation.
2.3 Stress amplitude and mean stress The simultaneous consideration of stress amplitude Va=VmaxVmin and mean stress Vm=(Vmax+Vmin)/2 suggests the application of 'S macro which micro will be made use of in the sequel. Here, Vmax and Vmin are the maximum and minimum cyclic applied stress, respectively. Further distinction must be made because they are different under traffic and notraffic conditions. The superscripts D refers to traffic condition and o to traffic absent condition. The values of V omax and V Dmax for the 52 cables of the Runyang bridge can be found in Table A1 of Appendix I of [9]. Two Cases I and II will be considered; they are defined as DV Dmax V omax Case I: V a DVDmax V omax , V m (1) 2 V Dmax DV omax Case II: V a V Dmax DVomax , V m (2) 2 Case I in Eq. (1) refers to tightening of the cables that correspond to D=1.0, 1.2, 1.4 and 1.6 with D=1 (normal tension) as the reference. Numerical values of Va, Vm and VaVm for the 52 cables in Runyang bridge with D=1.0, 1.2 and 1.6 are given in Tables A2, A3 and A4, Appendix II of [9]. Case II in Eq. (2) refers to loosening of the cables that correspond to V=0.91, 0.94, 0.97, 1.00 (normal tension). Henceforth, ĮıĮmax will be referred to as “max. stress with traffic” and Įıomax as “max. stress without traffic.” Remember that D=1.0 stands for normal tension while Dt1ҏ and Dd1ҏrefer, respectively to more and less cable tension. Cable tightening and loosening are defined in terms of Va and Vm as given by Eqs.(1) and (2).
216
G. C. Sih and X. S. Tang
2.3.1 Case I: cable tightening and loosening with traffic
Fig. 7 displays a plot of the product VaVm for the cables as a function of the cable position from left to right numbered as 1 to 52. Note that the product VaVm fluctuates according to the variations of the tension in the cables due to varying traffic as indicated in Fig. 4. The end cables peak with a dip for the middle cable. The minima tension occur in cables #14 and #38. Symmetry about cable #26 is not quite preserved. The cable tightens with increasing D from 1.0 to 1.6 with the maximum VaVm at D=1.6 which will tend to reduce fatigue life. The peaks of the curves corresponding to cable #3 and #50 rise very quickly with the parameter D.
Fig. 7 Product VaVm of cables versus position of cables for Case I (tightening) with D=1.0, 1.2, 1.4 and 1.6 under varying traffic.
Numerical values of Va, Vm and VaVm for the 52 cables of the Runyang bridge with D=0.97 and 0.91 can be found in [9] as mentioned earlier. Loosening of the cable under traffic has a beneficial effect to fatigue life. This can be seen from Fig. 8 where decreasing D from 1.00 (normal tension) to 0.91 (less tension) reduces the amplitude of VaVm although the amount of reduction in Fig. 8 is not as pronounced as the rise in Fig. 7 for cable tightening. It can be said that cable tightening under varying traffic tends to increase the product VaVm while cable loosening under varying traffic decreases the product VaVm that is beneficial.
Fatigue Crack Growth Rate of Runyang Bridge: Part I
217
Fig. 8 Product VaVm of cables versus position of cables for Case I (loosening)with D=0.91, 0.94, 0.97 and 1.00 under varying traffic. 2.3.2 Case II: cable tightening and loosening without traffic
Consider now Case II in Eq. (2) where the bridge is not under traffic while the tension in the cables can still vary that is accounted for by D as defined in Eq. (2). Numerical values of Va, Vm and VaVm for the 52 cables of the Runyang bridge with D=1.00, 1.04 and 1.12 are given in Tables A7, A8 and A9 of Appendix IV [9]. Case II refers to max. stress without traffic while Dt1 corresponds to more tension in the cables. It can be concluded from the results in Fig. 9 that tightening of the cable will now have a beneficial effect as the product VaVm will decrease when D is increased from 1.00 to 1.12 corresponding to “tightening”. Fig. 10 provides the results for loosening of the cables without traffic. This increases VaVm as D is decreased from 1.0 to 0.7. Therefore loosening of the cable is of no help in the absence of traffic. Numerical values of Va, Vm and VaVm for the 52 cables of the Runyang bridge with D=0.9 and 0.7 are given, respectively, in Appendix V of Tables A10 and A11 [9]. The results in Figs. 7 to 10 inclusive are summarized in Table 1. Table 1. Effect of cable tightening and loosening on VaVm with and without traffic. Cases Case I (traffic) Case II (no traffic)
VaVm
VaVm
Decrease (loosening) Decrease (tightening)
Increase (tightening) Increase (loosening)
218
G. C. Sih and X. S. Tang
Fig. 9 Product VaVm of cables versus position of cables for Case II (tightening) with D=1.00, 1.04, 1.08 and 1.12 in absence of traffic.
Fig. 10 Product VaVm of cables versus position of cables for Case II (loosening) with D=0.7, 0.8, 0.9 and 1.0 in absence of traffic.
Fatigue Crack Growth Rate of Runyang Bridge: Part I
219
3. Multiscale Micro/MacroCrack Model Multiscale crack growth models [79] must not only distinguish the size and time effects of small and large cracks but they must also be able to treat the transition region behavior of the cracks, say the transfer of microto macrocracking if only two scales are involved. Hence both the microand macroscale material properties must be considered in addition to micro and macrolength that must be differentiated. A dual scale model must contain at least three parameters d*, P* and V* such as d , * P micro , * V o (3) d* V P do Vf P macro in which d* is the normalized characteristic dimension compared to the micro length do. A comparison between the micro and macromodulus is reflected by P* while V* accounts for the ratio of the material restraining stress Vo to the applied stress Vf such that Vo/Vf must always be less than one. This corresponds to the threshold for the onset of crack growth. Such a behavior manifests the closing of the microcrack in contrast to the macrocrack that is defined to possess a macrodistance crack opening. The transition of microcracking to macrocracking can be essential in fatigue where the applied load switches repeatedly from tension to compression or vice versa for each cycle. 3.1 Fatigue crack growth of cable The bridge cable is a composite made of strands of steel wires wrapped in polymeric tubes with spacing filled by polymers. Although the properties of the cable will be obtained by approximation but they will be different from those for the wire. The details of which are discussed in [9]. It is more pertinent to consider the growth rate da/dN of a fatigue crack with length a (cm) in a cable as given by da \ (4) 0 and ED(V) > E0 for V < 0, as expected. In a first approximation, the differential Young’s moduli at the tensile and compressive peak stresses VT and VC can be evaluated from the slopes of the elastic curves immediately after stress reversal. With these two values, an optimal fit to eq. (3) yields E0 and k. Alternatively, the elastic unloadingreloading data can be evaluated to yield values of ED for the stresses from which the unloadings were performed. An optimal fit of these data to eq. (3) yields accurate values of E0 and k. For the example shown in Fig. 4, the following values were obtained: E0 = 88.6 r 0.3 GPa and k = 318 r 20 GPa [20]. Fig. 5 shows an example of the fit of the actually measured stress dependent values ED(V) to eq. (3) for the case of a bainitic variant of the roller bearing steel SAE 52100 [14]. Once the elastic data of the undamaged material are known, the development of fatigue damage can be followed continuously during the fatigue test by repeating the procedures described and noting the changes in ED(V), E0 and k compared with the values of the undamaged specimen. This will be explained in more detail in the examples to be discussed subsequently.
334
H. Mughrabi and H. W. Höppel
Fig. 4 Hysteresis curve of undamaged fatigued MMC AA6061Al2O315pT6, with elastic unloadings and reloadings. Note that the stress V is plotted against the plastic strain Hpl (obtained in the linear Hooke approximation), providing higher resolution. After [20].
Fig. 5 Stress dependence of differential Young’s modulus ED of a bainitic variant of the roller bearing steel SAE 52100, as a consequence of nonlinear elasticity effects. From [14].
Fatigue Damage of Heterogeneous Material
335
4. Examples of Assessment of Fatigue Damage Based on Changes of NonLinear Elastic Compliance 4.1 Fatigue damage in a particulatereinforced metalmatrix composite The study of fatigued particulatereinforced metal matrix composites is suitable to demonstrate the usefulness of compliance measurements and the assessment of the variation of the parameters E0 and k as a measure of the developing fatigue damage [17,18,20]. Figure 6 shows an example of such a study on the fatigued MMC AA6061Al2O320pT6 which contains a volume fraction fp = 20% of Al2O3 particles. The data refer to different values of the total strain amplitude 'Ht/2 in straincontrolled fatigue tests at half the fatigue life (N = Nf/2, where N is the number of cycles and Nf the number of cycles to failure). In the fatigued MMC studied, fatigue damage has been identified metallographically as the fracture of the particles, compare also [21], which occurs when the total strain amplitude 'Ht/2 exceeds a value of ca. 0.004. It is evident that, with increasing damage, E0 which is initially constant (97.9 GPa) loses its meaning as a material constant and starts to decrease as a result of the decreasing effective loadbearing cross section. In parallel, the elastic behaviour becomes increasingly more nonlinear. This is reflected in the fact that the magnitude of the parameter k which is initially constant (502 GPa) increases as the damage develops. In the case of MMCs, it is difficult to relate the changes in the nonlinear compliance quantitatively to the loss of the loadbearing cross section. One reason is that the Young’s moduli of the matrix ( 68 GPa) and the particles ( 380 GPa) differ very strongly. Another reason is that the damage is internal and distributed more or less homogeneously throughout the volume and not in the form of discrete cracks. As will be shown in the next section, the approach described can be applied more specifically and with better accuracy to materials in which the damage prevails in the form of cracks that are initially confined to the surface region and then propagate into the interior.
336
H. Mughrabi and H. W. Höppel
Fig. 6 Evolution of fatigue damage in particulatereinforced metalmatrix composite AA6061Al2O320pT6, shown the variation of the parameters Eo and k with increasing damage (particle fracture) as a function of total strain amplitude 'Ht/2 at half fatigue life, N = Nf/2. An increasingly nonlinear elastic behaviour (with increasing _k_) is found as the particles fracture at 'Ht/2 > 0.004. From [17].
4.2 Combined study of propagation of surface cracks in fatigued magnesium alloy AZ91 by replica techniques and compliance measurements In Section 2, the initiation and propagation of fatigue cracks in the cast magnesium alloy AZ91 had been discussed qualitatively. Here, it will be shown that the compliance technique introduced before lends itself to study in detail specific features of the crack propagation process in the alloy AZ91. This approach can be combined advantageously with the study of crack evolution at the surface by a suitable replica technique, as introduced in [22]. In that case, the fatigue test is interrupted repeatedly in order to take acetate replicas of the surface of the gauge length. Before viewing these replicas at fairly high magnification in a scanning electron microscope, a thin layer of gold is evaporated onto them in order to enhance the contrast and to provide electrical conductivity. By inspection of the sequences of replicas taken, one can then trace back from the fatal crack to the origin of microcrack nucleation and follow the process of crack coalescence and propagation as seen on the surface. Fig. 7 is an example showing the same location of the surface of a fatigued specimen of the alloy AZ91 with the main crack, as seen in two (composite) replicas taken after different
Fatigue Damage of Heterogeneous Material
337
numbers of cycles. From series of traces of the crack distribution in fatigued specimens of the alloy AZ91 it can be concluded how the main crack originated by a coalescence of a larger number of microcracks., as seen in the example shown in Fig. 8.
Fig. 7 Example of surface replicas taken from same location of fatigued magnesium alloy AZ91after different numbers of cycles. Plastic strain amplitude 'Hpl/2 = 9u 105, room temperature. After [6,11].
Fig. 8 Evolution of surface crack growth and coalescence in fatigued magnesium alloy AZ91, as obtained from successive replicas. Total strain amplitude 'Ht/2 = 5u 103, room temperature. From [6,11].
338
H. Mughrabi and H. W. Höppel
(a)Early in fatigue life; N/Nf  10%
(b)Later in fatigue life; N/Nf  80%
Fig. 9 Hysteresis loops of fatigued magnesium alloy AZ91. These are plots of stress V as a function of plastic strain in linear Hooke approximation. 'Ht/2 = 2.25 u 103, room temperature. After [6,11,12,15].
Complementary compliance measurements made during intermittent elastic unloadings and reloadings during a closed cycle reveal the loss of the loadbearing cross section and provide valuable additional information. This becomes evident when one compares the hysteresis loops with the unloadings/reloadings, as recorded early in fatigue life, see Fig. 9 (a), and near the end of fatigue life, shown in Fig. 9 (b). Early in the fatigue test, there is no influence from cracks. The slopes of the unloading/reloading paths are vertical in the limit of vanishing stresses and deviate marginally (to a large positive value) at higher tensile stresses and in the opposite sense at higher compressive stresses, as is typical of the intrinsic nonlinear elastic behaviour. Once cracks have developed and grown over a larger portion of the cross section, a completely different situation is observed which reflects the superposition of an appreciable additional nonlinear component due to the fatigue damage (Fig. 9 (b)). Now the slopes of the unloading/reloading paths deviate strongly and in opposite sense in the tensile and compressive phases of the cycle, respectively, from the initially vertical slope. The variation of the differential elastic modulus ED during the cycle can be evaluated (with appropriate values of the constants E0 and k) and plotted against the stress as shown in Fig. 10. In this figure, two important features can be recognized, namely the intrinsic stress dependence of ED when the cracks are closed (upper inclined line and dashed extension) and the stress dependence due to damage, when the (main) crack has opened in tension (lower inclined line). Moreover, there is a jump 'ED between the two lines which allows to recognize the transition
Fatigue Damage of Heterogeneous Material
339
from crack opening to crack closure (at ca. 25 MPa) and vice versa. Crack opening can be seen to occur at a tensile stress of about +12.5 MPa. This behaviour is appropriately described by the damage parameter 'ED/E0, as will be discussed next.
Fig. 10 Differential elastic modulus ED (stiffness), determined by intermittent elastic unloadings, see Fig. 9 (b), showing crack opening at ca. +12.5 MPa and crack closure at ca. 25 MPa. 'Ht/2 = 2.25 u 103, N/Nf  80%. After [6,11,12,15].
Fig. 11 Evolution of crack length (main crack) of fatigued magnesium alloy AZ91 at the surface (replicas) and in the bulk (see text), as derived from damage parameter 'ED/Eo. in different ways. After [6,11,12,15].
340
H. Mughrabi and H. W. Höppel
Based on the assumption that, after the initial stage of microcrack initiation, there is one main fatal crack, crack growth can be evaluated in different ways by assessing the length of the main crack as a function of the number of cycles. Data thus obtained are plotted in Fig. 11. The damage parameter 'ED/E0 is in good approximation proportional to the length of the surface crack, as determined from the replicas, up to about 80% of fatigue life, whereupon it deviates to higher values, as the crack propagates deeper into the material [6,11]. The continuous curve represents an automatic calculation of the damage parameter 'ED/E0 from the stiffness values at the tensile reversal points of the hysteresis loops (with 'ED computed according to eq. (5)). There is a remarkably good agreement between these values and those determined by the elastic unloadings/reloadings. In summary, it can be said that the compliance measurements, evaluated with appropriate consideration of the intrinsic nonlinear elastic properties, can yield detailed information on the crack propagation, including crack opening and crack closure stresses, in fatigued plain unnotched specimens of materials such as the cast magnesium alloy AZ91. Further complementary information can be obtained by combining the compliance technique with a replica study of the evolution of fatigue cracks at the surface. In closing, it is mentioned that a mesomechanical model has been developed which describes fatigue crack propagation and fatigue life of the alloy AZ91 very satisfactorily [23]. 5. Summary and Conclusions The studies discussed above lead to the following conclusions: x
x
x
The nonlinear compliance of a fatigued plain unnotched specimen includes contributions from the intrinsically nonlinear elastic material properties and from the damageinduced effects on the compliance. The intrinsic nonlinear elastic behaviour reflects the anharmonicity of the atomic potential. It can be assessed experimentally in cyclic deformation tests and evaluated in terms of the Young’s modulus in the limit of vanishing stresses and a parameter that characterizes the deviations from linearity at higher stresses. Compliance measurements, conducted on fatigued plain unnotched specimens and evaluated with appropriate consideration of the intrinsic nonlinear elastic properties, are a useful tool to monitor the evolution of fatigue damage. Thus, detailed information on crack propagation in fatigued plain unnotched specimens,
Fatigue Damage of Heterogeneous Material
x
x
x
341
including crack opening and crack closure stresses, can be obtained. The technique is particularly suitable to study fatigued materials in which one main fatal crack develops out of the initially large number of microcracks. The compliance technique can be combined advantageously with a replica study of the evolution of fatigue cracks at the surface to yield complementary information. The experimental approach described is novel and has the merit of providing crack growth data in a nondestructive manner during a standard straincontrolled fatigue test on a plain unnotched specimen without the need to use a standardized fracture mechanics specimen.
Appendix: Determination of differential Young’s modulus ED from slopes of elastic unloading curves in stress vs. plastic strain plots If the elastic unloading curve in the V vs. Hplplot (with plastic strain defined as previously, i.e. Hpl = Ht  V/Hel) has a stressdependent slope S(V) at a stress level V, then this slope is related to the differential elastic modulus ED(V) in the V vs. Htplot and the Young’s modulus E0 in the limit of vanishing stress as
1 SV
1 E D V
1 E0
(A1)
Resolving for ED(V), it follows that the stressdependent differential Young’s modulus can be derived from the slope S(V) by the relation
E D V
E 0 SV E 0 SV
(A2)
References [1] Saxena A. and Muhlstein CL. Fatigue crack growth testing.In: ASM Handbook,Vol. 19, Fatigue and Fracture, ASM International (1996) 168184. [2] Rroek D. Elementary Engineering Fracture Mechanics, Sijthoff & Noordhoff, Alphen aan den Rijn (1978) 316321.
342 [3]
[4] [5]
[6] [7] [8] [9] [10]
[11]
[12]
[13]
[14]
[15]
[16]
[17]
H. Mughrabi and H. W. Höppel Mayer HR. Lipowsky H. Papakyriacou M. Rösch R. Stich A. Zettl B. and TanzlTschegg S. Application of ultrasound for fatigue testing of lightweight alloys, Fatigue Fract Eng Mater Struct 22, (1999) 591599. Ting JC. and Lawrence FV. Modeling the longlife fatigue behavior of a cast aluminum alloy, Fatigue Fract Eng Mater Struct 16, (1993) 631647. Couper MJ. Neeson AE. and Griffiths JR. Casting defects and the fatigue behaviour of an aluminium casting alloy, Fatigue Fract Eng Mater Struct 13, (1990) 213227. Eisenmeier G. Holzwarth. Höppel HW. and Mughrabi H. Mater Sci Eng 319321 A, (2001) 578582. Murakami Y. Nomoto T. and Ueda T. Factors influencing the superlong fatigue failure in steels, Fatigue Fract Eng Mater Struct 22, (1999) 581590. Bathias C. There is no infinite fatigue life in metals, Fatigue Fract Eng Mater Struct 22, (1999) 559565. Mughrabi H. Specific features and mechanisms of fatigue in the ultrahigh cycle regime, Int J Fatigue 28, (2006) 15011508. Allison JE. Jones JW. Larsen JM. and Ritchie RO. Eds: Proceedings of 4th International Conference on Very High Cycle Fatigue (VHCF 4), TMS (The Minerals, Metals & Materials Society) (2007). Eisenmeier G. Ermüdungsverhalten der Magnesiumlegierung AZ91: Experimentelle Untersuchungen und Lebensdauervorhersage, Doctoral Thesis, Universität ErlangenNürnberg (2001). Eisenmeier G. Höppel HW. Ding HZ. and Mughrabi H. Ermüdungslebensdauer der Magnesiumlegierung AZ91: Experiment und Modellierung. In: DFG 2. Kolloquium Lebensdauervorhersage, Berlin, Deutscher Verband für Materialforschung und –prüfung e.V., (2002) 169178. Borbély A. Mughrabi H. Eisenmeier G. and Höppel HW. A finite element modelling study of strain localization in the vicinity of nearsurface cavities as a cause of subsurface fatigue crack initiation, Int. J. Fracture 115, (2002) 227232. Sommer C. Christ HJ. and Mughrabi H. Nonlinear elastic behaviour of the roller bearing steel SAE 52100 during cyclic loading, Acta Metall Mater 39, (1991) 11771187. Mughrabi H. Assessment of fatigue damage on the basis of nonlinear compliance effects. In: Handbook of Materials Behavior Models, Ed J. Lemaitre, Academic Press, (2001) 622632. Wasserbäch W. Nonlinear elastic behaviour and thirdorder elastic constants of a rollerbearing steel and some standard steels, Phys. Stat. Sol. (b) 164, (1991) 121125. Hartmann O. Biermann H. and Mughrabi H. Cyclic stressstrain and fatigue behaviour of particulatereinforced Almatrix composites. In: Low Cycle Fatigue and ElastoPlastic Behaviour of Materials, Eds K. T. Rie & P. D. Portella, Elsevier Science Ltd., (1998) 431436.
Fatigue Damage of Heterogeneous Material
343
[18] Biermann H. Kemnitzer M. and Hartmann O. On the temperature dependence of the fatigue and damage behaviour of a particulatereinforced metalmatrix composite, Mater. Sci. Eng A 319312, (2001)671674. [19] Mughrabi H. Some aspects of fatigue of engineering materials. In: Fracture Mechanics: Applications and Challenges, Invited Papers presented at the 13th European Conference on Fracture, ESIS Publication 26, M. Fuentes, M. Elices, A. MartinMeizoso, J. M. MartinezEsnaola, Eds, Elsevier, (2000) 1328. [20] Biermann H. Beyer G. and Mughrabi H. SpannungsDehnungsHyteresekurven wechselverformter Proben eines etallMatrixVerbundwerkstoffes. In: Verbundwerkstoffe und Werkstoffverbunde, Ed. G. Ziegler, DGM I nformationsgesellschaft, Oberursel, (1996) 197200. [21] Lloyd DJ. Aspects of fracture in particulate reinforced metal matrix composites, Acta Metall Mater 39, (1991) 5971. [22] Ebi G. Ausbreitung von Mikrorissen in duktilen Stählen, Doctoral Thesis, Rheinisch Westfälische Technische Hochschule Aachen (1987). [23] Ding HZ. Eisenmeier G. and Mughrabi H. A mesomechanical model of fatigue crack initiation and growth with application to the lowcycle fatigue life prediction of the cast magnesium alloy AZ91. In: Proceedings of Fourth International Conference FATIGUE 2000: Fatigue and Ductility Assessment of Materials, Components and Structures, Eds. M. R. Bache et al, EMAS Ltd, ( 2000) 209217.
Fatigue Crack Growth of Aircraft Aluminum Alloys Sp. G. Pantelakis1* and Al Th. Kermanidis2 1
Laboratory of Technology and Strength of Materials (LTSM) Department of Mechanical Engineering & Aeronautics University of Patras, 26500 Patras, Greece 2 Department of Mechanical and Industrial Engineering, University of Thessaly, 38334 Volos, Greece *Email:
[email protected] Abstract The microstructural characteristics and the influence of existing corrosion on fatigue crack growth in 2024 T351 aircraft aluminium alloy are investigated. Examined is the elongated grain morphology due to the rolling process that exhibited higher crack growth resistance than the microstructure of the sheet material with smaller equiaxed grains. Moreover, plate microstructure with high purity composition offered better damage tolerance characteristics in contrast to the conventional sheet microstructure.Shown is the need to account for the influence of preexisting corrosion on the aluminum alloys in order to obtain more reliable results from fatigue and damage tolerance analyses of components with corroded areas. 1. Introduction Damage tolerance analyses and reliable prediction of crack growth under fatigue loading rely heavily on experimental data and the comprehensive understanding of the underlying crack growth mechanisms. Fatigue damage in the material can be divided into a number of subsequent phases characterized by cyclic slip, crack nucleation, microcrack growth and macrocrack growth up to the final material failure. The different physical processes, which prevail in the gradual fatigue damage accumulation during the fatigue life of a metallic component, are complex and interrelated. They develop with increasing number of fatigue cycles from atomic to macroscale damage mechanisms and also entail a host of material, geometric and loading parameters [1]. Their interaction cannot be easily assessed in quantitative terms. Mechanistically, the fatigue damage phases mentioned above may be summarized in the crack initiation and crack growth stage, with the latter starting once cracks become visible. Different quantities are essential to assess crack initiation or crack growth respecG.C. Sih (ed.), Multiscale Fatigue Crack Initiation and Propagation of Engineering Materials: Structural Integrity and Microstructural Worthiness, 345–366. © Springer Science+Business Media B.V. 2008
346
Sp. G. Pantelakis and Al Th. Kermanidis
tively. For crack initiation relevant is the severity of stress concentration. Material properties and loading conditions control principally the behaviour of long cracks. Crack growth is dominated by the intensity of the cracktip stress distribution. The volume energy density criterion, [24], which first has been used to predict failure initiation under monotonic loading, can also be applied to predict crack initiation and crack growth under cyclic loading. It assumes that failure occurs in a critical element when the volume energy density reaches a certain threshold. The crack initiation model in [2] applies also to crack propagation [3,4], because attention is focused on a material element in a specimen without initial crack or in a local region ahead of a preexisting crack. According to the crack closure theory [5], crack growth is dependent to crack closure, which is correlated to several features, such as fracture surface roughness, residual plasticity in the wake or ahead of the crack tip, oxide debris etc. Herein, the role of microstructure and material properties ahead of the crack tip is important. For instance, fracture surface roughness is correlated to the grain morphology of the alloy; the amount of residual plasticity in the wake of the crack is dependent on the material’s yield stress. The same property influences crack growth retardation induced by the occurrence of an overload. While these aspects are important in the development of damage tolerance analysis tools, the availability of sufficient experimental data is a prerequisite. In the present chapter experimental fatigue crack growth data for selected aircraft aluminum alloys are presented and discussed with the support of metallographic analyses. The work presented, resulted from two extensive studies. In the first study the effect of variation in microstructure of the 2024 T351 alloy due to the aluminum product form (sheet or plate) as well as the purity content (FeSi content) of the alloy on the fatigue crack growth were investigated [6]. In the second study the fatigue crack growth behaviour of precorroded 2024 T351 alloy was investigated and discussed under the view of a synergetic effect of corrosion and corrosioninduced hydrogen embrittlement [7]. 1.1 Aircraft aluminum alloys Aluminum alloys are the primary material for aircraft structures since 1930. Despite the increasing use of advanced polymer matrix composites in aircraft structures, aluminum alloys remain the main choice for fuselage, wings and supporting structure of commercial airliners. High specific properties, superior damage tolerance behaviour and good corrosion resistance along with well known performance characteristics, design experi
Fatigue Crack Growth of Aircraft Aluminum Alloys
347
ence and established manufacturing methods represent the main reasons for the continued wide use of aluminum alloys in modern aircrafts. The 2xxx, 6xxx and 7xxx aluminum series as well as some AlLi alloys enjoy the widest use in aircraft structural applications. The 2xxx series alloys contain copper as the primary alloying element, which produces high strength but reduced corrosion resistance. The 2024 alloy is probably the most widely used alloy in aircraft applications. The lower yield stress of the 2xxx series alloys compared to the 7xxx series is compensated by improved damage tolerance, thus making this alloy series the first choice for damage tolerant primary structure applications. The 2xxx series alloys are not easily weldable but new alloy types along with advanced welding technologies make welding of these alloys manageable. The 6xxx series contains magnesium and silicon, which form the magnesium silicide (Mg2Si). The alloys of this series offer a good balance between corrosion resistance and strength along with a good weldability. The most popular alloy of the 6xxx series for use in aircraft applications is the 6061. In the 7xxx group the primary alloying element is zinc. In this group two types of alloys exist: the aluminum –zinc –magnesium alloys and the aluminum – zincmagnesiumcopper alloys, with the second type being less corrosion resistant. This series includes some of the most high strength aluminum alloys such as 7075 and 7178, which are exploited for aircraft frames and structural components. All above mentioned aluminum alloy series are heat treatable. Aluminum –Lithium alloys are attractive for lightweight aircraft applications due to the element Lithium, which is the lightest metallic element. They are often alloyed with copper, magnesium, zirconium and other elements to improve properties. They have been used in limited applications so far (2090 and 8090 are typical alloys used) mainly due to low corrosion resistance and anisotropic behaviour. New weldable AlLi alloys of the 2xxxseries (copper being the greatest alloying element) seem to be attractive for further applications. 2. Microstructural Effects on Fatigue Crack Growth It is known that microstructural features influence fatigue crack growth in the near threshold (low ¨Ȁ) regime where the slip characteristics are significant [8]. In the low ǻȀ regime crack growth has been found to be sensitive to crack closure, namely plasticity induced crack closure, corrosion oxide closure and surface roughness crack closure [5, 913]. In [14] the
effect of sheet/plate microstructure on the 2090 aluminum–lithium
348
Sp. G. Pantelakis and Al Th. Kermanidis
alloy on fatigue crack growth in the near threshold region has been demonstrated. At low ǻȀ values in the order of 1010 m/cycle the sheet material exhibits significantly higher crack growth rates compared to the plate material. In the crack growth region corresponding to medium ¨Ȁ values, the crack plane becomes normal to the applied nominal stress and crack growth sensitivity on microstructure is considered to be less significant. Nevertheless, a correlation between microstructural features and closure mechanisms in long crack growth behaviour of aluminum alloys seems to exist. Specifically, surface roughness induced closure (RICC) mechanisms have been found to influence Stage II fatigue crack growth rates [1011, 1415]. The closure mechanisms have been attributed to grain morphology characteristics. Additionally, crack deflection and consequent crack closure from wedging of fracturesurface asperities, which are related to variations in the degree of recrystallization, grain morphology and texture (evident between sheet and plate product forms) may increase the crack growth resistance of the material [14]. When fatigue load interaction effects are present the complex damage accumulation phenomena make a correlation between fatigue crack growth mechanisms and microstructure even more difficult. Suresh argued in [16] that the postoverload crack propagation behavior is influenced by microstructure as well as crack tip/grain boundary interactions. In the same work it is reported that surface roughness may lead to sustained crack growth retardation following the application of overloads by reducing the effective stress intensity range. However limited data can be found in the open literature on the postoverload fatigue crack response of the same alloy with variation in microstructure. This work will first discussed the influence of variations in microstructure resulting from sheet and plate product form, as well as from variations in purity composition (FeSi content), on the long crack growth behaviour of the conventional 2024 T351 aluminum alloy is presented. The experimental results provide evidence that the effect of microstructural features (e.g. grain size and morphology) can influence the medium ǻȀ fatigue crack propagation, which is of high technological interest for damage tolerant wrought aluminium alloys design. 2.1 Material The material used in the experimental investigation was aluminum alloy 2024 T351 in plate and sheet product configuration with a thickness of 15 and 3.2 mm respectively. Both plate and sheet materials were tested in
Fatigue Crack Growth of Aircraft Aluminum Alloys
349
conventional and high purity (HP) composition, which refers to the 2024 material with reduced Ferich and Mg2Si phases. The volume fractions of the respective phases are given in Table 1 for HP and reference material. In Figure 1 micrographs of the grain structure of the materials used in the present investigation are shown [6]. The grain morphology obtained for the plate and sheet product is the result of the different degree of rolling process in order to achieve the required thickness (15mm and 3.2 mm respectively). As a result a different grain microstructure was obtained which corresponds to larger, elongated grains for the plate materials compared to the fine equiaxed grains in the sheet microstructure.
(a) AA2024
(b) AA2024
(c) 2024HP
Fig. 1 Micrographs showing grain morphology in the materials investigated [6].
Grain size measurements in terms of equivalent circle diameter in planes LST, LTST and LLT are displayed in Table 2. The average grain size in the plate material was noticeably larger in all3 planar dimensions measured exhibiting a coarse and elongated microstructure compared to the finer equiaxed grain structure in the sheet material. The largest grain sizes were measured in the plate with high purity composition, which for the case of the LLT planar dimension reaches 700µm. The respective value for the sheet high purity alloy was 30 µm. Table 1 Calculated volume fractions of Ferich and Mg2Si phases in reference and HP material [6]
Phase Ferich Mg2Si balance
2024 plate 1 0.16 1.16
HP plate 0.5 0.06 0.56
2024 sheet 1.26 0.22 1.48
HP sheet 0.65 0.13 0.78
350
Sp. G. Pantelakis and Al Th. Kermanidis Table 2 Average planar grain size measured in the four alloys [6].
2024HP sheet 2024 plate 2024 HP plate 2024 sheet
Plane direction and circle equivalent diameter (µm) LST LTST LLT average 18,3 18,2 28,5 21,2 49,4 48,3 101,1 62,3 175,0 96,0 349,0 180,3 97,0 62,0 707,0 162,0
2.2 Fatigue testing, results and fractographic observations The fatigue tests carried out were constant amplitude fatigue crack growth tests as well as constant amplitude fatigue crack growth experiments including single and periodic tensile overloads. For the fatigue crack propagation experiments center cracked specimens of 3.2 mm thickness were machined according to ASTM E647 standard [17]. To avoid thickness effects in the investigation specimens were cut from the midplane of the plate product and were machined to the required thickness of 3.2 mm. The fatigue crack growth experiments performed are summarized in Table 3. Table 3 Summary of fatigue crack growth tests.
Constant Amplitude Tests Material Maximum stress ımax (MPa) 2024HP sheet 130 2024 plate 130 2024 HP plate 130 2024 sheet 130 Tests with single overload Material Stress Ratio R=ımin/ ımax 2024HP sheet 0.1 2024 plate 0.1 2024 HP plate 0.1 2024 sheet 0.1 Tests with periodic overloads Material Stress Ratio R=ımin/ ımax 2024HP sheet 0.1 2024 sheet 0.1
Frequency (Hz)
Stress Ratio R=ımin/ ımax
Overl.ratio ıov/ ımax
25 25 25 25
0.1 0.1 0.1 0.1
1.6 1.6 1.6 1.6
Overl.ratio ıov/ ımax 1.6 1.6 1.6 1.6
Crack length at overload (mm) 8.5,11(2 tests) 9,11(2 tests) 10,12(2 tests) 7.5
Overl.ratio ıov/ ımax 1.6 1.6
Crack length at overload (mm) 6.5, 8, 10 6.5, 7.5, 10
Fatigue Crack Growth of Aircraft Aluminum Alloys
351
Fig. 2 Constant amplitude fatigue crack growth results.
In Fig. 2 constant amplitude fatigue crack propagation curves of the materials tested are displayed in terms of half crack length versus stress intensity factor range. The higher crack growth resistance for specimens taken from plate product is reflected through the lower crack growth rates compared to the sheet material in the medium ¨Ȁ region (1030 MPam1/2). For both rolling products the material with high purity composition exhibited superior crack growth behaviour in the mentioned ǻȀ region. Optical micrographs of the fractured specimen surfaces with plate microstructure revealed increased roughness and discontinuities along the crack path direction (Fig.3). The surface roughness was evaluated by means of the surface profile parameter RL according to the ASM guidelines [18]. RL values measured for plate specimens were higher compared to the sheet material. The RL values measured at specific segments taken at the same crack path location for plate and sheet 2024 material were RLPLATE =1.18 and RLSHEET =1.07 respectively (Fig. 4).
(a) Sheet
(b) Plate material
Fig. 3 Micrographs showing segments of the free edge of fractured surfaces at the same location of crack propagation with different degree of surface roughness.
352
Sp. G. Pantelakis and Al Th. Kermanidis
Fig. 4 Profile roughness parameter for sheet and plate material.
The obtained response under constant stress amplitude may be correlated to pronounced crack closure effects of specimens with plate microstructure due to increased surface roughness, which produces pronounced crack surface contact. The above observation is in agreement with results reported in [1415,19]. The increased surface roughness along the crack path direction is promoted by the coarse and elongated grain morphology, as a result of the different rolling process involved. Macroscopic fractographic examination revealed a fractured surface region perpendicular to the load followed by shear fracture (Fig. 5). For all materials tested double shear lips are evident along the fracture path.
Fig. 5 Fractured surfaces macrographs of different materials subjected to constant amplitude fatigue tests.
Fatigue Crack Growth of Aircraft Aluminum Alloys
353
As shown in Fig. 6 in the case of the plate product the fractured surface region which is perpendicular to the load is smaller and the developed shear lips are wider in comparison to the sheet material. On the fracture surfaces of the plate materials pronounced black debris could be observed, which according to [20] could be evidence of increased lower and upper crack surfaces contact during fatigue crack growth. By careful examination of fractured surfaces in Fig. 6 it can be observed that crack surface contact marks are more pronounced on the shear lips of plate material specimens. The described mechanism can lead to increased crack closure. In order to assess the fatigue crack retardation response following application of overloads, constant stress amplitude fatigue crack growth experiments including single and periodic tensile overloads were carried out. The testing parameters were the same as in the previous tests. The applied overload ratio was ıov/ımax= 1.6, while application of overload was performed at similar ǻȀ levels (at approximately 20 MPam1/2). From the experimental crack growth curves obtained (Figs. 67) it was observed that crack growth rates measured at comparable ¨Ȁ levels in the post – overload stage were lower in the specimens with plate microstructure. The post overload crack growth behaviour observed is consistent with the results obtained in the constant amplitude crack propagation curves showing an increased crack growth resistance for the plate microstructures both in the prior and post overload stage. Figures 8, 9 and 10 are showing a sustained retardation of the alloy with high purity composition for the case of single and periodic overloads. Micrographs of fracture surfaces of the specimens subjected to tensile overloads revealed similar characteristics to the constant amplitude tests in terms of shear lip development and surface
(a) Crack length
(b) Crack growth rate
Fig. 6 Crack length and fatigue crack growth rates after tensile overload for sheet and plate material.
354
Sp. G. Pantelakis and Al Th. Kermanidis
(a) Crack length
(b) Crack growth rate
Fig. 7 Crack length and fatigue crack growth rates after tensile overload for sheet and plate material.
(a) Crack length
(b) Crack growth rate
Fig. 8 Crack length and fatigue crack growth rates after tensile overload for sheet and plate material.
(a) Crack length
(b) Crack growth rate
Fig. 9 Crack length and fatigue crack growth rates after tensile overload for conventional and HP sheet material.
Fatigue Crack Growth of Aircraft Aluminum Alloys
355
roughness. In the case of single and multiple overloads the load interaction phenomena present lead to significant plasticity effects. Thus, crack growth mechanisms become more complex and the results obtained cannot be discussed solely under the viewpoint of pronounced crack closure effects due to fracture surface characteristics.
(a) Crack length
(b) Crack growth rate
Fig. 10 Crack length and fatigue crack growth rates after periodic tensile overload for conventional and HP sheet material
3. Effect of existing corrosion damage on Fatigue Crack Growth It is without doubt that the Aloha Airlines accident in 1988 showed the global aviation industry the dangers of the structural degradation of aging components. In the years that followed intensive investigations have shown that the occurrence of corrosion appreciably degrades the mechanical performance of aluminum alloys [e.g.21]. Corrosion damage of aluminum alloys has been classically attributed to the complex process of oxidation. In recent years experimental efforts on a series of aircraft alloys have provided evidence that corrosion is also the cause for diffusion controlled material hydrogen embrittlement [2129]. This hydrogen embrittlement phenomenon is reflected into an appreciable reduction of tensile ductility of the corroded material areas [2122,28–29]. The hydrogen embrittlement process is explained in [30] through a hydrogen induced local microplasticity. Both processes, corrosion and hydrogen embrittlement, are diffusioncontrolled, hence the degradation of the material’s mechanical performance is expected to occur in local scale. However at present there are neither experimental data nor an established methodology for assessing the values of the local material properties of the corroded areas of the material. Notice that experimental investigations on the interaction of corrosion and fatigue usually refer to fatigue and fatigue crack growth tests which are performed in a certain corrosive environment [31
356
Sp. G. Pantelakis and Al Th. Kermanidis
32] and not to tests performed on precorroded material whereby, the latter represents a different and, for a series of practical cases in older airplanes, more relevant situation. Structural degradation due to existing corrosion has been considered as a load capacity decrease of the structural component [33]. Furthermore, it has been recognized that the occurrence of corrosion facilitates the onset of fatigue cracks [3435] and, hence causes the decrease in fatigue life due to corrosionpitting damage [34], as well as multisite damage scenarios from corrosion pits [35]. In Figure 11 the SN curves of uncorroded and precorroded 2024 T351 aluminum alloy specimens are displayed [36]. The results reveal the essential degradation of fatigue life in the corroded coupons as a result of premature onset of crack initiation due to corrosion pits. The degradation is reflected in a significant decrease in the material’s fatigue limit of the order of 28.5 % compared to the uncorroded material.
Fig.11 SN curves of uncorroded and precorroded 2024 T351 aluminum alloy specimens
On the other hand, the effect of prior corrosion damage on the fatigue crack growth behaviour of aircraft structures is presently disregarded and a few experimental data exist correlating the effect of prior corrosion on the fatigue crack growth rate [37]. The fatigue and damage tolerance behaviour of precorroded 2024 T351 aluminum alloy specimens is presented and discussed under the viewpoint of a synergetic effect of corrosion and corrosioninduced hydrogen embrittlement. The results demonstrate the essential effect of existing corrosion on the fatigue and damage tolerance behaviour of the 2024 alloy, as well as the need to account for the effect of corrosion on the mechanical proper
Fatigue Crack Growth of Aircraft Aluminum Alloys
357
ties in fatigue and damage tolerance analyses of the corroded areas of a structure. 3.1 Experimental procedure, testing and results The experiments were conducted on bare 2024 T351 aluminium alloy of 1.6 mm thickness. The performed experiments included fatigue crack growth tests for different stress ratio R on corroded and uncorroded material. An overview of the performed tests is given in Table 4. ȉhe selected fatigue stress ratios were R=ımin/ımax 0.01, 0.1, 0.5 țĮȚ 0.7 and the test frequency 20 Hz. In order to evaluate the Reffect the stress range ǻı was kept constant at a ımax between 101 and 180 MPa. Machining of the specimens was made according to ASTM E 64793 specification. All specimens were cut in longitudinal (L) orientation relative to the rolling direction. The experimental investigation included uncorroded and precorroded specimens in exfoliation corrosion environment for 36 hours according to ASTM standard G3490 [38]. Exfoliation corrosion environment has been selected as the environment that satisfactory simulates the effect of long duration outdoor corrosion exposure on the material’s mechanical properties [34]. After exposure, the specimens were cleaned according to ASTM G3490. During all fatigue crack growth tests crack growth was recorded via a DC Potential Drop measurement method. Table 4 Summary of fatigue crack growth tests. Corrosion exposure
Stress Ratio R=ımin/ ımax
Frequency (Ǿz)
Max. stress ımax (MPa)
none
0.01
20
109
2
EXCȅ 36 hrs
0.01
20
109
2
none
0.1
20
101
2
EXCȅ 36 hrs
0.1
20
101
2
none
0.5
20
180.4
2
EXCȅ 36 hrs
0.5
20
180.4
1
none
0.7
20
176.1
2
EXCȅ 36 hrs
0.7
20
176.1
2
No. tests
358
Sp. G. Pantelakis and Al Th. Kermanidis
The fatigue crack growth results are summarized in Tables 57 and Figs. 1216. In Table 5 the values of ǻȀ and Ȁmax referring to the critical crack length are given. Calculation of ǻȀ and Ȁmax was made with implementation of the equation [17]: K EV SD (1) In the interpretation of results the effect of corrosion on the correction factor ȕ in Eqn. (1) was not taken into account. In Table 6 the number of cycles corresponding to specimen failure are displayed together with the critical crack length Įcr defined at a time step that corresponds to 3 seconds prior to specimen failure. The critical crack length was defined in this manner because of the unfeasibility due to the data recording frequency of measuring the actual value at fracture. The critical crack length corresponds to the last data point of the curves in Figs. 12a15a. Table 5 ǻȀ țĮȚ Kmax values at critical crack length. Stress int. factor Max. stress int. Corrosion Stress ratio range ǻK (at Įcr ) factor Kmax (at Įcr) exposure R=ımin/ımax [ MPa m ] [ MPa m ] none 0.01 29.74 30.04 ǼXCO 0.01 22.87 23.09 none 0.1 32.54 36.16 ǼXCO 0.1 25.28 28.09 none 0.5 38.74 77.48 ǼXCO 0.5 16.94 33.88 none 0.7 11.70 40.32 ǼXCO 0.7 11.25 37.54
Table 6 Fatigue crack growth data of corroded and uncorroded specimens. Corrosion exposure
Stress ratio R=ımin/ımax
Max. stress (MPa)
None
0.01
109
ǼXCO 36 hrs
0.01
109
None
0.1
101
ǼXCO 36 hrs
0.1
101
None
0.5
180.4
Fatigue life Nf (cycles(mean values)
Critical crack length Įcr (mm(mean values)
46640/47460 (47050) 42700 (42700) 81620/69100 (75360) 58640/51960 (55300) 43960/49820 (46890)
20.02/16.46 (18.24) 12.59 (12.59) 24.8/23.2 (24.0) 15.59/21.31 (18.45) 19.4/35.73 (27.56)
Fatigue Crack Growth of Aircraft Aluminum Alloys
ǼXCO 36 hrs
0.5
180.4
None
0.7
176.1
ǼXCO 36 hrs
0.7
176.1
30560/29560 (30060) 213540 (213540) 139880/121260 (130570)
359
9.72/10.92 (10.32) 14.17 (14.17) 11.75/13.67 (12.71)
Table 7 Paris coefficients of corroded and uncorroded material. Mean Corrosion Stress ratio n C Mean value value exposure R=ımin/ımax 11 0.01 3.09 7.38*10 3.13 4.69*1011 3.16 2.0*1011 0.1 3.35 5.56*1011 3.21 9.38*1011 3.07 1.32*1010 none 0.5 3.0 1.94*1010 3.12 1.60*1010 3.23 1.26*1010 0.7 3.6 9.25*1011 3.6 9.25*1011 0.01 2.85 4.88*1011 2.85 4.88*1011 0.1 3.16 1.62*1010 3.11 1.5*1010 3.05 1.38*1010 ǼXCO 36 hrs 0.5 3.04 2.38*1010 3.21 4.37*1010 3.38 1.99*1010 0.7 3.16 5.03*1010 2.9*1010 3.47 3.78 7.61*1010
In Figs. 1216 the fatigue crack growth curves together with the crack growth rate measurements versus stress intensity factor range ǻȀ are displayed for the corroded and uncorroded specimens at different stress ratios.
360
Sp. G. Pantelakis and Al Th. Kermanidis
(a) Crack length
(b) Crack growth rate
Fig. 12 Crack length and fatigue crack growth rates of corroded and uncorroded specimens at R=0.01.
(a) Crack length
(b) Crack growth rate
Fig. 13 Crack length and fatigue crack growth rates of corroded and uncorroded specimens at R=0.1.
(a) Crack length
(b) Crack growth rate
Fig. 14 Crack length and fatigue crack growth rates of corroded and uncorroded specimens at R=0. 5.
Fatigue Crack Growth of Aircraft Aluminum Alloys
(a) Crack length
361
(b) Crack growth rate
Fig. 15 Crack length and fatigue crack growth rates of corroded and uncorroded specimens at R=0.7.
(a) Uncorroded
(b) Corroded
Fig. 16 Fatigue crack growth rates of specimens at R=0.01, 0.1, 0.5, 0.7.
From the obtained results the deteriorating effect of corrosion on fatigue life of precorroded specimens is revealed for all stress ratios examined. Fatigue life reduction, corresponding to fatigue crack propagation cycles, which as expected is promoted by the existence of localized corrosion sites acting as stress concentration locations, is ranging from 12% (R=0.01) to 38.8% (R=0.7). The effect of corrosion on fatigue crack propagation is more pronounced for small values of R. The observed behaviour can be explained by considering the mechanisms of partial embrittlement of the specimens as a result of corrosion exposure. For small values of ǻȀ damage accumulation mechanisms seem not to be influenced to the same degree by the partially embrittled material. At higher tensile stresses (higher ǻȀ values) embrittlement may have a more pronounced effect in the ability of the material to deform plastically ahead of the crack tip.
362
Sp. G. Pantelakis and Al Th. Kermanidis
By examining Table 6 the effect of corrosion damage on the critical crack length to failure is illustrated. The critical crack length of the corroded specimens is reduced by a magnitude of 45% compared to the respective value of the uncorroded specimens, while the stress intensity factor values corresponding to Įcr is reduced by 34% with regard to the uncorroded material. The stress intensity factor reduction is attributed to the reduction of the critical crack length due to fracture toughness degradation of the corroded alloy. From the experimental findings obtained in Figs. 1216 it can be concluded that the crack propagation resistance at high ǻȀ values suffers a significant degradation compared to the medium ǻȀ region where corrosion attack does not have the same impact. The latter observation is supported by the calculated differences in the coefficients of the Paris equation. The differences in the coefficients for the corroded and uncorroded specimens, derived from the da/dN–ǻK plots for stress intensity ranging from 10– 18 MPa m1/2 are compared in Table 7. The coefficients do not differ appreciably. This is consistent with the results in [35]. At stage III crack growth (high ǻȀ), the calculated crack growth rates are high and cannot be described by the Paris law. At this stage Paris equation cannot assess the influence of corrosion on fatigue crack growth. The obtained decrease in fatigue life of corroded specimens is attributed to the reduction of the critical crack length at failure. The latter is dependent on the material’s fracture toughness. These parameters are influenced by the partially embrittled material due to corrosion. The fatigue crack growth behaviour described above is not easy to explain by means of the classical interpretation of corrosion. Fractographic analyses performed in [29] on 1.6 mm thick specimen subjected to exfoliation corrosion exposure for 24 h confirm the embrittlement of the material during the corrosion exposure. The fracture surface appearance varies from the specimen surface to the specimen interior. At the specimen surface the fracture is intergranular as shown in Fig. 17. Immediately below there is a zone of quasicleavage fracture and further below the fracture turns to entirely ductile (dimples) as shown in Fig. 17. The results underline the need to consider the fatigue crack growth behaviour of corroded 2024 as the result of the synergetic effect of corrosion and corrosion induced hydrogen embrittlement.
Fatigue Crack Growth of Aircraft Aluminum Alloys
363
Specimen surface Intergranular
Quasicleavage
D
til f
Fig. 17 Local embrittled areas in corroded 2024 specimens.
4. Concluding Remarks The fatigue crack growth behaviour of 2024 T351 aircraft aluminium alloy (i) with variation in microstructural characteristics and (ii) under the influence of existing corrosion damage has been investigated. The experimental findings concerning the microstructural effects on fatigue crack growth revealed the following: (1) The effect of microstructural features (e.g. grain size and morphology), as well as variations in purity composition can influence fatigue crack propagation in the medium ǻȀ region, which is of high technological interest for damage tolerance design. (2) Plate microstructure with elongated grain morphology induced by the rolling process exhibited higher crack growth resistance than the microstructure of the sheet material with smaller equiaxed grains. This behaviour could be attributed to pronounced roughness induced crack closure effects in the plate microstructure. (3) The experimental results showed that the plate microstructure with high purity composition provides better damage tolerance characteristics compared to the conventional sheet microstructure. With regard to the effect of existing corrosion on the fatigue crack growth the following conclusions can be made: (4) The synergetic effect of corrosion and corrosioninduced hydrogen embrittlement resulted in an appreciable decrease in fatigue resistance and damage tolerance of the corroded material. (5) The experimental results have demonstrated the need to account for the influence of preexisting corrosion on the material’s properties for the reliable fatigue and damage tolerance analyses of components involving corroded areas.
364
Sp. G. Pantelakis and Al Th. Kermanidis
References [1] [2]
[3] [4]
[5] [6] [7]
[8] [9] [10]
[11]
[12]
[13] [14]
[15]
[16] [17]
Suresh S. Fatigue of Materials, second ed., Cambridge University Press, 1998, ISBN 0521578477, 700 pages Sih GC. and Chao CK. Failure initiation of unnotched specimens subjected to monotonic and cyclic loading, Theor. Appl. Fract. Mech. 2(1), (1984) 6773 Sih GC. and Moyer ET. Jr., Path dependent nature of fatigue crack growth, Inter. J. Eng. Fract. Mech. 7, (1983), 269280 Sih GC.and Chao CK. Influence of load amplitude and uniaxial tensile preties on fatigue crack frowth, Theor. Appl. Fract. Mech. 2(3), (1984) 247257 Elber W. Damage Tolerance in Aircraft Structures, ASTM Spec. Tech.Publ.486, (1981) 230 Investigation on Damage Tolerance Behaviour of Aluminum Alloys, IDA,European Project, Project No: GRD200140120, Final Report (2005) Kermanidis AlTh. Effect of Corrosion on the Structural Integrity of Lightweight Aircraft Structures, PhD Thesis, University of Patras, Department of Mechanical and Aeronautical Engineering, Patras, Greece, (2003) Garrett GG. and Knott JF. Crystallographic Fatigue Crack Growth in Aluminum Alloys, Acta Metallurgica, 25, (1975) 841849 Suresh S. and Ritchie RO. Metall. Trans. A, 13, (1982) 1627 Zaiken E. and Ritchie RO. Effects of Microstructure on Fatigue Crack Propagation and Crack Closure Behavior in Aluminum Alloy 7150 Materials Science and Engineering, 70 (1985) 151160. E. Zaiken E. and Ritchie RO. On the Location of Crack Closure and the Threshold Condition for Fatigue Crack Growth, Scripta Metallurgica, 18 (1984) 847850 Tzou JL.Suresh S. Ritchie RO. Fatigue Crack Propagation in Oil Environments. 1 Crack Growth Behaviour in Silicone and Parafin Oils, Acta Metall. 33 (1) (1985) 105116 Minakawa K. and McEvily AJ. On Crack Closure in the near Threshold Region, Scripta Metallurgica, 15 (1981) 633636 Venkateswara KT. Rao RJ. Bucci KV. Jata. and Ritchie RO. A comparison of fatigue crack propagation behavior in sheet and plate aluminumlithium alloys, Materials Science and Engineering, A141 (1991) 3948 Henk F. and Jong De. Thickness Direction Inhomogeneity of Mechanical Properties and Fracture Toughness as observed in Aluminum 7075 T651 Plate Material, Enginneering Fracture Mechnanics 13 (1980) 175192 Suresh S. Micromechanisms of fatigue Crack Growth Retardation Following Overloads, Engineering Fracture Mechanics 18. (3) (1983) 577593, ASTM E64793, Standard Test Method for Measurement of Fatigue Crack Growth Tests, Annual Book of ASTM Standards, Metals –Test Methods and Analytical Procedures, Section 3, Vol. 03.01, MetalsMechanical Testing; Elevated LowTemperature Tests; Metallography, (1994)
Fatigue Crack Growth of Aircraft Aluminum Alloys [18] [19] [20] [21]
[22]
[23]
[24] [25]
[26] [13]
[27]
[28]
[29]
[30] [31]
365
ASM Handbook, Volume1 2, Fractography, The Materials Information Society, (2000) Pao PS. Cooley LA. Imam MA. And Yoder GR. Fatigue Crack Growth in 2090 AlLi Alloy, Scripta Metallurgica, 23, (1989) 14551460 Schijve J. Fatigue Cracks, Plasticity Effects and Crack Closure, Four Lectures on Fracture Mechanics, 1l. No. 1L, (1978) Pantelakis SpG. Vassilas NI. and Daglaras PG. Effects of corrosive environment on the mechanical behaviour of the advanced Al–Li alloys 2091 and 8090 and the conventional aerospace alloy 2024, Metall, 47 (1993) 135–141. Pantelakis SpG. DaglarasPG. and Apostolopoulos ChAlk. Tensile and energy density properties of 2024, 6013, 8090 and 2091 aircraft aluminum alloy after corrosion exposure, J. Theor. Appl. Fract. Mech. 33 (2000) 117– 134 Papanikos P. and Kermanidis AlTh. Effect of corrosioninduced hydrogen embrittlement on the fracture toughness of 2024T3 aluminum alloy, in: Proceedings of the 4th International Conference on New Challenges in Mesomechanics, Aalborg University, Denmark, (2002) Smiyan OD. Coval MV. and Melekhov RK. Local corrosion damage of aluminum alloys, Soviet Mater. Sci. 19 (1983) 422 Tuck CDS. Evidence for the formation of magnesium hydride on the gra boundaries of Al–Zn–Mg alloys during their exposure to water vapour, in: Proceedings of the Third International Conference of Hydrogen on the Behavior of Materials, Jackson, Wyoming, (1980) 503– 511 Scamans GM. R. Alani R. and Swann PR. Preexposure embrittlement andstress corrosion failure in Al–Zn–Mg alloys, Corros. Sci. 16 (1976) 443 E. Charitidou E. Papapolymerou G, Haidemenopoulos GN. Hassiotis N. and Bontozoglou HV. Characterization of trapped hydrogen in exfoliation corroded aluminium alloy 2024, Script. Mater. 41 (1999) 1327 Haidemenopoulos GN, Hassiotis N, Papapolymerou G. and Bontozoglou HV. Hydrogen absorption into aluminum alloy 2024T3 during exfoliation and alternate immersion testing, Corrosion 54 (1998) 73 Petroyiannis PV. Kermanidis AlTh. Papanikos P. and Pantelakis SpG, Corrosioninduced hydrogen embrittlement of 2024 and 6013 aluminium alloys, Special issue: Al.Th. Kermanidis et al. / Theoretical and Applied Fracture Mechanics 43 (2005) 121–132 131 mesofracture mechanics: current approaches to material damage at different size and time scales, Theor. Appl. Fract. Mech. 41 (1–3) (2004) 173 P.V. Petroyiannis PV. Kermanidis AlTh. E. Kamoutsi E. Pantelakis SpG. Bontozoglou HV. and Haidemenopoulos GN. Evidence on the corrosioninduced hydrogen embrittlement of the 2024 aluminum alloy, Fatigue Fract. Eng. Mater. Struct., 28 (2005) 565574 Birnbaum HK. and Sofronis P. Hydrogenenhanced localized plasticitya mechanism for hydrogenrelated fracture, Mat. Sci. Eng. A 176 (1994) 191 Ruiz J. and Elices M. The role of environmental exposure in the fatigue behaviour of an aluminium alloy, Corros. Sci. 39 (12) (1997) 2117
366 [32] [33]
[34] [35]
[36]
[37]
[38]
Sp. G. Pantelakis and Al Th. Kermanidis Lin CK. and Yang ST.Corrosion fatigue behavior of 7050 aluminum alloys in different tempers, Eng. Fract. Mech. 59 (6) (1998) 779 Inman ME. Kelly RG. S.A. Willard SA. and Piascik RS. in: Proceedings of the FAANASA Symposium on the Continued Airworthiness of Aircraft Structures, Virginia, USA, (1997) 129 Zamber JE. and Hillberry BM. Probabilistic approach to predicting fatigue lives of corroded 2024T3, AIAA J. 37 (10) (1999) 1311. Bray GH. Bucci RJ. Colvin EL. and Kulak M. Effects of prior corrosion on the S/N fatigue performance of aluminium sheet alloys 2024T3 and 2524T3, in: W.A. Van der Sluys, R.S. Piascik, R. Zawierucha (Eds.), Effects of the Environment on the Initiation of Crack Growth, ASTM STP 1298, American Society for Testing and Materials, (1997) 89 Kermanidis AlTh. Petroyiannis PV. and Pantelakis SpG. Fatigue and damage tolerance behaviour of corroded 2024 T351 aircraft aluminum alloy, Theoretical and Applied Fracture Mechanics 43 (2005) 121–132 Chubb JP. Morad TA. Hockenhull BS. and Bristow JW. The effect of exfoliation corrosion on the fatigue behaviour of structural aluminium alloys, Structural Integrity of Ageing Airplanes, SpringerVerlag, Berlin, (1991) 87 ASTM G3490, Standard Test Method for Exfoliation Corrosion Susceptbility in 2xxx and 7xxx Series Aluminum Alloys, (EXCO Test), Annual Book of ASTM Standards, Metals –Test Methods and Analytical Procedures, Section 3, Vol. 03.02, Wear and Erosion; Metal Corrosion, (1995)
Author Index
Pantelakis SpG, 345 Peng D, 23 Pitt S, 23 RichterTrummer V, 85 Rodopoulos CA, 113 Sih GC, 181, 209, 249 Tang XS, 209, 249 Valsan M, 133 Walsh MJ, 47 Wang ZG, 275 Zhang GP, 275
Barter SA, 65 de Castro PMST, 85 Dini D, 47 Farahmand B, 1 Höppel HW, 327 Jones R, 23, 65 Kermanidis ATh, 345 Korsunsky AK, 47 Mannan SL, 133 Molent L, 65 Moreira PMGP, 85 Mughrabi H, 327
367
Subject Index
aluminum 17050T7451, 2014T6, 2024T3, 2219T87, 6061T62, 6061T6, 6082T6, 7010T73651, 7075T6, 7150T651, pure (super), bridge cablestayed, Runyang, suspension, cable construction, loosen/tighten, mechanical property, compact tension, compliance, corroded/uncorroded, crack corner, creepfatigue, density, initiation, intergranular, length,
long, surface, termination, transgranular crack growth block, fatigue, growth, nonsimilitude, rate, stable/unstable, crystallographic position, damage fatigue, dislocation density, surface bulk, ductile iron, elastic modulus, shear, Young’s, energy 2024T351, absorbed, released, total, extrusion, fatigue creep, damage map, low cycle,
369
370
Subject Index
small specimen, SNcurve, striation, thermal, ﬁlm, foil, frequency, fracture, mechanics, surface, weld, fracture thoughness, grain morphology, size, heterogeneity, interface, invariant form, loading, const. amlitude, indentor tip, sequence, symmetric effect, trafﬁc/notrafﬁc, macrocrack, macromechanical, magnesium AZ91, microcrack, microhardness, microstructural, nimonic PE106, nanochemical, nanotube, necking, nondestructive test, overload, oxidation, plane strain/stress, plastic zone, pore, region I, II, III, scale dual,
invariant, length, macro/micro shifting, size/time, triple, sigmoidal, slip, slope, steel 9Cr1Mo, 316L(SS), inconel, low carbon, SAE 52100, strain energy density factor, function, strain rate, stress intensity factor, applied, maximum, range, stress singularity, double, strong/weak, stress type amplitude, applied, max./min., mean, restraining, ultimate, yield, temperature elevated, time (hold), titanium ally Ti2.5Cu, Ti6Al4V, threshold (fatigue), transition, virtual testing, wave form,
Subject Index simple loading, trapezoidal, weld,
wire, Yintercept
371
Mechanics SOLID MECHANICS AND ITS APPLICATIONS Series Editor: G.M.L. Gladwell Aims and Scope of the Series The fundamental questions arising in mechanics are: Why?, How?, and How much? The aim of this series is to provide lucid accounts written by authoritative researchers giving vision and insight in answering these questions on the subject of mechanics as it relates to solids. The scope of the series covers the entire spectrum of solid mechanics. Thus it includes the foundation of mechanics; variational formulations; computational mechanics; statics, kinematics and dynamics of rigid and elastic bodies; vibrations of solids and structures; dynamical systems and chaos; the theories of elasticity, plasticity and viscoelasticity; composite materials; rods, beams, shells and membranes; structural control and stability; soils, rocks and geomechanics; fracture; tribology; experimental mechanics; biomechanics and machine design. 1. 2. 3. 4. 5. 6. 7. 8. 9. 10. 11. 12. 13. 14. 15. 16. 17. 18. 19. 20. 21. 22. 23.
R.T. Haftka, Z. G¨urdal and M.P. Kamat: Elements of Structural Optimization. 2nd rev.ed., 1990 ISBN 0792306082 J.J. Kalker: ThreeDimensional Elastic Bodies in Rolling Contact. 1990 ISBN 0792307127 P. Karasudhi: Foundations of Solid Mechanics. 1991 ISBN 0792307720 Not published Not published. J.F. Doyle: Static and Dynamic Analysis of Structures. With an Emphasis on Mechanics and Computer Matrix Methods. 1991 ISBN 0792311248; Pb 0792312082 O.O. Ochoa and J.N. Reddy: Finite Element Analysis of Composite Laminates. ISBN 0792311256 M.H. Aliabadi and D.P. Rooke: Numerical Fracture Mechanics. ISBN 0792311752 J. Angeles and C.S. L´opezCaj´un: Optimization of Cam Mechanisms. 1991 ISBN 0792313550 D.E. Grierson, A. Franchi and P. Riva (eds.): Progress in Structural Engineering. 1991 ISBN 0792313968 R.T. Haftka and Z. G¨urdal: Elements of Structural Optimization. 3rd rev. and exp. ed. 1992 ISBN 0792315049; Pb 0792315057 J.R. Barber: Elasticity. 1992 ISBN 0792316096; Pb 079231610X H.S. Tzou and G.L. Anderson (eds.): Intelligent Structural Systems. 1992 ISBN 0792319206 E.E. Gdoutos: Fracture Mechanics. An Introduction. 1993 ISBN 079231932X J.P. Ward: Solid Mechanics. An Introduction. 1992 ISBN 0792319494 M. Farshad: Design and Analysis of Shell Structures. 1992 ISBN 0792319508 H.S. Tzou and T. Fukuda (eds.): Precision Sensors, Actuators and Systems. 1992 ISBN 0792320158 J.R. Vinson: The Behavior of Shells Composed of Isotropic and Composite Materials. 1993 ISBN 0792321138 H.S. Tzou: Piezoelectric Shells. Distributed Sensing and Control of Continua. 1993 ISBN 0792321863 W. Schiehlen (ed.): Advanced Multibody System Dynamics. Simulation and Software Tools. 1993 ISBN 0792321928 C.W. Lee: Vibration Analysis of Rotors. 1993 ISBN 0792323009 D.R. Smith: An Introduction to Continuum Mechanics. 1993 ISBN 0792324544 G.M.L. Gladwell: Inverse Problems in Scattering. An Introduction. 1993 ISBN 0792324781
Mechanics SOLID MECHANICS AND ITS APPLICATIONS Series Editor: G.M.L. Gladwell 24. 25. 26. 27. 28. 29. 30. 31. 32.
33. 34. 35. 36. 37.
38. 39.
40. 41. 42. 43.
44. 45. 46.
47.
48.
G. Prathap: The Finite Element Method in Structural Mechanics. 1993 ISBN 0792324927 J. Herskovits (ed.): Advances in Structural Optimization. 1995 ISBN 0792325109 M.A. Gonz´alezPalacios and J. Angeles: Cam Synthesis. 1993 ISBN 0792325362 W.S. Hall: The Boundary Element Method. 1993 ISBN 079232580X J. Angeles, G. Hommel and P. Kov´acs (eds.): Computational Kinematics. 1993 ISBN 0792325850 A. Curnier: Computational Methods in Solid Mechanics. 1994 ISBN 0792327616 D.A. Hills and D. Nowell: Mechanics of Fretting Fatigue. 1994 ISBN 0792328663 B. Tabarrok and F.P.J. Rimrott: Variational Methods and Complementary Formulations in Dynamics. 1994 ISBN 0792329236 E.H. Dowell (ed.), E.F. Crawley, H.C. Curtiss Jr., D.A. Peters, R. H. Scanlan and F. Sisto: A Modern Course in Aeroelasticity. Third Revised and Enlarged Edition. 1995 ISBN 0792327888; Pb: 0792327896 A. Preumont: Random Vibration and Spectral Analysis. 1994 ISBN 0792330366 J.N. Reddy (ed.): Mechanics of Composite Materials. Selected works of Nicholas J. Pagano. 1994 ISBN 0792330412 A.P.S. Selvadurai (ed.): Mechanics of Poroelastic Media. 1996 ISBN 0792333292 Z. Mr´oz, D. Weichert, S. Dorosz (eds.): Inelastic Behaviour of Structures under Variable Loads. 1995 ISBN 0792333977 R. Pyrz (ed.): IUTAM Symposium on MicrostructureProperty Interactions in Composite Materials. Proceedings of the IUTAM Symposium held in Aalborg, Denmark. 1995 ISBN 0792334272 M.I. Friswell and J.E. Mottershead: Finite Element Model Updating in Structural Dynamics. 1995 ISBN 0792334310 D.F. Parker and A.H. England (eds.): IUTAM Symposium on Anisotropy, Inhomogeneity and Nonlinearity in Solid Mechanics. Proceedings of the IUTAM Symposium held in Nottingham, U.K. 1995 ISBN 0792335945 J.P. Merlet and B. Ravani (eds.): Computational Kinematics ’95. 1995 ISBN 0792336739 L.P. Lebedev, I.I. Vorovich and G.M.L. Gladwell: Functional Analysis. Applications in Mechanics and Inverse Problems. 1996 ISBN 0792338499 J. Menˇcik: Mechanics of Components with Treated or Coated Surfaces. 1996 ISBN 079233700X D. Bestle and W. Schiehlen (eds.): IUTAM Symposium on Optimization of Mechanical Systems. Proceedings of the IUTAM Symposium held in Stuttgart, Germany. 1996 ISBN 0792338308 D.A. Hills, P.A. Kelly, D.N. Dai and A.M. Korsunsky: Solution of Crack Problems. The Distributed Dislocation Technique. 1996 ISBN 0792338480 V.A. Squire, R.J. Hosking, A.D. Kerr and P.J. Langhorne: Moving Loads on Ice Plates. 1996 ISBN 0792339533 A. Pineau and A. Zaoui (eds.): IUTAM Symposium on Micromechanics of Plasticity and Damage of Multiphase Materials. Proceedings of the IUTAM Symposium held in S`evres, Paris, France. 1996 ISBN 0792341880 A. Naess and S. Krenk (eds.): IUTAM Symposium on Advances in Nonlinear Stochastic Mechanics. Proceedings of the IUTAM Symposium held in Trondheim, Norway. 1996 ISBN 0792341937 D. Ies¸an and A. Scalia: Thermoelastic Deformations. 1996 ISBN 0792342305
Mechanics SOLID MECHANICS AND ITS APPLICATIONS Series Editor: G.M.L. Gladwell 49. 50. 51. 52.
53.
54. 55. 56. 57. 58. 59. 60.
61. 62.
63.
64. 65. 66.
67. 68.
J.R. Willis (ed.): IUTAM Symposium on Nonlinear Analysis of Fracture. Proceedings of the IUTAM Symposium held in Cambridge, U.K. 1997 ISBN 0792343786 A. Preumont: Vibration Control of Active Structures. An Introduction. 1997 ISBN 0792343921 G.P. Cherepanov: Methods of Fracture Mechanics: Solid Matter Physics. 1997 ISBN 0792344081 D.H. van Campen (ed.): IUTAM Symposium on Interaction between Dynamics and Control in Advanced Mechanical Systems. Proceedings of the IUTAM Symposium held in Eindhoven, The Netherlands. 1997 ISBN 0792344294 N.A. Fleck and A.C.F. Cocks (eds.): IUTAM Symposium on Mechanics of Granular and Porous Materials. Proceedings of the IUTAM Symposium held in Cambridge, U.K. 1997 ISBN 0792345533 J. Roorda and N.K. Srivastava (eds.): Trends in Structural Mechanics. Theory, Practice, Education. 1997 ISBN 0792346033 Yu.A. Mitropolskii and N. Van Dao: Applied Asymptotic Methods in Nonlinear Oscillations. 1997 ISBN 079234605X C. Guedes Soares (ed.): Probabilistic Methods for Structural Design. 1997 ISBN 079234670X D. Franc¸ois, A. Pineau and A. Zaoui: Mechanical Behaviour of Materials. Volume I: Elasticity and Plasticity. 1998 ISBN 079234894X D. Franc¸ois, A. Pineau and A. Zaoui: Mechanical Behaviour of Materials. Volume II: Viscoplasticity, Damage, Fracture and Contact Mechanics. 1998 ISBN 0792348958 L.T. Tenek and J. Argyris: Finite Element Analysis for Composite Structures. 1998 ISBN 0792348990 Y.A. BaheiElDin and G.J. Dvorak (eds.): IUTAM Symposium on Transformation Problems in Composite and Active Materials. Proceedings of the IUTAM Symposium held in Cairo, Egypt. 1998 ISBN 0792351223 I.G. Goryacheva: Contact Mechanics in Tribology. 1998 ISBN 0792352572 O.T. Bruhns and E. Stein (eds.): IUTAM Symposium on Micro and Macrostructural Aspects of Thermoplasticity. Proceedings of the IUTAM Symposium held in Bochum, Germany. 1999 ISBN 0792352653 F.C. Moon: IUTAM Symposium on New Applications of Nonlinear and Chaotic Dynamics in Mechanics. Proceedings of the IUTAM Symposium held in Ithaca, NY, USA. 1998 ISBN 0792352769 R. Wang: IUTAM Symposium on Rheology of Bodies with Defects. Proceedings of the IUTAM Symposium held in Beijing, China. 1999 ISBN 0792352971 Yu.I. Dimitrienko: Thermomechanics of Composites under High Temperatures. 1999 ISBN 0792348990 P. Argoul, M. Fr´emond and Q.S. Nguyen (eds.): IUTAM Symposium on Variations of Domains and FreeBoundary Problems in Solid Mechanics. Proceedings of the IUTAM Symposium held in Paris, France. 1999 ISBN 0792354508 F.J. Fahy and W.G. Price (eds.): IUTAM Symposium on Statistical Energy Analysis. Proceedings of the IUTAM Symposium held in Southampton, U.K. 1999 ISBN 0792354575 H.A. Mang and F.G. Rammerstorfer (eds.): IUTAM Symposium on Discretization Methods in Structural Mechanics. Proceedings of the IUTAM Symposium held in Vienna, Austria. 1999 ISBN 0792355911
Mechanics SOLID MECHANICS AND ITS APPLICATIONS Series Editor: G.M.L. Gladwell 69.
70. 71. 72. 73.
74. 75. 76. 77. 78. 79. 80.
81.
82.
83. 84. 85.
86. 87.
88. 89.
P. Pedersen and M.P. Bendsøe (eds.): IUTAM Symposium on Synthesis in Bio Solid Mechanics. Proceedings of the IUTAM Symposium held in Copenhagen, Denmark. 1999 ISBN 0792356152 S.K. Agrawal and B.C. Fabien: Optimization of Dynamic Systems. 1999 ISBN 0792356810 A. Carpinteri: Nonlinear Crack Models for Nonmetallic Materials. 1999 ISBN 0792357507 F. Pfeifer (ed.): IUTAM Symposium on Unilateral Multibody Contacts. Proceedings of the IUTAM Symposium held in Munich, Germany. 1999 ISBN 0792360303 E. Lavendelis and M. Zakrzhevsky (eds.): IUTAM/IFToMM Symposium on Synthesis of Nonlinear Dynamical Systems. Proceedings of the IUTAM/IFToMM Symposium held in Riga, Latvia. 2000 ISBN 0792361067 J.P. Merlet: Parallel Robots. 2000 ISBN 0792363086 J.T. Pindera: Techniques of Tomographic Isodyne Stress Analysis. 2000 ISBN 0792363884 G.A. Maugin, R. Drouot and F. Sidoroff (eds.): Continuum Thermomechanics. The Art and Science of Modelling Material Behaviour. 2000 ISBN 0792364074 N. Van Dao and E.J. Kreuzer (eds.): IUTAM Symposium on Recent Developments in Nonlinear Oscillations of Mechanical Systems. 2000 ISBN 0792364708 S.D. Akbarov and A.N. Guz: Mechanics of Curved Composites. 2000 ISBN 0792364775 M.B. Rubin: Cosserat Theories: Shells, Rods and Points. 2000 ISBN 0792364899 S. Pellegrino and S.D. Guest (eds.): IUTAMIASS Symposium on Deployable Structures: Theory and Applications. Proceedings of the IUTAMIASS Symposium held in Cambridge, U.K., 6–9 September 1998. 2000 ISBN 079236516X A.D. Rosato and D.L. Blackmore (eds.): IUTAM Symposium on Segregation in Granular Flows. Proceedings of the IUTAM Symposium held in Cape May, NJ, U.S.A., June 5–10, 1999. 2000 ISBN 079236547X A. Lagarde (ed.): IUTAM Symposium on Advanced Optical Methods and Applications in Solid Mechanics. Proceedings of the IUTAM Symposium held in Futuroscope, Poitiers, France, August 31–September 4, 1998. 2000 ISBN 0792366042 D. Weichert and G. Maier (eds.): Inelastic Analysis of Structures under Variable Loads. Theory and Engineering Applications. 2000 ISBN 079236645X T.J. Chuang and J.W. Rudnicki (eds.): Multiscale Deformation and Fracture in Materials and Structures. The James R. Rice 60th Anniversary Volume. 2001 ISBN 0792367189 S. Narayanan and R.N. Iyengar (eds.): IUTAM Symposium on Nonlinearity and Stochastic Structural Dynamics. Proceedings of the IUTAM Symposium held in Madras, Chennai, India, 4–8 January 1999 ISBN 0792367332 S. Murakami and N. Ohno (eds.): IUTAM Symposium on Creep in Structures. Proceedings of the IUTAM Symposium held in Nagoya, Japan, 37 April 2000. 2001 ISBN 0792367375 W. Ehlers (ed.): IUTAM Symposium on Theoretical and Numerical Methods in Continuum Mechanics of Porous Materials. Proceedings of the IUTAM Symposium held at the University of Stuttgart, Germany, September 510, 1999. 2001 ISBN 0792367669 D. Durban, D. Givoli and J.G. Simmonds (eds.): Advances in the Mechanis of Plates and Shells The Avinoam Libai Anniversary Volume. 2001 ISBN 0792367855 U. Gabbert and H.S. Tzou (eds.): IUTAM Symposium on Smart Structures and Structonic Systems. Proceedings of the IUTAM Symposium held in Magdeburg, Germany, 26–29 September 2000. 2001 ISBN 0792369688
Mechanics SOLID MECHANICS AND ITS APPLICATIONS Series Editor: G.M.L. Gladwell 90. 91.
92.
93. 94.
95. 96. 97.
98. 99. 100.
101.
102. 103.
104. 105. 106. 107. 108.
Y. Ivanov, V. Cheshkov and M. Natova: Polymer Composite Materials – Interface Phenomena & Processes. 2001 ISBN 0792370082 R.C. McPhedran, L.C. Botten and N.A. Nicorovici (eds.): IUTAM Symposium on Mechanical and Electromagnetic Waves in Structured Media. Proceedings of the IUTAM Symposium held in Sydney, NSW, Australia, 1822 Januari 1999. 2001 ISBN 0792370384 D.A. Sotiropoulos (ed.): IUTAM Symposium on Mechanical Waves for Composite Structures Characterization. Proceedings of the IUTAM Symposium held in Chania, Crete, Greece, June 1417, 2000. 2001 ISBN 079237164X V.M. Alexandrov and D.A. Pozharskii: ThreeDimensional Contact Problems. 2001 ISBN 0792371658 J.P. Dempsey and H.H. Shen (eds.): IUTAM Symposium on Scaling Laws in Ice Mechanics and Ice Dynamics. Proceedings of the IUTAM Symposium held in Fairbanks, Alaska, U.S.A., 1316 June 2000. 2001 ISBN 1402001711 U. Kirsch: DesignOriented Analysis of Structures. A Uniﬁed Approach. 2002 ISBN 1402004435 A. Preumont: Vibration Control of Active Structures. An Introduction (2nd Edition). 2002 ISBN 1402004966 B.L. Karihaloo (ed.): IUTAM Symposium on Analytical and Computational Fracture Mechanics of NonHomogeneous Materials. Proceedings of the IUTAM Symposium held in Cardiff, U.K., 1822 June 2001. 2002 ISBN 1402005105 S.M. Han and H. Benaroya: Nonlinear and Stochastic Dynamics of Compliant Offshore Structures. 2002 ISBN 1402005733 A.M. Linkov: Boundary Integral Equations in Elasticity Theory. 2002 ISBN 1402005741 L.P. Lebedev, I.I. Vorovich and G.M.L. Gladwell: Functional Analysis. Applications in Mechanics and Inverse Problems (2nd Edition). 2002 ISBN 1402006675; Pb: 1402007566 Q.P. Sun (ed.): IUTAM Symposium on Mechanics of Martensitic Phase Transformation in Solids. Proceedings of the IUTAM Symposium held in Hong Kong, China, 1115 June 2001. 2002 ISBN 1402007418 M.L. Munjal (ed.): IUTAM Symposium on Designing for Quietness. Proceedings of the IUTAM Symposium held in Bangkok, India, 1214 December 2000. 2002 ISBN 1402007655 J.A.C. Martins and M.D.P. Monteiro Marques (eds.): Contact Mechanics. Proceedings of the 3rd Contact Mechanics International Symposium, Praia da Consolac¸a˜ o, Peniche, Portugal, 1721 June 2001. 2002 ISBN 1402008112 H.R. Drew and S. Pellegrino (eds.): New Approaches to Structural Mechanics, Shells and Biological Structures. 2002 ISBN 1402008627 J.R. Vinson and R.L. Sierakowski: The Behavior of Structures Composed of Composite Materials. Second Edition. 2002 ISBN 1402009046 Not yet published. J.R. Barber: Elasticity. Second Edition. 2002 ISBN Hb 140200964X; Pb 1402009666 C. Miehe (ed.): IUTAM Symposium on Computational Mechanics of Solid Materials at Large Strains. Proceedings of the IUTAM Symposium held in Stuttgart, Germany, 2024 August 2001. 2003 ISBN 1402011709
Mechanics SOLID MECHANICS AND ITS APPLICATIONS Series Editor: G.M.L. Gladwell 109. P. St˚ahle and K.G. Sundin (eds.): IUTAM Symposium on Field Analyses for Determination of Material Parameters – Experimental and Numerical Aspects. Proceedings of the IUTAM Symposium held in Abisko National Park, Kiruna, Sweden, July 31 – August 4, 2000. 2003 ISBN 1402012837 110. N. Sri Namachchivaya and Y.K. Lin (eds.): IUTAM Symposium on Nonlnear Stochastic Dynamics. Proceedings of the IUTAM Symposium held in Monticello, IL, USA, 26 – 30 August, 2000. 2003 ISBN 1402014716 111. H. Sobieckzky (ed.): IUTAM Symposium Transsonicum IV. Proceedings of the IUTAM Symposium held in G¨ottingen, Germany, 2–6 September 2002, 2003 ISBN 1402016085 112. J.C. Samin and P. Fisette: Symbolic Modeling of Multibody Systems. 2003 ISBN 1402016298 113. A.B. Movchan (ed.): IUTAM Symposium on Asymptotics, Singularities and Homogenisation in Problems of Mechanics. Proceedings of the IUTAM Symposium held in Liverpool, United Kingdom, 811 July 2002. 2003 ISBN 1402017804 114. S. Ahzi, M. Cherkaoui, M.A. Khaleel, H.M. Zbib, M.A. Zikry and B. LaMatina (eds.): IUTAM Symposium on Multiscale Modeling and Characterization of ElasticInelastic Behavior of Engineering Materials. Proceedings of the IUTAM Symposium held in Marrakech, Morocco, 2025 October 2002. 2004 ISBN 1402018614 115. H. Kitagawa and Y. Shibutani (eds.): IUTAM Symposium on Mesoscopic Dynamics of Fracture Process and Materials Strength. Proceedings of the IUTAM Symposium held in Osaka, Japan, 611 July 2003. Volume in celebration of Professor Kitagawa’s retirement. 2004 ISBN 1402020376 116. E.H. Dowell, R.L. Clark, D. Cox, H.C. Curtiss, Jr., K.C. Hall, D.A. Peters, R.H. Scanlan, E. Simiu, F. Sisto and D. Tang: A Modern Course in Aeroelasticity. 4th Edition, 2004 ISBN 1402020392 117. T. Burczy´nski and A. Osyczka (eds.): IUTAM Symposium on Evolutionary Methods in Mechanics. Proceedings of the IUTAM Symposium held in Cracow, Poland, 2427 September 2002. 2004 ISBN 1402022662 118. D. Ies¸an: Thermoelastic Models of Continua. 2004 ISBN 140202309X 119. G.M.L. Gladwell: Inverse Problems in Vibration. Second Edition 2004 ISBN 1402026706 120. J.R. Vinson: Plate and Panel Structures of Isotropic, Composite and Piezoelectric Materials, Including Sandwich Construction. 2005 ISBN 1402031106 121. Forthcoming. 122. G. Rega and F. Vestroni (eds.): IUTAM Symposium on Chaotic Dynamics and Control of Systems and Processes in Mechanics. Proceedings of the IUTAM Symposium held in Rome, Italy, 8–13 June 2003. 2005 ISBN 1402032676 123. E.E. Gdoutos: Fracture Mechanics. An Introduction. 2nd edition. 2005 ISBN 1402028632 124. M.D. Gilchrist (ed.): IUTAM Symposium on Impact Biomechanics from Fundamental Insights to Applications. 2005 ISBN 1402037953 125. J.M. Huyghe, P.A.C. Raats and S.C. Cowin (eds.): IUTAM Symposium on Physicochemical and Electromechanical Interactions in Porous Media. 2005 ISBN 140203864X 126. H. Ding, W. Chen and L. Zhang: Elasticity of Transversely Isotropic Materials. 2005 ISBN 1402040334 127. W. Yang (ed.): IUTAM Symposium on Mechanics and Reliability of Actuating Materials. Proceedings of the IUTAM Symposium held in Beijing, China, 1–3 September 2004. 2005 ISBN 1402041316
Mechanics SOLID MECHANICS AND ITS APPLICATIONS Series Editor: G.M.L. Gladwell 128. J.P. Merlet: Parallel Robots. 2006 ISBN 1402041322 129. G.E.A. Meier and K.R. Sreenivasan (eds.): IUTAM Symposium on One Hundred Years of Boundary Layer Research. Proceedings of the IUTAM Symposium held at DLRG¨ottingen, Germany, August 12–14, 2004. 2006 ISBN 1402041497 130. H. Ulbrich and W. G¨unthner (eds.): IUTAM Symposium on Vibration Control of Nonlinear Mechanisms and Structures. 2006 ISBN 1402041608 131. L. Librescu and O. Song: ThinWalled Composite Beams. Theory and Application. 2006 ISBN 1402034571 132. G. BenDor, A. Dubinsky and T. Elperin: Applied HighSpeed Plate Penetration Dynamics. 2006 ISBN 1402034520 133. X. Markenscoff and A. Gupta (eds.): Collected Works of J. D. Eshelby. Mechanics of Defects and Inhomogeneities. 2006 ISBN 140204416X 134. R.W. Snidle and H.P. Evans (eds.): IUTAM Symposium on Elastohydrodynamics and Microelastohydrodynamics. Proceedings of the IUTAM Symposium held in Cardiff, UK, 1–3 September, 2004. 2006 ISBN 1402045328 135. T. Sadowski (ed.): IUTAM Symposium on Multiscale Modelling of Damage and Fracture Processes in Composite Materials. Proceedings of the IUTAM Symposium held in Kazimierz Dolny, Poland, 23–27 May 2005. 2006 ISBN 1402045654 136. A. Preumont: Mechatronics. Dynamics of Electromechanical and Piezoelectric Systems. 2006 ISBN 1402046952 137. M.P. Bendsøe, N. Olhoff and O. Sigmund (eds.): IUTAM Symposium on Topological Design Optimization of Structures, Machines and Materials. Status and Perspectives. 2006 ISBN 1402047290 138. A. Klarbring: Models of Mechanics. 2006 ISBN 1402048343 139. H.D. Bui: Fracture Mechanics. Inverse Problems and Solutions. 2006 ISBN 140204836X 140. M. Pandey, W.C. Xie and L. Xu (eds.): Advances in Engineering Structures, Mechanics and Construction. Proceedings of an International Conference on Advances in Engineering Structures, Mechanics & Construction, held in Waterloo, Ontario, Canada, May 14–17, 2006. 2006 ISBN 1402048904 141. G.Q. Zhang, W.D. van Driel and X. J. Fan: Mechanics of Microelectronics. 2006 ISBN 140204934X 142. Q.P. Sun and P. Tong (eds.): IUTAM Symposium on Size Effects on Material and Structural Behavior at Micron and NanoScales. Proceedings of the IUTAM Symposium held in Hong Kong, China, 31 May–4 June, 2004. 2006 ISBN 1402049455 143. A.P. Mouritz and A.G. Gibson: Fire Properties of Polymer Composite Materials. 2006 ISBN 140205355X 144. Y.L. Bai, Q.S. Zheng and Y.G. Wei (eds.): IUTAM Symposium on Mechanical Behavior and MicroMechanics of Nanostructured Materials. Proceedings of the IUTAM Symposium held in Beijing, China, 27–30 June 2005. 2007 ISBN 1402056230 145. L.P. Pook: Metal Fatigue. What It Is, Why It Matters. 2007 ISBN 1402055966 146. H.I. Ling, L. Callisto, D. Leshchinsky and J. Koseki (eds.): Soil StressStrain Behavior: Measurement, Modeling and Analysis. A Collection of Papers of the Geotechnical Symposium in Rome, March 16–17, 2006. 2007 ISBN 9781402061455 147. A.S. Kravchuk and P.J. Neittaanm¨aki: Variational and QuasiVariational Inequalities in Mechanics. 2007 ISBN 9781402063763
Mechanics SOLID MECHANICS AND ITS APPLICATIONS Series Editor: G.M.L. Gladwell 148. S.K. Kanaun and V. Levin: SelfConsistent Methods for Composites. Vol. 1: Static Problems. 2008 ISBN 9781402066634 149. G. Gogu: Structural Synthesis of Parallel Robots. Part 1: Methodology. 2008 ISBN 9781402051029 150. S.K. Kanaun and V. Levin: SelfConsistent Methods for Composites. Vol. 2: Wave Propagation in Heterogeneous Materials. 2008 ISBN 9781402069673 151. U. Kirsch: Reanalysis of Structures. A Uniﬁed Approach for Linear, Nonlinear, Static and Dynamic Systems. 2008 ISBN 9781402081972 152. G.C. Sih (ed.): Multiscale Fatigue Crack Initiation and Propagation of Engineering Materials: Structural Integrity and Microstructural Worthiness. Fatigue Crack Growth Behaviour of Small and Large Bodies. 2008 ISBN 9781402085192
springer.com